TITLES OF RELATED INTEREST
Analytical and computational methods in engineering rock mechanics
Boundary element methods in elastodynamics
G.D.Manolis & D.E.Beskos
Boundary element methods in solid mechanics
S.L.Crouch & A.M.Starfield
Computers in construction planning and control
A concise introduction to engineering economics
H.R.Neave & P.B.Worthington
Earth structures engineering
The finite element method in thermomechanics
Hemispherical projection methods in rock mechanics
P.Novak et al.
Hydraulics in civil engineering
A.Chadwick & J.Morfett
Numerical methods in engineering and science
Planning and design of engineering systems
R.Warner & G.Dandy
P.Zeman & H.M.Irvine
Rock mechanics for underground mining
B.H.G.Brady & E.T.Brown
DESIGN OF PRESTRESSED CONCRETE
R.I.Gilbert & N.C.Mickleborough
School of Civil Engineering
The University of New South Wales, Sydney, Australia
LONDON AND NEW YORK
The design of structures in general, and prestressed concrete structures in particular, requires
considerably more information than is contained in building codes. A sound understanding of
structural behaviour at all stages of loading is essential. The aim of this book is to present a
detailed description and explanation of the behaviour of prestressed concrete members and
structures both at service loads and at ultimate loads and, in doing so, provide a
comprehensive guide to design. The design criteria and procedures contained in several major
building codes, including ACI 318–83, BS 8110:1985, and AS 3600–1988, are also presented.
Each aspect of the analysis and design of fully prestressed and partially prestressed
concrete members is approached from first principles and illustrated by numerous worked
examples. The text is written for senior undergraduate and postgraduate students of civil and
structural engineering, and also for practising structural engineers.
The book began as notes for a series of lectures to structural engineers in a short course on
prestressed concrete design conducted in Sydney in 1985 and has been further developed over
the past 5 years as part of the authors’ involvement in research and the teaching of prestressed
concrete to graduate students at the University of New South Wales. The work has also
gained much from the membership of Professor Gilbert on committees of the Standards
Association of Australia and his involvement in the development of the Australian Standard
for Concrete Structures, AS 3600–1988.
The scope of the work ranges from an introduction to the fundamentals of prestressed
concrete to in-depth treatments of more advanced topics. Chapter 1 introduces the basic
concepts of prestressed concrete and the limit states design philosophies used in North
American, British, European, and Australian practice. Material properties relevant to design
are discussed in Chapter 2. A comprehensive treatment of the design of prestressed concrete
beams for serviceability is presented in Chapter 3. The instantaneous and time-dependent
behaviour of cross-sections under service loads are discussed in considerable detail. Both
uncracked and cracked cross-sections are considered. Techniques for determining the section
size, the magnitude and eccentricity of prestress, the losses of prestress and the deflection of
members are outlined. Each aspect of design is illustrated by numerical examples.
Chapters 4 and 5 deal with the design of members for strength in bending, shear, and
torsion, and Chapter 6 covers the design of the anchorage zones
in both pretensioned and post-tensioned members. A guide to the design of composite
prestressed concrete beams is provided in Chapter 7, and includes a detailed worked example
of the analysis of a composite trough girder footbridge. Chapter 8 discusses design procedures
for statically determinate beams. Comprehensive self-contained design examples are provided
for fully prestressed and partially prestressed, post-tensioned, and pretensioned concrete
The analysis and design of statically indeterminate beams and frames is covered in Chapter
9, and provides guidance on the treatment of secondary effects at all stages of loading.
Chapters 10 and 11 provide a detailed discussion of the analysis and design of two-way slab
systems. Chapter 10 is concerned with the behaviour and strength of slabs, whilst Chapter 11
deals with serviceability. Complete design examples are provided for panels of an edge-
supported slab and a flat slab. The behaviour of axially loaded members is dealt with in
Chapter 12. Compression members, members subjected to combined bending and
compression, and prestressed concrete tension members are discussed and design aspects are
illustrated by examples.
A special feature of the book is the treatment of serviceability aspects of design. Concrete
structures are prestressed to improve behaviour at service loads and thereby increase the
economical range of concrete as a construction material. In conventional prestressed
structures, the level of prestress and the position of the tendons are usually based on
considerations of serviceability. Practical methods for accounting for the non-linear and time-
dependent effects of cracking, creep, shrinkage, and relaxation are presented in a clear and
The authors hope that Design of Prestressed Concrete will be a valuable source of
information and a useful guide to design.
R.I.Gilbert & N.C.Mickleborough
1 Basic concepts 1
1.1 Introduction 1
1.2 Methods of prestressing 2
1.3 Introductory example 4
1.4 Transverse forces caused by draped tendons 6
1.5 Calculation of elastic stresses 9
1.6 Flexural behaviour—from initial to ultimate loads 15
1.7 Design procedures 17
1.8 References 28
2 Design properties of materials 29
2.1 Introduction 29
2.2 Composition of concrete 30
2.3 Strength of concrete 30
2.4 Deformation of concrete 34
2.5 Predictions of the creep coefficient and shrinkage 42
2.6 Thermal expansion 47
2.7 Steel used for prestressing 48
2.8 Steel relaxation 52
2.9 Non-prestressed reinforcement 54
2.10 References 58
3 Design for serviceability 60
3.1 Introduction 60
3.2 Stress limits 61
3.3 Determination of prestress and eccentricity in flexural members 64
3.4 Cable profiles 75
3.5 Short-term analysis of cross-sections 77
3.6 Time-dependent analysis of cross-sections 89
3.7 Losses of prestress 102
3.8 Deflection calculations 108
3.9 References 120
4 Ultimate flexural strength 121
4.1 Introduction 121
4.2 Flexural behaviour at overloads 122
4.3 Flexural strength theory 124
4.4 Approximate code-oriented procedures 140
4.5 Design calculations 147
4.6 Flanged sections 153
4.7 References 159
5 Design for shear and torsional strength 160
5.1 Introduction 160
SHEAR IN BEAMS
5.2 Inclined cracking 161
5.3 Effect of prestress 162
5.4 Web reinforcement 163
5.5 Shear strength 165
TORSION IN BEAMS
5.6 Compatibility torsion and equilibrium torsion 182
5.7 Effects of torsion 183
5.8 Design provisions for torsion in AS 3600–1988 185
SHEAR IN SLABS AND FOOTINGS
5.9 Punching shear 195
5.10 Design procedures for punching shear in AS 3600–1988 198
5.11 References 208
6 Anchorage zones 209
6.1 Introduction 209
6.2 Pretensioned concrete—force transfer by bond 210
6.3 Post-tensioned concrete anchorage zones 214
6.4 References 238
7 Composite members 240
7.1 Types and advantages of composite construction 240
7.2 Behaviour of composite members 242
7.3 Stages of loading 243
7.4 Determination of prestress 246
7.5 Methods of analysis at service loads 249
7.6 Ultimate flexural strength 265
7.7 Horizontal shear transfer 265
7.8 Ultimate shear strength 275
7.9 References 280
8 Design procedures for determinate beams 281
8.1 Introduction 281
8.2 Types of section 281
8.3 Initial trial section 283
8.4 Design procedures—fully prestressed beams 286
8.5 Design procedures—partially prestressed beams 312
9 Statically indeterminate members 319
9.1 Introduction 319
9.2 Tendon profiles 321
9.3 Continuous beams 323
9.4 Staticaily indeterminate frames 350
9.5 Design of continuous beams 354
9.6 References 375
10 Two-way slabs—behaviour and design 376
10.1 Introduction 376
10.2 Effects of prestress 378
10.3 Design approach—general 381
10.4 One-way slabs 382
10.5 Two-way edge-supported slabs 382
10.6 Flat plate slabs 394
10.7 Flat slabs with drop panels 415
10.8 Band-beam and slab systems 416
10.9 References 417
11 Two-way slabs—serviceability 418
11.1 Introduction 418
11.2 The balanced load stage 419
11.3 Initial sizing of slabs 421
11.4 A review of simplified slab deflection models 429
11.5 Cracking in prestressed slabs 438
11.6 Long-term deflections 442
11.7 Worked examples 443
11.8 References 452
12 Compression and tension members 454
12.1 Types of compression members 454
12.2 Classification and behaviour of compression members 455
12.3 Cross-sectional analysis—compression and bending 457
12.4 Slenderness effects 471
12.5 Reinforcement requirements in compression members 481
12.6 Tension members 483
12.7 References 489
Appendix I Alternative models for creep and shrinkage 490
A.1 Introduction 490
A.2 The ACI Committee 209 Method (1978) 490
A.3 The CEB–FIP Method (1978) 493
A.4 References 497
All symbols are defined in the text where they first appear. The more frequently used symbols
and those that appear throughout the book are listed below. Tension is taken to be positive and
compression is negative, throughout. Positive bending about a horizontal axis causes tension
in the bottom fibres of a cross-section.
Ac area of concrete
Ag area of gross cross-section
Amin minimum required area of a cross-section
Apc area of the precast element of a composite cross-section
Apt area of prestressed steel in the tensile zone
As, Ap areas of the non-prestressed and prestressed steel, respectively
Asi, Api areas of non-prestressed and prestressed steel at the ith steel level, respectively
Asb, A ss area of the transverse non-prestressed reinforcement required for bursting and spalling,
respectively, in an anchorage zone (Eqns 6.11 and 6.12)
Ast, Asc areas of the non-prestressed tensile and compressive reinforcement, respectively
Asυ area of shear reinforcement at each stirrup location
Asw area of bar used for closed torsional stirrup
(A s)min minimum area of non-prestressed reinforcement
A' area of concrete under idealized rectangular compressive stress block
A1 bearing area
A2 largest area of the concrete surface geometrically similar to A1
a width of the torsion strip
B first moment of area of the transformed cross-section about the top fibre
property B of the concrete part of the cross-section and of the age-adjusted transformed
b width of the compressive zone of the cross-section of a beam or slab
b ef effective width of the flange of a flanged cross-section
bf width of the contact surface between the precast and in situ parts of a composite cross-section
bo width of an opening adjacent to the critical shear perimeter (Fig. 5.12)
b tr width of the transformed flange of a composite cross-section (Eqn 7.1)
bυ effective width of the web for shear calculations (bw –0.5d d)
bw width of the web of a flanged cross-section
C resultant compressive force carry over factor
Cb transverse compressive force behind an anchorage plate caused by bursting
Cc compressive force carried by the concrete
Cm factor to account for the effect of the magnitude and direction of end moments on the moment
magnification factor for a slender column
Cs compressive force in the non-prestressed steel
c1 , c2 side dimensions of a column
D overall depth of a cross-section
Db overall depth of the beam in a beam and slab system
De depth of the symmetrical prism within an anchorage zone
Dmin minimum overall depth
Ds depth of a slab
d effective depth from the extreme compressive fibre to the resultant tensile force at the ultimate
strength in bending
db bar diameter
dc depth to the top layer of non-prestressed steel
dd diameter of a prestressing duct
dn depth from the extreme compressive fibre to the neutral axis
do depth to the bottom layer of tensile reinforcement
d s, dp depths to the non-prestressed and prestressed steel, respectively
d si, dpi depths to the ith level of non-prestressed and prestressed steel, respectively
dz depth to the compressive force in the concrete
Ec, Es, elastic moduli of concrete, non-prestressed steel, and prestressed steel, respectively
Eci initial elastic modulus of concrete
Ec,28 static elastic modulus at 28 days (Eqn 2.17)
Ec1 , Ec2 elastic moduli of concrete in precast and in situ elements, respectively, of a composite cross-
Ee, Ē effective modulus of concrete (Eqn 2.12) and age-adjusted effective modulus of concrete (Eqn
e eccentricity of prestress eccentricity of load in a compression member
e base of the natural logarithm
e* eccentricity of the pressure line from the centroidal axis
emax maximum possible eccentricity of prestress
emin minimum acceptable eccentricity of prestress
eo initial eccentricity of load in a slender column
epc eccentricity of prestress measured from the centroidal axis of the precast part of a
functions of x (Eqn 9.4)
Fb design strength of concrete in bearing
Fc, Fci compressive stress limits for concrete under full load and immediately after transfer,
Fep force caused by earth pressure
Feq force caused by earthquake
Flp force caused by liquid pressure
Fs force caused by snow loads
Ft, Fti tensile stress limits for concrete under full load and immediately after transfer,
absolute value of the design force in the compressive zone due to bending
fB flexibility coefficient associated with a release at point B
fc (t) mean compressive strength of concrete at time t
fc υ permissible concrete shear stress on the critical shear perimeter
characteristic compressive strength of concrete at 28 days
characteristic compressive strength of concrete at time t
characteristic compressive strength of concrete at transfer
fcu cube strength of concrete
fp ultimate strength of the prestressing steel
fpy 0.2% proof stress for prestressing steel
flexural tensile strength of concrete (Eqn 2.3)
direct tensile strength of concrete (Eqn 2.4)
fy yield stress of non-prestressed steel
G dead load
g dead load per unit area
h dimension of anchorage plate
drape of tendon
h x, hy drape of the tendons running in the x and y directions, respectively
I second moment of area (moment of inertia) about centroidal axis
Iaυ average second moment of area after cracking
Ic1 , Ic2 second moments of area of precast and in situ elements on a composite cross-section
Icr second moment of area of a cracked cross-section
Ie effective second moment of area after cracking
Ig second moment of area of the gross cross-section
Ī second moment of area of the transformed section about the top fibre of the section
Ī Ī property Ī the concrete part of the cross-section and of the age-adjusted transformed section,
c, e of
i, j, k integers
Jt torsional constant
klu effective length of a column
kAB stiffness coefficient for member AB
ku ratio of the depth to the neutral axis to the effective depth at the ultimate bending moment
k1 , k2 factors used for the determination of stress in the prestressing steel at ultimate (Eqn 4.18)
k1 , k2 , material multiplication constants
K slab system factor
La length of anchorage zone measured from the loaded face (Fig. 6.3b)
Lb , L c length of a beam and a column, respectively
Ldi length of tendon associated with draw-in losses (Eqn 3.61)
Le effective span, i.e. the lesser of the centre to centre distance between the supports and the clear
span plus depth (Ln +D)
Lo distance between points of zero bending moment in a beam
Ln clear span
Lpa distance along a tendon from the jack
Lt transverse span
Lx , Ly shorter and longer orthogonal span lengths, respectively, in two-way slabs
l internal level arm
lb , l s lever arms associated with bursting and spalling moment, respectively
lc , ls lever arm distance of compressive forces in the concrete and in the steel, respectively, above
the non-prestressed tensile steel (Fig. 4.6)
ld development length for a pretensioned tendon (Eqn 6.2)
lt transmission length for a pretensioned tendon (Eqn 6.2)
additional length required to develop (σ − pe ) in a pretensioned tendon (Eqn 6.2)
lu unsupported length of a column
ln natural logarithm
M bending moment
virtual bending moment
Mb bursting moment
moment transferred to front face of a column
M cr cracking moment
M fixed-end moment
M G, MQ moment caused by the dead and live loads, respectively
Mi initial moment about top fibre of the transformed cross-section
Mo moment at a cross-section at transfer total static moment in a two-way flat slab
M pt, Mps total and secondary moments due to prestress in a continuous member
Ms spalling moment
moment transferred to side face of a column
M sus moment caused by the sustained loads
M sw moment caused by self-weight
MT moment caused by total service loads
Mu ultimate flexural strength
M ub unbalanced moment
M* factored design moment for the strength limit state
magnified design moment
design moment transferred to a column through the critical shear perimeter
ultimate moment of resistance per unit length along a positive and a negative yield line,
N axial force
virtual axial force
Nc critical buckling load
N cr tensile axial force at cracking
Ni initial axial force on the transformed cross-section
Nu ultimate axial strength
N ub ultimate axial force at the balanced failure point
N* factored design axial force for the strength limit state
N increments of axial force and moment about the top fibre of the cross-section, respectively
N, M restraining actions which develop during a time interval due to restrained creep, shrinkage
and relaxation (Eqns 3.41–3.48)
n, n s modular ratio for non-prestressed steel (Es/Ec)
n, n p modular ratio for prestressed steel (Ep /Ec)
age-adjusted modular ratio (Es/Ē or Ep/Ē)
nc modular ratio for the in situ concrete on a composite cross-section (Ec2/Ec1 )
P prestressing force
Pe effective prestressing force after time-dependent losses
Pi prestressing force immediately after transfer
Pj prestressing force at the jack before transfer
Pυ vertical component of prestress
Q live load
first moment of an area about the centroidal axis
q live load per unit area
q p, qs reinforcement indices for prestressed and non-prestressed steel
R relaxation force in the prestressing steel
relaxation of prestress (in percent)
time-dependent loss parameter (Pe/Pi)
ratio of cube and cylinder strengths
radius of curvature
Ru ultimate strength
R* factored design action for the strength limit state
R1000, R∞ relaxation of prestressing steel (in percent) after 1000 h and at time infinity, respectively
r radius of gyration
s spacing between stirrups or ties
T resultant tensile force
twisting moment or torque temperature
Tb tension resulting from bursting
Tcr twisting moment at first cracking
Tp tension in the prestressed steel
Ts tension in the non-prestressed steel
twisting moment transferred to side face of column
Tu ultimate strength in torsion
Tuc torsional strength of a beam without torsional reinforcement (Eqn 5.28)
Tus torsional strength of a beam containing torsional reinforcement (Eqn 5.29)
Tu,max maximum torsional strength of a cross-section
T1 twisting moment carried by the torsion strip
T* factored design torsion for the strength limit state
ΔT restraining force at level of non-prestressed steel
T tensile force increment imposed on concrete
T restraining force at level of prestressed steel
U internal work
u perimeter of the critical section for punching shear
V shear force
Vb , Vs shear transferred to the front and side faces of a column, respectively
Vcr shear force acting with torque Tcr at first cracking
Vo shear force corresponding to the decompression moment Mo
Vt shear force required to produce a web-shear crack
Vu ultimate shear strength
Vuc contribution of concrete to the shear strength
Vuo shear strength of the critical shear perimeter with no moment transferred
Vus contribution of transverse steel to the shear strength
Vu,max maximum shear strength of a beam (Eqn 5.7)
Vu,min shear strength of a beam containing the minimum shear reinforcement (Eqn 5.6)
V1 shear carried by the torsion strip
V* factored design shear force for the strength limit state
design horizontal shear force and nominal shear stress; respectively
C deflection at midspan
cr deflection due to creep
cx mx deflection of the column strip and the middle strip in the x-direction
υ , υ deflection of the column strip and the middle strip in the y-direction
i deflection immediately after transfer
LT time-dependent part of the total deflection
max maximum permissible total deflection
maximum deflection of a flat plate (Eqn 11.11)
sh deflection due to shrinkage
sus short-term deflection caused by the sustained loads
tot total deflection
υ var deflection due to variable loads
W wind load
w uniformly distributed load
wb the balanced load
w G, wQ uniformly distributed dead and live loads, respectively
wp uniformly distributed transverse load exerted on a member by a parabolic tendon profile
w px, wpy transverse loads exerted by tendons in the x- and y-directions, respectively (Eqn 10.3)
w sw self-weight
wt total equivalent long-term load (Eqn 8.4)
w ub, wu unbalanced load
w us sustained part of the unbalanced load
wυ variable or transient part of the uniform load
w* factored design load for the strength limit state
x direction of member axis
x, y shorter and longer overall dimensions of the rectangular parts of a solid section
x1 , y1 shorter and larger dimension of a closed rectangular tie
y direction perpendicular to the member axis depth below reference level (either centroidal axis
or top fibre)
yb , yt distance from centroidal axis to bottom and top fibre, respectively
Z section modulus
Zb , Z t bottom and top fibre section moduli (I/y b, I/yt) respectively
Zb,pc, bottom and top fibre section moduli of the precast part of a composite cross-section
Zb,comp bottom fibre section modulus of a composite cross-section
(Zb )min minimum bottom fibre section modulus (Eqn 3.9)
α a parameter to account for the effect of cracking and reinforcement quantity on the restraint to
creep (Eqn 3.76)
twice the slope of the prestress line (Fig. 3.21b)
constant associated with the development of concrete strength with time (Eqn 2.2)
factor that depends on the support conditions of a two-way edge-supported slab
b t section properties relating to bottom and top fibres (A/Zb and A/Zt, respectively)
αn factor to define the shape of a biaxial bending contour (Eqn 12.18)
αt sum of the successive angular deviations of a tendon (Eqn 3.60)
αυ angle between shear reinforcement and longitudinal tensile steel
β deflection coefficient
shrinkage deflection coefficient
constant associated with the development of concrete strength with time (Eqn 2.2)
βc ratio of long side to short side of the loaded area (in punching shear calculations)
βh ratio of the longest overall dimension of the effective loaded area to the overall dimension
measured in the perpendicular direction (Eqn 5.52)
βp angular deviation term (Eqn 3.60)
x y moment coefficients in a two-way slab (Eqn 10.8)
1 2 tension stiffening constants (Eqn 3.74)
4 5 coefficients related to the surface of the shear plane (Eqn 7.29)
γ ratio of the depth of the idealized rectangular compressive stress block to the depth of the
neutral axis at the ultimate strength in bending or combined bending and compression
c, s partial safety factor for concrete and steel, respectively
m partial material safety factor
υ fraction of unbalanced moment transferred to a column by eccentricity of shear (Eqn 5.49)
Δ an increment or a change
lateral displacement (sway) at the top of a column
slip or draw-in (in mm) at the anchorage of a tendon
b s moment magnification factor for a braced and for an unbraced column, respectively
i, δ initial and time-dependent lateral displacement, respectively, of a slender column
c, c(t) creep strain of concrete at time t
creep strain at time t due to a stress first applied at
final creep strain at time infinity
ce strain in the concrete at the level of the prestressed steel due to the effective prestress
cu extreme concrete fibre compressive strain at the ultimate limit state
e, e(t) instantaneous or elastic component of concrete strain at time t
oi initial strain in the top concrete fibre
p, s strain in the prestressed and non-prestressed steel, respectively
pe strain in the prestressed steel due to the effective prestress (Eqn 3.31)
pt tensile strain in the concrete at the level of the prestressed steel in the post-cracking range
and at the ultimate moment
pu strain in the prestressed steel at ultimate
s strain in the non-prestressed steel
sc st strain in the non-prestressed compressive and tensile steel, respectively
ε, ε(t) shrinkage strain at time t
final shrinkage strain at time infinity
sh shrinkage strain after 28 days of drying
y yield strain
Δε change in strain with time t
ε change in top fibre strain with time
θp angle between the direction of the prestressing tendon and the horizontal
υ t angles of the inclined crack caused by shear (Eqn 5.4) and by torsion (Eqn 5.30) respectively
xi initial curvature
xp curvature of prestressing tendon
xsh curvature induced by shrinkage
xsus curvature caused by the sustained loads
xu curvature at ultimate
(x u)min minimum curvature at ultimate for a ductile cross-section (Eqn 4.6)
Δx change in curvature with time
λ long-term deflection multiplication factor
µ friction curvature coefficient (Eqn 3.60)
friction coefficient on the surface of a crack (Eqn 7.33)
ν Poisson’s ratio for concrete
ρ reinforcement ratio, Ast/Ac
density of concrete
Σ sum of
σ stress in the concrete
σb bearing stress
σcp stress in the concrete at the level of the prestressing steel
σcu maximum compressive concrete stress
cube strength of concrete
σi initial stress in the concrete
σo stress at the time of first loading
σoi initial concrete stress in the top fibre
p s stress in the prestressed and non-prestressed steel, respectively
σpe stress in the prestressed steel due to the effective prestressing force
σpi stress in the prestressed steel immediately after transfer
σpu stress in the prestressed steel at ultimate
σs permissible steel stress
sc st stress in the non-prestressed compressive and tensile steel, respectively
t, b top and bottom fibre concrete stresses, respectively
x y longitudinal and transverse stress in the anchorage zone
average stress imposed by the longitudinal prestress in each direction of a two-way slab
1 2 principal stresses in the concrete
age of concrete at first loading
strength reduction factor
creep coefficient at time t due to stress first applied at
a reference creep coefficient (Eqn 2.20)
final creep coefficient at time infinity
increment of the creep coefficient associated with a particular time interval
ageing coefficient at time t for concrete first loaded at
* final ageing coefficient at time infinity
serviceability load factor
short-term serviceability load factor
long-term serviceability load factor
ζ coefficient associated with the effective moment of inertia (Eqn 3.74).
Reinforced concrete is the most widely used structural material of the 20th century. Because
the tensile strength of concrete is low, steel bars are embedded in the concrete to carry all
internal tensile forces. Tensile forces may be caused by imposed loads or deformations, or by
load-independent effects such as temperature changes or shrinkage.
Consider the simple reinforced concrete beam shown in Figure 1.1. The external loads
cause tension in the bottom fibres which may lead to cracking, as shown. Practical reinforced
concrete beams are usually cracked under the day-to-day service loads. On a cracked cross-
section, the applied moment is resisted by compression in the concrete above the crack and
tension in the bonded reinforcing steel. Although the steel reinforcement provides the cracked
concrete beam with flexural strength, it does not prevent cracking and does not prevent the
loss of stiffness caused by cracking. Crack widths are approximately proportional to the strain,
and hence stress, in the reinforcement. Steel stresses must therefore be limited to some
appropriately low value in order to avoid excessively wide cracks. Similarly, large steel strain
is the result of large curvature, which in turn is associated with large deflection. There is little
benefit to be gained, therefore, by using higher strength steel or concrete, since in order to
satisfy serviceability requirements, the increased strain capacity afforded by higher strength
steel cannot be utilized.
Prestressed concrete is a particular form of reinforced concrete. Prestressing involves the
application of an initial compressive load on a structure to reduce or eliminate the internal
tensile forces and thereby control or eliminate cracking. The initial compressive load is
imposed and sustained by highly tensioned steel reinforcement reacting on the concrete. With
cracking reduced or eliminated, a prestressed section is considerably stiffer than the
equivalent (usually cracked) reinforced section. Prestressing may also impose internal forces
which are of opposite sign to the external loads and may therefore significantly reduce or even
Figure 1.1 A reinforced concrete beam.
With service load behaviour improved, the use of high-strength steel reinforcement and high-
strength concrete becomes both economical and structurally efficient. As will be seen
subsequently, only steel which can be tensioned with large initial elastic strains is suitable for
prestressing concrete. The use of high-strength steel is therefore not only an advantage to
prestressed concrete, it is a necessity. Prestressing results in lighter members, longer spans,
and an increase in the economical range of application of reinforced concrete.
1.2 Methods of prestressing
As mentioned in the previous section, prestress is usually imparted to a concrete member by
highly tensioned steel reinforcement (wire, strand, or bar) reacting on the concrete. The high-
strength prestressing steel is most often tensioned using hydraulic jacks. The tensioning
operation may occur before or after the concrete is cast and, accordingly, prestressed members
are classified as either pretensioned or post-tensioned.
1.2.1 Pretensioned concrete
Figure 1.2 illustrates the procedures for pretensioning a concrete member. The prestressing
tendons are initially tensioned between fixed abutments and anchored. With the formwork in
place, the concrete is cast around the highly stressed steel tendons and cured. When the
concrete has reached its required strength, the wires are cut or otherwise released from the
abutments. As the highly stressed steel attempts to contract, the concrete is compressed.
Prestress is imparted via bond between the steel and the concrete.
Pretensioned concrete members are often precast in pretensioning beds long enough to
accommodate many identical units simultaneously. To decrease the construction cycle time,
steam curing may be employed to
Figure 1.2 Pretensioning procedure.
facilitate rapid concrete strength gain and the concrete is often stressed within 24 hours of
casting. Because the concrete is usually stressed at such an early age, elastic shortening of the
concrete and subsequent creep strains tend to be high. This relatively high time-dependent
shortening of the concrete causes a significant reduction in the tensile strain in the bonded,
prestressing steel and a relatively high loss of prestress.
1.2.2 Post-tensioned concrete
The procedures for post-tensioning a concrete member are shown in Figure 1.3. With the
formwork in position, the concrete is cast around hollow ducts which are fixed to any desired
profile. The steel tendons are usually in place, unstressed in the ducts during the concrete pour,
or alternatively may be threaded through the ducts at some later time. When the concrete has
reached its required strength, the tendons are tensioned. Tendons may be stressed from one
end with the other end anchored or may be stressed from both ends, as shown in Figure 1.3b.
The tendons are then anchored at each stressing end.
The concrete is compressed during the stressing operation and the prestress is maintained
after the tendons are anchored by bearing of the end anchorage plates onto the concrete. The
post-tensioned tendons also impose a transverse force to the member wherever the direction
of the cable changes.
After the tendons have been anchored and no further stressing is
Figure 1.3 Post-tensioning procedure.
required, the ducts containing the tendons are often filled with grout under pressure. In this
way, the tendons are bonded to the concrete and are more efficient in controlling cracks and
providing ultimate strength. Bonded tendons are also less likely to corrode or lead to safety
problems if a tendon is subsequently lost or damaged. In some situations, however,
particularly in North America and Europe, tendons are not grouted for reasons of economy
and remain permanently unbonded.
Most in situ prestressed concrete is post-tensioned. Relatively light and portable hydraulic
jacks make on-site post-tensioning an attractive proposition. Post-tensioning is also used for
segmental construction of large-span bridge girders.
Prestress may also be imposed on new or existing members using external tendons or such
devices as flat jacks. These systems are useful for temporary prestressing operations but may
be subject to high time-dependent losses.
1.3 Introductory example
Consider an unreinforced concrete beam of rectangular section, simply supported over a span
L, and carrying a uniform load w, as shown in Figure 1.4a. When the tensile strength of
concrete is reached in the bottom fibre
Figure 1.4 Introductory example.
at mid-span, cracking and a sudden brittle failure occur. If it is assumed that the concrete
possesses zero tensile strength, then no load can be carried and at failure w=0.
An axial compressive force P applied to the beam, as shown in Figure 1.4b, induces a
uniform compressive stress of intensity P/A. For failure to extreme fibre tensile stress at mid-
span equal to P/A. If linear-elastic occur, the moment caused by the external load w must now
induce an material behaviour is assumed, simple beam theory gives
If the prestressing force P is applied at an eccentricity of D/6, as shown in Figure 1.4c, the
compressive stress caused by P in the bottom fibre at mid-span is equal to
and the external load at failure w must now produce a tensile stress of 2P/A in the bottom
fibre. That is
By locating the prestress at an eccentricity of D/6, the load-carrying capacity is effectively
The eccentric prestress induces an internal bending moment Pe which is opposite in sign to
the moment caused by the external load. An improvement in behaviour is obtained by using a
variable eccentricity of prestress along the member. This may be achieved using a draped
If the prestress countermoment Pe is equal and opposite to the load-induced moment all
along the span, each cross-section is subjected only to axial compression, i.e. each section
suffers a uniform compressive stress of P/A. No cracking can occur and, since the curvature
on each section is zero, the beam does not deflect. This is the balanced load stage.
1.4 Transverse forces caused by draped tendons
In addition to the longitudinal force P exerted on a prestressed member at the anchorages,
transverse forces are also exerted on the member wherever curvature exists in the tendons.
Consider the simply supported beam in Figure 1.5a which is prestressed by a cable with a kink
at mid-span. The eccentricity of the cable is zero at each end and e at mid-span. The slope of
the two straight segments of cable is θand because θ small
Figure 1.5 Beam with centrally depressed tendon.
In Figure 1.5b, the forces exerted by the tendon on the concrete are shown. At mid-span, the
cable exerts an upward force R on the concrete. From statics, R equals the sum of the vertical
component of the prestressing force in the tendon on both sides of the kink:
At each anchorage, the cable has a horizontal component of P cos θ P for small θ and a
vertical component of P sin θ =2Pe/L.
The beam is said to be self-stressed. No external reactions are induced at the supports.
However, the beam suffers curvature and deflects upward owing to the internal bending
moment caused by prestress. As illustrated in Figure 1.5c, the internal bending moment at any
section can be calculated from statics and equals the product of the prestressing force P and
If the prestressing cable has a curved profile, the cable exerts transverse forces on the
concrete throughout its length. Consider the prestressed beam with the parabolic cable profile
shown in Figure 1.6. The shape of the parabolic cable is
Figure 1.6 Simple beam with parabolic tendon profile.
and its slope and curvature are, respectively,
From Equation 1.4, the slope of the cable at each anchorage when x=0 and x=L is
and therefore the horizontal and vertical components of the prestressing force at each
anchorage are P and 4Pe/L, respectively.
Equation 1.5 indicates that the curvature of the parabolic cable is constant along its length.
The curvature xp is the angular change in direction of the cable per unit length, as illustrated in
From the freebody diagram in Figure 1.7b, the cable exerts an upward transverse force
wp=Pxp per unit length. This upward force is an equivalent distributed load along the member
and, for a parabolic cable with the
Figure 1.7 Forces on a curved cable of unit length.
Figure 1.8 Forces exerted on a concrete beam by a parabolic tendon.
constant curvature given in Equation 1.5, wp is given by
If P is constant, which is never quite the case in practice, wp is uniformly distributed.
A freebody diagram of the concrete beam showing the forces exerted by the cable is
illustrated in Figure 1.8. Once again, the beam is self-stressed. No external reactions are
induced by the prestress. With the maximum eccentricity usually known, Equation 1.7 may be
used to calculate the value of P required to cause an upward force wp which exactly balances a
selected portion of the external load. Under this balanced load, the beam suffers no curvature
and is subjected only to the longitudinal compressive force P. This is the basis of a useful
design approach sensibly known as load balancing.
1.5 Calculation of elastic stresses
The components of stress on a prestressed cross-section caused by the prestress, the self-
weight, and the external loads are usually calculated using simple beam theory and assuming
linear-elastic material behaviour. In addition, the properties of the gross concrete section are
usually used in the calculations, provided the section is not cracked. Indeed, these
assumptions have already been made in the calculations for the introductory example in
Concrete, however, does not behave in a linear-elastic manner. Linear-elastic calculations
provide, at best, only an approximation of the state of stress on a concrete section immediately
after the application of the load. Inelastic creep and shrinkage strains may cause a substantial
redistribution of stresses with time, particularly on a section containing significant amounts of
Elastic calculations are useful, however, in determining, for example, if
tensile stresses occur at service loads, and therefore if cracking is likely, or if compressive
stresses are excessive and large time-dependent shortening may be expected. Elastic stress
calculations may therefore be used to indicate potential serviceability problems.
If an elastic calculation indicates that cracking may occur at service loads, the cracked
section analysis presented in Section 3.5 should be used to determine appropriate section
properties for all serviceability calculations. A more comprehensive picture of the variation of
concrete stresses with time can be obtained using the time analysis described in Section 3.6.
In the following sub-sections, several different approaches to the calculation of elastic
concrete stresses on an uncracked cross-section are described.
1.5.1 Combined load approach
The stress distributions on a cross-section caused by prestress, self-weight, and the applied
loads may be calculated separately and summed to obtain the combined stress distribution at
any particular load stage. Consider first the stresses caused by prestress and ignore all other
loads. On a section, such as that shown in Figure 1.9, equilibrium requires that the resultant of
the concrete stresses is a compressive force which is equal and opposite to the tensile force in
the steel tendon and located at the level of the steel, i.e. at an eccentricity e below the
centroidal axis. This is statically equivalent to an axial compressive force P and a moment Pe
located at the centroidal axis, as shown.
Figure 1.9 Concrete stress resultants and stresses caused by prestress.
The stresses caused by the compressive force P and the hogging (− moment Pe are also
shown in Figure 1.9. The resultant stress induced by the prestress is given by
where A and I are the area and second moment of area about the centroidal axis of the cross-
section, respectively, and y is the distance from the centroidal axis (positive downward). It is
common in elastic stress calculations to ignore the stiffening effect of the reinforcement and
to use the properties of the gross cross-section. For cross-sections containing significant
amounts of bonded steel reinforcement, however, the steel should be included in the
determination of the section properties.
The elastic stresses caused by an applied positive moment M on the uncracked section are
and the combined stress distribution due to prestress plus applied moment is shown in Figure
1.10 and given by
Figure 1.10 Combined stresses.
1.5.2 Internal couple concept
The resultant of the combined stress distribution shown in Figure 1.10 is a compressive force
of magnitude P located at a distance l above the level of the steel tendon, as shown in Figure
1.11. The compressive force in the concrete and the tension force in the steel form a couple
with magnitude equal to the applied bending moment, i.e.
Figure 1.11 Internal couple.
When M=0, the lever arm l is zero and the resultant concrete compressive force is located at
the steel level. As M increases and compressive stresses in the top fibres increase and those in
the bottom fibres decrease, the location of the resultant compressive force moves upward.
It is noted that provided the section is uncracked, the magnitude of P does not change
appreciably as the applied moment increases. The lever arm l is therefore almost directly
proportional to the applied moment. If the magnitude and position of the resultant of the
concrete stresses are known, the stress distribution can be readily calculated.
1.5.3 Load balancing approach
In Figure 1.8, the forces exerted on a prestressed beam by a parabolic cable were shown and
the uniformly distributed transverse load wp may be calculated from Equation 1.7. In Figure
1.12, all the loads acting on the beam, including the external gravity loads w, are shown.
If w=wp, the bending moment and shear force caused by the gravity load on every cross-
section are balanced by the equal and opposite values caused by wp . With the transverse loads
balanced, the beam is subjected only to the longitudinal prestress P applied at the anchorage.
If the anchorage is located at the centroid of the section, a uniform stress distribution of
intensity P/A occurs on each section and the beam does not deflect.
If w≠ p, the bending moment Mub caused by the unbalanced load (w− p) must be
calculated and the resultant stress distribution (given by Equation 1.9) must be added to the
stresses, caused by the axial prestress (P/A).
Figure 1.12 Forces imposed on a concrete beam with a parabolic tendon.
1.5.4 Example 1.1
The elastic stress distribution at mid-span of the simply supported beam shown in Figure 1.13
is to be calculated. Each of the procedures discussed in Sections 1.5.1–3 are illustrated in the
Figure 1.13 Beam of Example 1.1.
Combined load approach
The extreme fibre stresses at mid-span (σ σ) due to P, Pe and M are calculated separately
Due to P:
Due to Pe:
Figure 1.14 Component stress distributions in Example 1.1.
Due to M:
The corresponding concrete stress distributions are shown in Figures 1.14a, b and d,
respectively, and the combined elastic stress distribution on the concrete section at mid-span
is shown in Figure 1.14e.
Internal couple concept
An alternative approach for the calculation of elastic stresses is based on the internal couple
concept of Section 1.5.2. From Equation 1.11,
The resultant compressive force on the concrete section is 1760 kN and is located
306.8− 250=56.8 mm above the centroidal axis. This is statically equivalent to an axial
compressive force of 1760 kN (applied at the centroid) plus a moment
Mub=1760×56.8×10 −=100 kNm.
The extreme fibre concrete stresses are therefore
as shown in Figure 1.14e.
Load balancing approach
The elastic concrete stresses can also be determined using the load balancing procedure
outlined in Section 1.5.3. The transverse force imposed on the concrete by the parabolic cable
is obtained using Equation 1.7. That is,
The unbalanced load is therefore
and the resultant unbalanced moment at mid-span is
which, of course, is identical to the moment Mub calculated using the internal couple concept.
Once again, the elastic stresses at mid-span are obtained by adding the P/A stresses to those
caused by Mub:
1.6 Flexural behaviour—from initial to ultimate loads
The choice between reinforced and prestressed concrete for a particular structure is one of
economics. For relatively short-span beams and slabs, reinforced concrete is usually the most
economical alternative. As the span increases, however, reinforced concrete design is more
and more controlled by the serviceability requirements. Strength and ductility can still be
economicalIy achieved but, in order to prevent excessive deflection, cross-sectional
dimensions become uneconomically large. Excessive deflection is usually the governing limit
For medium- to long-span beams and slabs, the introduction of prestress improves both
serviceability and economy. The optimum level of prestress depends on the span, the load
history, and the serviceability requirements. Until recently, the level of prestress was usually
selected so that cracking at service loads did not occur. Frequently, this resulted in
unnecessarily high initial prestressing forces and, consequently, uneconomical designs. The
high initial prestress also often led to excessively large camber and/or axial shortening.
Members designed to remain uncracked at service loads are termed fully prestressed.
In building structures, there are relatively few situations in which it is necessary to avoid
cracking at service loads. In fact, the most economic design often results in significantly less
prestress than is required for a fully prestressed member. Frequently, such members are
designed to remain uncracked under the sustained or permanent load, with cracks opening and
closing as the variable live load is applied and removed. Prestressed concrete members
behave well in the post-cracking load range, provided they contain sufficient bonded
reinforcement to control the cracks. A cracked prestressed concrete section under service
loads is significantly stiffer than a cracked reinforced concrete section of similar size and
containing similar quantities of bonded reinforcement. Members that are designed to crack at
the full service load are called partially prestressed.
The elastic stress calculations presented in the previous section are applicable only if
material behaviour is linear-elastic and the principle of superposition is valid. These
conditions may be assumed to apply on a prestressed section prior to cracking, but only
immediately after the loads are applied. As was mentioned in the introduction to Section 1.5,
the gradual development of inelastic creep and shrinkage strains in the concrete can cause a
marked redistribution of stress between the bonded steel and the concrete on the cross-section.
The greater the quantity of bonded reinforcement, the greater is the time-dependent
redistribution of stress. For the determination of the long-term stress and strain distributions,
elastic stress calculations are not meaningful and may be misleading.
If the external loads are sufficient to cause cracking (i.e. the extreme fibre stress exceeds
the tensile strength of concrete), the short-term behaviour also becomes non-linear and the
principle of superposition is no longer applicable. As the applied moment on a cracked,
prestressed section increases, the crack depth gradually increases from the tension surface
towards the compression zone and the size of the uncracked part of the cross-section in
compression above the crack decreases. This is different to the post-cracking behaviour of a
conventionally reinforced concrete section. At first cracking on a reinforced section, the crack
suddenly propagates deep into the beam and the crack height and the depth of the concrete
compression zone remains approximately constant as the applied moment is subsequently
As the moment increases further into the overload region, the material behaviour becomes
increasingly non-linear, Permanent deformation occurs in the bonded prestressing tendons as
the stress approaches its ultimate value, the non-prestressed conventional reinforcement yields,
and the compressive concrete in the ever decreasing region above the crack enters the non-
linear range. The external moment is resisted by an internal couple,
with tension in the reinforcement crossing the crack and compression in the concrete and in
any reinforcement in the compressive zone. At the ultimate load stage, the prestressed section
behaves in the same way as a reinforced concrete section, except that the stress in the high-
strength steel reinforcement is very much higher. A significant portion of the very high steel
stress and strain is due to the initial prestress or, more precisely, the initial prestrain. If the
same higher strength steel were to be used without being initially prestrained, excessive
deformation and unacceptably wide cracks would result at only a small fraction of the
ultimate load (well below normal service loads).
The ultimate strength of a prestressed section depends on the quantity and strength of the
steel reinforcement. The level of prestress, however, and therefore the quantity of prestressing
steel are determined from serviceability considerations. In order to provide a suitable factor of
safety for strength, additional conventional reinforcement may be required to supplement the
prestressing steel in the tension zone. This is particularly so in the case of partially prestressed
members and may even apply for fully prestressed construction. The avoidance of cracking at
service loads and the satisfaction of selected elastic stress limits do not ensure adequate
strength. Strength must be determined from a rational analysis which accounts for the non-
linear material behaviour of both steel and concrete. Flexural strength analysis is described
and illustrated in Chapter 4, and analyses for shear and torsional strength are contained in
1.7 Design procedures
1.7.1 Limit states requirements
A structure and its components must simultaneously satisfy a number of different limit states
or design requirements. It must possess adequate strength, be stable, and perform
satisfactorily under service loads. Further, it must be durable, have adequate fire protection,
resist fatigue loading, and satisfy any special requirements which are related to its intended
use. Codes of practice specify design criteria which provide a suitable margin of safety
against a structure becoming unfit for service in any of these ways.
If a structure becomes unfit for service in any way, it is said to have entered a limit state.
Limit states are the undesirable consequences associated with each possible mode of failure.
In order to satisfy the design criteria set down in codes of practice, methods of design and
analysis should be used which are appropriate to the limit state being considered. For example,
if the strength of a cross-section is to be calculated, ultimate strength analysis and design
procedures are usually adopted. Collapse load methods of analysis and design (plastic
methods) may be suitable for calculating the
strength of ductile, indeterminate structures. If the serviceability limit states of excessive
deflection (or camber) or excessive cracking are considered, an analysis which accounts for
the non-linear and inelastic nature of concrete is usually required. The sources of this concrete
material non-linearity include cracking, tension stiffening, creep, and shrinkage. In addition,
creep of the high-strength prestressing steel (more commonly referred to as relaxation) may
affect in-service behaviour.
Each limit state must be considered and designed for separately. Satisfaction of one does
not ensure satisfaction of others. All undesirable consequences should be avoided. For each
limit state, the designer must compare the structure’s capacity with the appropriate external
loads. In the following sections, the design requirements for prestressed concrete are
discussed, including the specified loads and load combinations and the treatments of structural
safety contained in several major codes of practice.
1.7.2 Loads on structures
In the design of a concrete structure, the internal actions arising from the following loads
should be considered if applicable. The notation used here is based, where possible, on the
recommendations of ISO 3898:
Dead load (G); Live load (Q); Wind load (W); Prestress (P); Earthquake (Feq ); Earth pressure
(Fep ); Liquid pressure (Flp); and Snow load (Fs).
In addition, possible accidental loading and construction loads should be considered where
they may adversely affect the limit states requirements. Other actions which may cause either
stability, strength or serviceability failures include, creep of concrete, shrinkage (or
expansion) of concrete, temperature changes and gradients, foundation movements, and
Dead loads are usually defined as loads imposed by both the structural and non-structural
components of a structure. Dead loads include the self-weight of the structure and the forces
imposed by all walls, floors, roofs, ceilings, permanent partitions, service machinery, and
other permanent construction. Dead loads are usually permanent, fixed in position, and can be
estimated reasonably accurately from the mass of the relevant material or type of construction.
Normal weight prestressed (or reinforced) concrete, for example, weighs about 24 kN/m 3.
Lightweight reinforced concrete weighs between 15 and 20 kN/m 3.
Live loads are the loads which are assumed to arise from the intended use or purpose of the
structure and are generally specified by regional or national codes and specifications. A
number of these references are listed at the end of this chapter. Specified live loads depend on
the expected use
or occupancy of the structure and usually include allowances for impact and inertia loads
(where applicable) and for possible overload. In general, both uniformly distributed and
concentrated live loads are specified. At the design stage, the magnitude of the maximum live
load is never accurately known, and there is a small, but significant, probability that the
specified live load will be exceeded at some stage during the life of the structure. Live loads
may or may not be present at any particular time; they are not constant and their position can
vary. Although part of the live load is transient, some portion may be permanently applied to
the structure and have effects similar to dead loads. Live loads also occur during construction
due to stacking of building materials, the use of equipment, or the construction procedure
(such as the loads induced by floor-to-floor propping in multistorey construction).
Specified wind, earthquake, snow and temperature loads depend on the geographical
location and the relative importance of the structure (the mean return period). Wind loads also
depend on the surrounding terrain, the degree of shielding, and the height of the structure
above the ground. These environmental loads are also usually specified by regional or
national codes and specifications.
1.7.3 Load combinations for the strength limit states
The loads used in the design for strength are the specified values discussed above multiplied
by minimum load factors contained in the various codes of practice. With the built-in
allowance for overloads in most loading specifications, the specified loads will not often be
exceeded in the life of a structure. The load factors applied to each load type ensure that the
probability of strength failure is extremely low. Load factors provide only part of the overall
factor of safety against strength failure and are referred to in Europe as partial safety factors
for load. As will subsequently be seen, partial safety factors, in one form or another, are also
applied to the calculated strength of the structure.
The load factors depend on the type of load and the load combination under consideration.
For example, the load factors associated with dead loads are less than those for live or wind
loads, because the dead load is known more reliably and therefore less likely to be exceeded.
The load factors specified in several widely used concrete codes for particular load
combinations are summarized below. The most severe factored load combination should be
used in the design for strength.
ACI 318–83 (1983)
Wind: 0.75(1.4G+1.7Q+1.7W) or
Earthquake: As for wind, except that 1.1Feq is substituted for W
Earth pressure: 1.4G+1.7Q+1.7Fep or
BS 8110: Part 1 (1985)
Wind: 1.2G+1.2Q+1.2W or
Earth pressure: 1.4G+1.6Q+1.4Fep or
Liquid pressure: As for earth pressure
CEB–FIP Model Code (1978)
For earthquake, earth pressure, or liquid pressure, the same two load combinations as for wind
are used except that W is replaced by Feq , Fep or Flp, respectively. is a combination factor
which depends on the type of structure and accounts for the reduced probability that the
specified live load will be acting when the design wind (or earthquake) occurs. For example,
for dwellings and highway bridges and for offices, retail stores, and parking
Wind: 1.25G+1.5W or
Earthquake loads are treated similarly to wind loads. Earth and liquid pressures are taken as
live loads and factored accordingly.
AS 3600 (1988)
Dead+Live: 1.25G+1.5Q or
Earth pressure: 1.25G+1.5Q+1.5Fep or
Liquid pressure is factored similarly to earth pressure. depends on the type of occupancy:
for domestic, office, and parking areas, 0.5 for retail stores, and 0.6 for storage areas.
In addition to the above load combinations, AS 3600− 1988 specifies the following factored
combination of prestressed and dead load when considering compressive failure at transfer:
1.15G+1.15P or 0.8G+1.15P.
1.7.4 Load combinations for the stability limit states
All structures should be designed such that the factor of safety against instability due to
overturning, uplift, or sliding is suitably high. In general, most codes require that the structure
remains stable under the most severe of the load combinations for the strength limit states (see
Section 1.7.3). The Australian Standard for Concrete Structures AS 3600− 1988 suggests that
the loads causing instability should be separated from those tending to resist it. The design
action effect is then calculated from the most severe of the load combinations for the strength
limit state. The design resistance effect is calculated from 0.8 times the loads and other forces
tending to resist instability. The structure should be so proportioned that its design resistance
effect is not less than the design action effect.
Consider, for example, the case of a standard cantilever retaining wall. When checking for
overturning in accordance with AS 3600–1988, the overturning moment caused by both the
lateral earth pressure and the lateral thrust of any dead and live load surcharge would be
calculated using the worst factored load combination of Section 1.7.3. To provide a suitable
margin of safety against stability failure, the overturning moment should not be greater than
0.8 times the restoring moment caused by the wall self-weight and the weight Of the backfill
and other permanent surcharge above the wall.
1.7.5 Load combinations for the serviceability limit states
The design loads to be used in serviceability calculations are the day-to-day service loads
which may be considerably less than the specified loads. The specified live load Q, for
example, has a built-in allowance for overload and impact, and there is a relatively low
probability that this value will be exceeded. It is usually not necessary, therefore, to ensure
acceptable deflections and crack widths under the full specified live loads. The day-to-day
load combinations that exist under normal conditions of service are more appropriate.
ACI 318–83 (1983) does not make specific recommendations regarding load combinations
for serviceability calculations, except that adequate stiffness is required to limit the
deformation of a structure at service loads to a specified maximum value. Where the long-
term deformation is calculated,
only the dead load and the permanent portion of the live load need be considered.
BS 8110: Part 2 (1985) differentiates between the characteristic (or specified) loads and the
expected loads. Depending on the type of structure, the expected loads may be significantly
less than the characteristic loads. If the aim of the serviceability calculation is to produce a
best estimate of the likely behaviour, then expected loads should be used. The actual values of
these expected live loads are not specified and are deemed to be a matter for engineering
judgement. If the aim is to satisfy a particular serviceability limit state, and the consequences
of failure to do so are high, then the specified or characteristic service loads may be more
appropriate. Once again, the decision should be based on engineering judgement and
experience. BS 8110 specifies that for dead load the expected and the characteristic values are
the same and, therefore, the characteristic dead load should be used in all serviceability
calculations. For normal domestic or office occupancy, BS 8110 specifies that 25% of the live
load should be considered as permanent or sustained and the remainder may be assumed to be
transitory in nature. For storage areas, when an upper limit to the final long-term deflection is
required, 75% of the live load should be considered to be permanent.
The CEB–FIP Model Code (1978) specifies live load factors, and for serviceability
calculations. The following service load combinations should be considered:
The quasi-permanent loads:
The frequent (day-to-day) loads:
The infrequent (one-off) loads: G+P+Q
P is the mean prestressing force. is the short-term service load factor and equals 0.4 for
dwellings, 0.6 for offices and retail stores, 0.7 for parking areas, and for highway bridges may
be linearly interpolated between 0.7 for spans of 10 m and 0.5 for spans of 100 m. is the
long-term service load factor and equals 0.2 for dwellings, 0.3 for offices and retail stores, 0.6
for parking areas, and zero for highway bridges. For wind and snow loads, lies between 0.2
and 0.5 and
The Canadian code CAN3–A23.3–M84 (1984) suggests that the specified loads should be
used in serviceability calculations, except that for the estimate of long-term deflections, the
sustained loads only are to be considered. A load combination factor is introduced when
combinations of dead load and each of the following loads are considered: (a) live load, Q; (b)
wind or earthquake load, W; and (c) the cumulative effects of temperature, creep, shrinkage,
and differential settlement, T. The load combination for serviceability is therefore
where when only one of Q, W, or T is acting, 0.7 when two of Q, W, or T are acting,
and 0.6 when all three are acting.
The Australian code AS 3600–1988 adopts a similar approach to the CEB–FIP model code.
Live load factors, and are used in the following service load combinations:
is the minimum fraction of Q which is considered to be appropriate for short-term
serviceability calculations and is equal to 0.7 for dwellings, 0.5 for offices and parking areas,
0.6 for retail stores, 1.0 for storage areas, and for bridges varies linearly from 0.7 for spans of
10 m to 0.5 for spans of 100 m. is the minimum fraction of Q which may reasonably be
expected to be sustained or permanent in nature and is equal to 0.3 for dwellings and retail
stores, 0.25 for parking areas, 0.2 for offices, between 0.5 and 0.8 for storage areas, and zero
1.7.6 Design for the strength limit states
The design strength of a member or connection must always be greater than the design action
produced by the most severe factored load combination (as outlined in Section 1.7.3). On a
particular cross-section, the design action may be the axial load N*, shear force V*, the
bending moment M*, or the twisting moment T*, or combinations thereof.
The design strength of a cross-section is a conservative estimate of the actual strength. In
modern concrete codes, one of two alternative design philosophies is used to determine the
design strength. The first involves the use of strength (or capacity) reduction factors and the
second approach involves the use of partial safety factors for material strengths.
Design strength using strength reduction factors
The design strength of a cross-section is taken as the product of the ultimate strength, Ru, and
a strength reduction factor, . The strength reduction factor is a factor of safety introduced to
account for the variability of the material properties controlling strength and the likelihood of
underperformance; also accounts for possible variations in steel positions and concrete
dimensions, inaccuracies in design procedures and workmanship, and the degree of ductility
of the member.
Both ACI 318–83 (1983) and AS 3600 (1988) adopt this approach and the strength
reduction factors contained therein are summarized in Table 1.1. varies between 0.7 and 0.9
in ACI 318–83 (and 0.6 and 0.8 in AS 3600–1988), the lower end of the range being
applicable when concrete directly controls the strength and the upper end of the range when
strength depends primarily on the properties of the steel.
Table 1.1 Strength reduction factors (ACI 318–83 and AS 3600–1988).
Type of Action ACI 318–83 AS 3600–1988
(a) Flexure (with or without axial tension) and Axial tension 0.9 0.8
(b) Axial Compression and Axial Compression with Flexure
(i) Spiral reinforcement 0.75 0.6
(ii) Tied reinforcement 0.70 0.6
For small axial compression, may be increased linearly from the value given in (b) to the value given
in (a) as the axial compression tends to zero.
(c) Shear and torsion 0.85 0.7
(d) Bearing on Concrete 0.7 0.6
The determination of the ultimate strength Ru of a prestressed concrete section is based on the
characteristic strengths of the materials and their idealized constitutive relationships, the
principles of ultimate strength theory, and the fundamental concepts of mechanics. Procedures
for calculating the ultimate bending strength Mu are discussed in Chapter 4, the ultimate shear
strength Vu and torsional strength Tu in Chapter 5, and the ultimate strength of members in
axial compression and tension Nu in Chapter 12.
The design requirement for the strength limit state on each cross-section and at each
connection throughout the structure is
The design strength must be greater than or equal to the most severe design action.
Design strength using partial safety factors
The strength reduction factor is a safety factor which is applied to the ultimate strength of a
section, the ultimate strength being calculated from the characteristic or specified material
strengths. An alternative approach to
the determination of the design strength of a section is to apply the safety factors directly to
the material strengths.
For concrete, reinforcement bars, and prestressing tendons, the design strength of the
material is obtained from the characteristic strength divided by the appropriate partial safety
factor, γ. These reduced material strengths are then used to determine the design strength of
the section directly (using similar procedures to those used for calculating the ultimate
The partial safety factors for the constituent materials, γ, take account of the variability of
the material, the differences between actual material properties and laboratory-measured
values, local weaknesses, and inaccuracies in the methods of assessment of the resistance of
cross-sections. They serve the same function as strength reduction factors, but do so in,
arguably, a more rational way and provide a more consistent level of safety.
BS 8110: Part 1 (1985), the CEB–FIP Model Code (1978) and CAN3–A23.3–M84 (1984)
all use this approach. The partial safety factors for materials specified in each code are
BS 8110: Part 1 (1985)
For reinforcement (all types): γ=1.15
Concrete in flexure or axial load: γ
Shear strength without shear reinforcement: γ
Bond strength: γ
Others (e.g. bearing stress):
CEB–FIP Model Code (1978)
For concrete: γ
For steel: γ
For concrete: γ
For prestressing tendons (and structural steel): γ
For conventional reinforcing bar: γ
1.7.7 Design for the serviceability limit states
When designing for serviceability, the designer must ensure that the structure behaves
satisfactorily and can perform its intended function at service loads. Deflection (or camber)
must not be excessive, cracks must be adequately controlled, and no portion of the structure
should suffer excessive vibration.
The design for serviceability is possibly the most difficult and least well understood aspect
of the design of concrete structures. Service load behaviour depends primarily on the
properties of the concrete which are
often not known reliably. Moreover, concrete behaves in a non-linear and inelastic manner at
service loads. The non-linear behaviour of concrete which complicates serviceability
calculations is caused by cracking, tension stiffening, creep, and shrinkage.
In Chapter 3, design procedures for determining the in-service behaviour of beams are
presented, and Chapter 11 deals with serviceability aspects of the design of prestressed
concrete slabs. The level of prestress in beams and slabs is generally selected to satisfy the
The control of cracking in a prestressed concrete structure is usually achieved by limiting
the stress increment in the bonded reinforcement to some appropriately low value and
ensuring that the bonded reinforcement is suitably distributed. Many codes of practice specify
maximum steel stress increments after cracking and maximum spacing requirements for the
bonded reinforcement. For example, for the control of flexural cracking in partially
prestressed concrete beams, AS 3600 (1988) requires that the increment of stress in the steel
near the tension face is limited to 200 MPa as the load is increased from its value when the
extreme concrete tensile fibre is at zero stress to the full short-term service load. In addition,
the centre to centre spacing of reinforcement (including bonded tendons) must not exceed 200
For deflection control, the structural designer should select maximum deflection limits
which are appropriate to the structure and its intended use. The calculated deflection (or
camber) must not exceed these limits. Codes of practice give general guidance for both the
selection of the maximum deflection limits and the calculation of deflection. However, the
simplified procedures for calculating deflection in most codes were developed from tests on
simply supported reinforced concrete beams and often produce grossly inaccurate predictions
when applied to more complex structures. Reliable procedures for calculating deflections of
partially prestressed concrete beams are presented in some detail in Chapter 3.
Deflection problems which may affect the serviceability of prestressed concrete structures
can be classified into three main types:
(a) Where excessive deflection causes either aesthetic or functional problems.
(b) Where excessive deflection results in damage to either structural or non-structural
elements attached to the member.
(c) Where dynamic effects due to insufficient stiffness cause discomfort to occupants.
Examples of deflection problems of type (a) include objectionable visual sagging (or hogging),
and ponding of water on roofs. In fact, any deflection which prevents a member fulfilling its
intended function causes a problem of this type. Type (a) problems are generally overcome by
limiting the total
deflection to some appropriately low value. The total deflection is the sum of the short-term
and time-dependent deflection caused by the dead load (including self-weight), the prestress,
the expected in-service live load, and the load-independent effects of shrinkage and
Some codes (including ACI 318–83, BS 8110 1985, and CAN3–A23.3– M84) place no
maximum limit on the total deflection. However, when the total deflection exceeds about
span/200 below the horizontal, it may become visually unacceptable. Total deflection limits
which are appropriate for the particular member and its intended function must be decided by
the designer. A total deflection limit of span/200, for example, may be appropriate for the
floor of a carpark, but is inadequate for a gymnasium floor which may be required to remain
essentially plane under service conditions.
Examples of type (b) problems include deflections which result in cracking of masonry or
other partitions, damage to ceiling or floor finishes, and improper functioning of sliding
windows and doors. To avoid these problems, a limit must be placed on that part of the total
deflection that occurs after the attachment of such elements. This incremental deflection is
usually the sum of the long-term deflection due to all the sustained loads and shrinkage, the
short-term deflection due to the transitory live load, and any temperature-induced deflection.
For roof or floor construction supporting or attached to non-structural elements that are
unlikely to be damaged by large deflection, ACI 318–83 (1983) limits the incremental
deflection to span/240. Where such elements are likely to be damaged by large deflection, the
incremental deflection limit is reduced to span/480. Incremental deflections of span/480 can
cause cracking of supported masonry walls, particularly when doorways or corners prevent
arching and no provisions are made to minimize the effect of movement. AS 3600 (1988)
limits the incremental deflection for members supporting masonry partitions to between
span/500 and span/1000, depending on the provisions made to minimize the effect of
Type (c) deflection problems include the perceptible springy vertical motion of floor
systems and other vibration-related problems. Very little quantitative information for
controlling this type of deflection problem is available in codes of practice. ACI 318–83
(1983) places a limit of span/360 on the short-term deflection of a floor due to live load (and
span/180 for a flat roof). This limit provides a minimum requirement on the stiffness of
members which may, in some cases, be sufficient to avoid problems of type (c). For
prestressed concrete floors, type (c) problems are potentially the most common. Load
balancing is often employed to produce a nearly horizontal floor under the sustained load.
Such structures are generally uncracked at service loads, total deflection is small, and types
(a) and (b) deflection problems are easily avoided.
Where a structure supports vibrating machinery (or any other significant dynamic load) or
where a structure may be subjected to ground motion
caused by earthquake, blasting, or adjacent road or rail traffic, vibration control becomes an
important design requirement. This is particularly so for slender structures, such as tall
buildings or long-span beams and slabs.
Vibration is best controlled by isolating the structure from the source of vibration. Where
this is not possible, vibration may be controlled by limiting the frequency of the fundamental
mode of vibration of the structure to a value which is significantly different from the
frequency of the source of vibration. When a structure is subjected only to pedestrian traffic, 5
Hz is often taken as the minimum frequency of the fundamental mode of vibration of a beam
or slab (Irwin 1978, Mickleborough & Gilbert 1986).
AASHTO 1983. Standard specifications for highway bridges. Washington, DC: American Association
of State Highway and Transportation Officials.
ACI 318–83 1983. Building code requirements for reinforced concrete. Detroit: American Concrete
ACNBC 1985. National building code of Canada. Ottawa: National Research Council of Canada.
ANSI A58.1 1982. Minimum design loads for buildings and other structures. New York: American
National Standards Institute.
AS 1170.1 1989. SAA loading code, Part 1—Dead and live loads and load combinations. Sydney:
Standards Association of Australia.
AS 1170.2 1989. SAA loading code, Part 2—Wind loads. Sydney: Standards Association of Australia.
AS 3600 1988. Australian standard for concrete structures. Sydney: Standards Association of
BS 8110 1985. Structural use of concrete—parts 1 and 2. London: British Standards Institution.
CAN3–A23.3–M84 1984. Design of concrete structures for buildings. Rexdale, Canada: Canadian
CEB–FIP 1978. Model code for concrete structures. Paris: Comité Euro-International du Béton—
Fédération Internationale de la Precontrainie.
Irwin, A.W. 1978. Human response to dynamic motion of structures. Structural Engineer 56A, No. 9,
ISO 3898. Basis for the design of structures. Geneva: International Standards Organization.
Mickleborough, N.C. & R.I.Gilbert 1986. Control of concrete floor slab vibration by L/D limits.
Proceedings of the 10th Australasian Conference on the Mechanics of Structures and Materials.
Adelaide: University of Adelaide, 51–6.
Ministry of Transportation and Communications 1983. Ontario highway bridge design code
(OHBDC–1983), 2nd edn. Downsview, Ontario: Ministry of Transportation and Communications.
NAASRA 1976. Bridge design specification. Sydney: National Association of Australian State Road
Structural Engineers Association of California 1980. Recommended lateral force requirements and
commentary. San Francisco: Seismology Committee.
Design properties of materials
The behaviour of a prestressed concrete member throughout the full range of loading depends
on the properties and behaviour of the constituent materials. In order to satisfy the design
objective of adequate structural strength, the ultimate strengths of both concrete and steel
need to be known. In addition, factors affecting material strength and the non-linear behaviour
of each material in the overload range must be considered. In order to check for serviceability,
the instantaneous and time-dependent properties of concrete and steel at typical in-service
stress levels are required.
As was mentioned in Chapter 1, the prestressing force in a prestressed member gradually
decreases with time. This loss of prestress, which is usually 10–25% of the initial value, is
mainly caused by inelastic creep and shrinkage strains which develop with time in the
concrete at the level of the bonded steel. Reasonable estimates of the creep and shrinkage
characteristics of concrete and procedures for the time analysis of prestressed structures are
essential for an accurate prediction and a clear understanding of in-service behaviour.
Relaxation of the prestressing steel also causes a time-dependent loss of prestress. With the
current trend towards the use of low relaxation steels, however, this component of prestress
loss is usually small (less than 5%).
The intention in this chapter is to present a broad outline of material behaviour and to
provide sufficient quantitative information on material properties to complete most design
A more comprehensive treatment of the properties of concrete and the factors affecting them
was given by Neville (1981).
2.2 Composition of concrete
Concrete is a mixture of cement, water, and aggregates. It may also contain one or more
chemical admixtures. Within hours of mixing and placing, concrete sets and begins to develop
strength and stiff ness as a result of chemical reactions between the cement and water. These
reactions are known as hydration. Calcium silicates in the cement react with water to produce
calcium silicate hydrate and calcium hydroxide. The resultant alkalinity of the concrete helps
to provide corrosion protection for the reinforcement.
The relative proportions of cement, water, and aggregates may vary considerably
depending on the chemical properties of each component and the desired properties of the
concrete. A typical mix used for prestressed concrete by weight might be coarse aggregate
44%, fine aggregate 31%, cement 18%, and water 7%.
In most countries, several different types of Portland cement are available, including
normal cements, high early strength cements, low heat of hydration cements, and various
cements which provide enhanced sulphate resistance. In order to alter and improve the
properties of concrete, other cementitious materials may be used to replace part of the
Portland cement, e.g. fly ash, natural pozzolans, blast furnace slag, and condensed silica fume.
The ratio of water to cement by weight that is required to hydrate the cement completely is
about 0.25, although larger quantities of water are required in practice in order to produce a
workable mix. For the concrete typically used in prestressed structures, the water-to-cement
ratio is about 0.4. It is desirable to use as little water as possible, since water not used in the
hydration reaction causes voids in the cement paste that reduce the strength and increase the
permeability of the concrete.
The use of chemical admixtures to improve one or more properties of the concrete is now
commonplace. In recent years, high-strength concretes with low water-to-cement ratios have
been made more workable by the inclusion of superplasticizers in the mix. These polymers
greatly improve the flow of the wet concrete and allow very high-strength, low-permeability
concrete to be used with conventional construction techniques.
The rock and sand aggregates used in concrete should be properly graded and inert.
Expansive and porous aggregates should not be used and aggregates containing organic
matter or other deleterious substances, such as salts or sulphates, should also be avoided.
2.3 Strength of concrete
In structural design, the quality of concrete is usually controlled by the specification of a
minimum characteristic compressive strength at 28 days,
. The characteristic strength is the stress which is exceeded by 95% of the uniaxial
compressive strength measurements taken from standard compression tests. Such tests are
most often performed on 150 mm concrete cubes (in Europe and the UK) and on 150 mm
diameter by 300 mm long concrete cylinders (in North America and Australia). Because the
restraining effect at the loading surfaces is greater for the cube than for the longer cylinder,
strength measurements taken from cubes are higher than those taken from cylinders. The ratio
between cylinder and cube strength, R, is about 0.8 for low-strength concrete (i.e. cylinder
strengths of 20–30 MPa) and increases as the strength increases. The following expression for
R is often used (Neville 1981):
where σ is the cube strength in MPa (psi) and c=19.6 (2480). Throughout this book, refers
to the characteristic compressive strength obtained from cylinder tests.
In practice, the concrete used in prestressed construction is usually of better quality and
higher strength than that required for ordinary reinforced concrete. Values of in the range
30–40 MPa are most often used, but strengths as high as 60 MPa are not uncommon. In some
recent structures in North America, concrete strengths of over 100 MPa have been used
successfully. The forces imposed on a prestressed concrete section are relatively large and the
use of high-strength concrete keeps section dimensions to a minimum. High-strength concrete
also has obvious advantages in the anchorage zone of post-tensioned members where bearing
stresses are large, and in pretensioned members where a higher bond strength better facilitates
the transfer of prestress. As the compressive strength of concrete increases, so too does the
tensile strength. The use of higher strength concrete may therefore delay (or even prevent) the
onset of cracking in a member.
High-strength concrete is considerably stiffer than low-strength concrete. The elastic
modulus is higher and elastic deformations due to both the prestress and the external loads are
lower. In addition, high-strength concrete generally creeps less than low-strength concrete.
This results in smaller losses of prestress and smaller long-term deformations.
The effect of concrete strength on the shape of the stress-strain curve for concrete in
uniaxial compression is shown in Figure 2.1. The modulus of elasticity (the slope of the
ascending portion of each curve) increases with increasing strength and each curve reaches its
maximum stress at a strain of about 0.002.
The shape of the unloading portion of each curve (after the peak stress has been reached)
depends on, among other things, the characteristics of the testing machine. By applying
deformation to a specimen, instead of load,
Figure 2.1 Effect of strength on the compressive stress-strain curve.
in a testing machine which is stiff enough to absorb all the energy of a failing specimen, an
extensive unloading branch of the stress-strain curve can be obtained. Concrete can undergo
very large compressive strains and still carry load. This deformability of concrete tends to
decrease with increasing strength.
The strength of properly placed and well compacted concrete depends primarily on the
water-to-cement ratio, the size of the specimen, the size, strength, and stiffness of the
aggregate, the cement type, the curing conditions, and the age of the concrete. As mentioned
in Section 2.2, the strength of concrete increases as the water-to-cement ratio decreases.
The compressive strength of concrete increases with time, a rapid initial strength gain (in
the first day or so after casting) and a much slower, gradually decreasing rate thereafter. The
rate of development of strength with time depends on the type of curing and the type of
cement. In prestressed concrete construction, a rapid initial gain in strength is usually
desirable in order to apply the prestress as early as possible. This is particularly so in the case
of precast, pretensioned production. Steam curing and high early strength cement are often
used to this end.
The following expression is recommended by ACI–209 (1978) for predicting the strength
at any time from the measured or specified 28 day value:
where is the strength of the concrete at age t in days, is the concrete strength at
age 28 days, and α and β constants:
For normal Portland cement:
For moist cured concrete: α=4.0 β=0.85
For steam cured concrete: α=1.0 β=0.95
For high early strength cement:
For moist cured concrete: α=2.3 β=0.92
For steam cured concrete: α=0.7 β=0.98
The strength of concrete in tension is an order of magnitude less than the compressive
strength and is far less reliably known. A reasonable estimate is required, however, in order to
predict service-load behaviour in the post-cracking range. The flexural tensile strengths of
concrete (or modulus of rupture, ) is the extreme fibre stress calculated from the results of
standard flexural strength tests on plain concrete prisms and usually lies within the range
(in MPa). Because of the relatively large scatter of measured tensile strengths,
the lower end of this range is usually specified in building codes [such as ACI 318–83 (1983)
and AS 3600 (1988)]. For design purposes, the flexural tensile strength of normal weight
concrete may be taken as
In direct tension, where the tensile stress is uniform (or nearly so) over the section, the tensile
strength of concrete, , is lower and may be taken as
For lightweight aggregate concrete, these tensile strengths should be reduced by a factor of
In practice, concrete is often subjected to multi-axial states of stress. For example, a state of
biaxial stress exists in the web of a beam, or in a shear wall, or a deep beam. Triaxial stress
states exist within connections, in confined columns, in two-way slabs, and other parts of a
structure. A number of experimental studies of the behaviour of concrete under multi-axial
states of stress (particularly biaxial stress) have been undertaken, including those by Kupfer et
al. (1975) and Tasuji et al. (1978). The results of such studies have been particularly useful in
the formulation of material modelling laws for use in finite element studies of concrete
structures, such as by Darwin & Pecknold (1977), Gilbert (1979), and many more. A typical
biaxial strength envelope is shown in Figure 2.2. The strength of concrete under biaxial
compression is greater than for uniaxial compression. Transverse compression improves the
longitudinal compressive strength by confining
Figure 2.2 Typical biaxial strength envelope for concrete.
the concrete, thereby delaying (or preventing) the propagation of internal microcracks. Figure
2.2 also shows that transverse compression reduces the tensile strength of concrete, due
mainly to the Poisson’s ratio effect. Similarly, transverse tension reduces the compressive
strength. In triaxial compression, both the strength of concrete and the strain at which the peak
stress is reached are greatly increased and even small confining pressures can increase
strength significantly. Correctly detailed transverse reinforcement provides confinement to
produce a triaxial stress state in the compressive zone of columns and beams, thereby
improving both strength and ductility.
2.4 Deformation of concrete
The deformation of a loaded concrete specimen is both instantaneous and time dependent. If
the load is sustained, the deformation of the specimen gradually increases with time and may
eventually be several times larger than the instantaneous value.
The gradual development of strain with time is caused by creep and shrinkage. Creep strain
is produced by sustained stress. Shrinkage is independent of stress and results primarily from
the loss of water as the concrete dries. Creep and shrinkage cause increases in axial
deformation and curvature on reinforced and prestressed concrete cross-sections, losses of
prestress, local redistribution of stress between the concrete and the steel reinforcement, and
redistribution of internal actions in statically indeterminate members. Creep and shrinkage are
often responsible for excessive deflection (or camber) and excessive shortening of prestressed
members. In addition, shrinkage may cause unsightly cracking which could lead to
serviceability or durability problems. On a more positive note, creep relieves concrete of
stress concentrations and imparts a measure of deformability to concrete. A comprehensive
treatment of the effects of creep and shrinkage on the behaviour of concrete structures is
available elsewhere (Gilbert 1988).
Researchers have been investigating the time-dependent deformation of concrete ever since
it was first observed and reported almost a century ago, and an enormous volume of literature
has been written on the topic. Detailed summaries of the time-dependent properties of
concrete and the factors which affect them are contained in the books by Neville (1970, 1981)
and Neville et al. (1983).
The time-varying deformation of concrete may be illustrated by considering a uniaxially
loaded concrete specimen subjected to a constant sustained stress σfirst applied at time .
The total strain at any time may be assumed to be the sum of the instantaneous, creep,
and shrinkage components, as represented by the equation
The components of strain are illustrated diagramatically in Figure 2.3.
Figure 2.3 Strain vs time for specimen under constant compressive stress.
Shrinkage strains begin to develop as soon as drying commences at time (immediately
after setting or at the end of moist curing). Shrinkage continues to increase with time at a
gradually decreasing rate, as shown. When the stress is first applied at , the instantaneous
strain component causes a sudden jump in the strain diagram, which is followed by a further
increase in strain due to creep. Creep also increases with time at a gradually decreasing rate.
To predict accurately the time-varying behaviour of concrete, a knowledge of the
magnitude and rate of development of each of these strain components is required. In a
concrete structure, prediction of time-dependent deformation is complicated by the restraint to
creep and shrinkage provided by both the reinforcement and the external supports, and the
continuously varying concrete stress history that inevitably results. In Sections 2.4.2–4, the
material properties that influence each of the strain components in Figure 2.3 are summarized.
Methods for predicting the time-dependent behaviour of prestressed concrete cross-sections
and members are discussed in detail in Section 3.6.
2.4.2 Instantaneous strain
The magnitude of the instantaneous strain ε caused by either compressive or tensile stress
depends on the magnitude of the applied stress, the rate at which the stress is applied, the age
and the properties of the concrete and the proportions of its constituent materials. Consider the
uniaxial instantaneous strain versus compressive stress curve shown in Figure 2.4. When the
applied stress is less than about half of the compressive strength, the curve is essentially linear,
and the instantaneous strain is usually con-s sidered to be elastic (fully recoverable). In this
low-stress range, the secant
Figure 2.4 Typical stress vs instantaneous strain curve for concrete in compression.
modulus Ec does not vary significantly with stress and is only slightly smaller than the initial
tangent modulus. At higher stress levels, the curve is decidedly non-linear and a significant
proportion of the instantaneous strain is irrecoverable.
In concrete structures, compressive concrete stresses caused by the day-to-day service loads
rarely exceed half of the compressive strength. It is therefore reasonable to assume that the
instantaneous behaviour of concrete at service loads is linear-elastic and that instantaneous
strain is given by
The value of the elastic modulus Ec increases with time as the concrete gains strength and
stiffness. E c also depends on the rate of application of the stress and increases as the loading
rate increases. For most practical purposes, these variations are usually ignored and it is
common practice to assume that Ec is constant with time and equal to its initial value
calculated at the time of first loading, . For stress levels less than about , and for
stresses applied over a relatively short period (say up to 5 min), a numerical estimate of the
elastic modulus may be obtained from Pauw’s well known expression (Pauw 1960):
where ρ the density of concrete (about 2400 kg/m 3 for normal weight concrete) and
the average compressive strength in MPa at the time of first loading. Equation 2.7 is specified
in both ACI 318–83 (1983) and AS 3600 (1988).
When the stress is applied more slowly, say over a period of 1 day, significant additional
deformation occurs owing to the rapid early development of creep. For the estimation of
short-term deformation in such a case, it is recommended that the elastic modulus given by
Equation 2.7 be reduced by about 20% (Gilbert 1988).
The in-service performance of a concrete structure is very much affected by concrete’s
ability (or lack of it) to carry tension. It is therefore necessary to consider the instantaneous
behaviour of concrete in tension, as well as in compression. Prior to cracking, the
instantaneous strain of concrete in tension consists of both elastic and inelastic components.
In design, however, concrete is usually taken to be elastic-brittle in tension, i.e. at stress levels
less than the tensile strength of concrete the instantaneous strain versus stress relationship is
assumed to be linear. Although the initial elastic modulus in tension is a little higher than that
in compression, it is usual to assume that both values are equal and given by Equation 2.7.
cracking, therefore, the instantaneous strain in tension may be calculated using Equation 2.6.
When the tensile strength is reached, cracking occurs and the concrete stress perpendicular to
the crack is usually asssumed to be zero. In reality, if the rate of tensile deformation is
controlled, and crack widths are small, concrete can carry some tension across a crack owing
to friction on the rough, mating surfaces.
Poisson’s ratio for concrete, νlies within the range 0.15–0.22 and for most practical
purposes may be taken equal to 0.2.
2.4.3 Creep strain
For concrete subjected to a constant sustained stress, the gradual development of creep strain
was illustrated in Figure 2.3. In the period immediately after first loading, creep develops
rapidly, but the rate of increase slows appreciably with time. Creep is generally thought to
approach a limiting value as the time after first loading approaches infinity. Approximately
50% of the final creep develops in the first 2–3 months and about 90% after 2–3 years. After
several years under load, the rate of change of creep with time is very small. Creep of
concrete has its origins in the hardened cement paste and is caused by a number of different
mechanisms. A comprehensive treatment of creep in plain concrete was given by Neville et al.
Many factors influence the magnitude and rate of development of creep, including the
properties of the concrete mix and its constituent materials. In general, as the concrete quality
increases, the capacity of concrete to creep decreases. At a particular stress level, creep in
higher-strength concrete is less than that in lower-strength concrete. An increase in either the
aggregate content or the maximum aggregate size reduces creep, as does the use of a stiffer
aggregate type. Creep also decreases as the water-to-cement ratio is reduced.
Creep depends on the environment, and increases as the relative humidity decreases. Creep
is therefore greater when accompanied by shrinkage (drying). Creep is also greater in thin
members with large surface area to volume ratios, such as slabs. Near the surface of a member,
creep takes place in a drying environment and is therefore greater than in regions remote from
a drying surface. In addition to the relative humidity, creep is dependent on the ambient
temperature. A temperature rise increases the deformability of the cement paste and
accelerates drying, and thus increases creep. At 40°C, creep in concrete is about 25% higher
than that at 20°C. The dependence of creep on temperature is much more significant at more
In addition to the environment and the characteristics of the concrete mix, creep depends on
the loading history, in particular the magnitude of the stress and the age of the concrete when
the stress was first applied. When the sustained concrete stress is less than about (and
this is usually the
case in real structures at service loads), creep is proportional to stress and is sensibly known
as linear creep. At higher sustained stress levels, creep increases at a faster rate and becomes
non-linear with respect to stress. From a structural design point of view, non-linear creep is of
little interest and only the effects of linear creep are considered here. The age of the concrete
when the stress is first applied has a marked influence on the magnitude of creep. Concrete
loaded at an early age creeps more than concrete loaded at a later age.
Creep strain is made up of a recoverable component [called the delayed elastic strain, ε d(t)]
and an irrecoverable component [called flow, ε These components are illustrated by the
creep strain versus time curve in Figure 2.5a, which is caused by the stress history shown in
Figure 2.5b. The delayed elastic strain develops rapidly and is of the order of 40% of the
elastic strain. The flow component is sometimes further sub-divided into basic flow and
drying flow components; however, in structural analysis, it is not usually necessary to
distinguish between these components.
The capacity of concrete to creep is usually measured in terms of the creep coefficient
In a concrete specimen subjected to a constant sustained compressive stress σfirst
applied at age , the creep coefficient at time t is the ratio of creep strain to instantaneous
strain and is represented by
Figure 2.5 Recoverable and irrecoverable creep components.
For stress levels less than about , the creep coefficient is a pure time function,
independent of the applied stress, and has the same shape as the creep-time curve in Figure
2.3. As time approaches infinity, the creep coefficient is assumed to approach a final value
which usually falls within the range 1.5–4.0. A number of the well known
methods for predicting the creep coefficient were described and compared by Gilbert (1988).
Two of the simpler (and, therefore, more useful) approaches for making numerical estimates
of are presented in Section 2.5.
The effect of ageing is illustrated in Figure 2.6. The magnitude of the final creep coefficient
decreases as the age at first loading increases. That is,
This time-hardening or ageing of concrete complicates the calculation of creep strain caused
by a time-varying stress history.
The load-dependent strain at time t caused by a constant sustained stress σ is the sum of
the elastic and creep components and, using Equation 2.9, is given by
where is known as the effective modulus and is given by
If the stress is gradually applied to the concrete, rather than suddenly applied, the subsequent
creep strain is reduced significantly, since the concrete ages during the period of application
of the stress. This can be accom-
Figure 2.6 Effect of age at first loading on the creep coefficient (Gilbert 1988).
modated analytically by the use of a reduced or adjusted creep coefficient. For an increment
of stress, Δ , applied gradually to the concrete, the load-dependent strain may be obtained by
modifying Equation 2.11 as follows:
is often called the age-adjusted effective modulus, and χ an ageing coefficient first
introduced by Trost (1967) and later used by Bazant (1972). Like the creep coefficient, the
ageing coefficient depends on the duration of loading and the age at first loading and varies
between 0.6 and 1.0. For most practical purposes, χ be taken as 0.8. More accurate
estimates of χ based on the creep predictive models of ACI 209 (1978) and the CEB Model
Code (1978) have been made by Bazant (1972) and Neville et al. (1983), respectively.
The above discussion is concerned with compressive creep. In many practical situations,
however, creep of concrete in tension is also of interest. Tensile creep, for example, plays an
important part in delaying the onset of cracking caused by restrained shrinkage. The
mechanisms of tensile creep are thought to be different from those of compressive creep, but
at the same stress levels the magnitudes are similar. In design, it is usual to assume that the
creep coefficients in tension and in compression are identical. Although not strictly correct,
this assumption simplifies calculations and does not usually introduce serious inaccuracies. A
comprehensive comparison between tensile and compressive creep was made by Neville et al
2.4.4 Shrinkage strain
Shrinkage is the time-dependent strain measured in an unloaded and unrestrained specimen at
constant temperature. Concrete begins shrinking when drying commences and continues to
increase with time at a decreasing rate, as illustrated in Figure 2.3. Shrinkage is assumed to
approach a final value as time approaches infinity and is dependent on all the factors which
affect the drying of concrete, including the relative humidity, the mix characteristics (in
particular, the water content and water-to-cement ratio), and the size and shape of the member.
Shrinkage increases as the relative humidity of the surrounding air decreases. The drier the
atmosphere, the more rapid is the rate of drying
of the concrete and the larger are both the magnitude and rate of development of shrinkage
strain. A temperature rise accelerates drying and therefore increases the rate of shrinkage.
The amount of drying depends on the initial water content. A concrete specimen with a
high initial water-to-cement ratio will shrink more than a similar specimen made from
concrete with a lower water-to-cement ratio and kept under the same atmospheric conditions.
In addition, the volume and type of aggregate also affect shrinkage. Aggregate provides
restraint to deformation of the cement paste, so that shrinkage tends to decrease if the volume
of aggregate is increased or if a stiffer aggregate is used. Shrinkage in lightweight concrete is
therefore considerably greater (up to 50%) than in normal weight concrete.
The size and shape of the concrete member have a major influence on the magnitude and
rate of development of shrinkage. For a thin member with a large drying surface to volume
ratio, such as a suspended slab or wall, drying takes place rapidly and may be essentially
complete after several years. For the concrete in the interior of thicker members, such as
beams or columns, drying takes place more slowly and may continue throughout the lifetime
of the member. Shrinkage strain therefore varies across the depth (and width) of structural
members and is highest at the surfaces exposed to the atmosphere. In fact, for more massive
members, there is no significant drying (shrinkage) except in the concrete located within
about 300 mm of a drying surface.
Procedures for estimating the mean shrinkage on a cross-section are contained in many
building codes and other technical specifications. Two of the more simple approaches for
making rough estimates of shrinkage strain are presented in Section 2.5.
2.5 Predictions of the creep coefficient and shrinkage
Great accuracy in the prediction of the creep coefficient and shrinkage strain is not possible.
The variability of these material characteristics is high. Reasonable estimates can be made,
however, by extrapolation from short-term test results, using one of a number of mathematical
expressions which have been proposed to model the shape of the creep-time and shrinkage-
time curves. Creep strain is measured over a relatively short time period in laboratory
specimens subjected to constant stress. Shrinkage is also measured during the same period in
identical unloaded specimens. The longer the initial period of measurement, the better are the
Based on 28 day measurements , the ACI Committee 209 (1978) suggests
the following expressions for the creep coefficient at any time t after first loading and the
shrinkage strain in moist cured concrete at any time T after the commencement of drying:
In practice, structural designers seldom have the time or resources to commission laboratory
testing to determine material properties. Design predictions are more often made using one of
many numerical methods which are available for predicting the creep coefficient and
shrinkage strain. These methods vary in complexity, ranging from relatively complicated
methods, involving the determination of numerous coefficients that account for the many
factors affecting creep and shrinkage, to much simpler procedures. Comparisons between
predictions made using several of the more well known procedures were made by Gilbert
(1988) and Neville et al. (1983). Although the properties of concrete vary from country to
country as the mix characteristics and environmental conditions vary, the agreement between
the procedures for estimating both creep and shrinkage is still remarkably poor, particularly
for shrinkage. In addition, the comparisons between predictive models show that the accuracy
of a particular model is not directly proportional to its complexity, and predictions made using
several of the best known methods differ widely.
In the following sections, two simple methods for the estimation of the creep and shrinkage
characteristics of concrete are outlined. The first is that recommended in BS 8110 (1985) and
the second is similar to that recommended in AS 3600 (1988). In Appendix I, two of the most
widely used (and considerably more complex) alternative procedures are presented, namely
the recommendations of ACI 209 (1978) and CEB–FIP (1978). The variability of the time-
dependent properties of concrete is highlighted by the large differences in the predictions
made by each of these methods. From the point of view of the structural designer, there is
much to recommend a simple, approximate method which will provide a rough estimate of the
creep coefficient and shrinkage strain. After all, a rough estimate is all that is possible.
Predictions made using the following procedures will, in general, lead to estimates of
structural behaviour which are satisfactory for most practical purposes.
2.5.2 British standard—structural use of concrete, BS 8110: Part 2 (1985)
British Standard BS 8110 (1985) specifies a simple method for estimating the final (30 year)
creep and shrinkage.
The procedure outlined in BS 8110 is similar to an earlier proposal by the British Concrete
Society (1978) and is in fact based on the CEB–FIP (1970) recommendations. The static
modulus of elasticity of normal weight concrete at 28 days is specified as
where K o is a constant that depends on the stiffness of the aggregate and may be taken as 20
GPa for normal weight concrete, and fcu (28) is the 28 day cube strength in MPa. For
lightweight concrete of density ρ kg/m3), the right-hand side of Equation 2.17 should be
multiplied by (ρ /2400) 2. The elastic modulus at any time t may be derived from E c,28 using the
Figure 2.7 Final creep coefficient (BS 8110 1985).
The Standard suggests that the final creep strain may be predicted from
where is the elastic modulus at the time of loading and is the final creep coefficient.
Numerical estimates of may be obtained from Figure 2.7 [which is based on the CEB–FIP
(1970) recommendations]. Equation 2.19 implies that the final creep strain depends only on
the current concrete stress σ not on the previous stress history, which of course is wrong.
If reliable estimates of long-term deformation are required, Equation 2.19 should not be used.
A more reliable procedure for predicting creep strain, which better accounts for the previous
stress history, is presented in Section 3.6. The Standard points out that 40%, 60%, and 80% of
the final creep may be assumed to develop during 1, 6, and 30 months, respectively, under
Shrinkage strains after 6 months and after 30 years may be estimated from Figure 2.8 for
concrete of normal workability, without water reducing admixtures. Figure 2.8 was proposed
originally by Parrott (1979) and applies to concrete with a water content of about 190 l/m3.
Figure 2.8 Shrinkage for normal weight concrete (BS 8110 1985).
with a different water content, shrinkage may be regarded as proportional to water content
within the range 150–230 l/m3.
2.5.3 Australian standard AS 3600–1988
The creep coefficient at time t due to a sustained stress first applied at age is expressed as
In the absence of more reliable test data, the reference creep coefficient may be taken as
(MPa) 20 25 32 40 50
5.2 4.2 3.4 2.5 2.0
The constant k2 depends on the hypothetical thickness t h, the environment, and the duration of
load and can be determined from Figure 2.9. The hypothetical thickness of a member is
the ratio of its cross-sectional area to half of that part of the perimeter of the section which is
exposed to the atmosphere (the drying perimeter). k3 depends on the age of the concrete at the
time of loading and is obtained from the strength ratio using Figure 2.10.
Figure 2.9 Creep coefficient, k2 (AS 3600–1988).
Figure 2.10 Creep coefficient, k3 (AS 3600–1988).
The shrinkage strain at any time after the commencement of drying is given by
where k1 is obtained from Figure 2.11 and depends on the environment and the hypothetical
Figure 2.11 Shrinkage coefficient, k1 (AS 3600–1988).
2.6 Thermal expansion
The coefficient of thermal expansion of concrete depends on the coefficient of thermal
expansion of the coarse aggregate and on the mix proportions in general. For most types of
coarse aggregate, the coefficient lies within the
range 5×10 −− 13×10− per °C (Neville, 1981). For design purposes and in the absence of more
detailed information, a coefficient of thermal expansion for concrete of 10×10− per °C is
often recommended (AS 3600–1988).
2.7 Steel used for prestressing
The shortening of the concrete caused by creep and shrinkage in a prestressed member causes
a corresponding shortening of the prestressing steel which is physically attached to the
concrete either by bond or by anchorages at the ends of the tendon. This shortening can be
significant and usually results in a loss of stress in the steel of between 150 and 350 MPa.
Significant additional losses of prestress can result from other sources, such as friction along a
post-tensioned tendon or draw-in at an anchorage at the time of prestressing.
For an efficient and practical design, the total loss of prestress should be a relatively small
portion of the initial prestressing force. The steel used to prestress concrete must therefore be
capable of carrying a very high initial stress. A tensile strength of between 1000 and 1900
MPa is typical for modern prestressing steels. The early attempts to prestress concrete with
low-strength steels failed because the entire prestressing force was rapidly lost owing to the
time-dependent deformations of the poor-quality concrete in use at that time.
There are three basic types of high-strength steel commonly used as tendons in modern
prestressed concrete construction:
(a) cold-drawn, stress-relieved round wire;
(b) stress-relieved strand; and
(c) high-strength alloy steel bars.
Cold-drawn wires are manufactured to conform to the requirements of the relevant local code
or specification (such as ASTM A421 in the USA and AS 1310 in Australia). These
specifications outline the minimum required mechanical properties (such as ultimate tensile
strength, yield stress, and elongation at rupture) and dimensional tolerances. Wires are
produced by drawing hot-rolled steel rods through dies to produce wires of the required
diameter. The drawing process cold works the steel, thereby altering its mechanical properties
and increasing its strength. The wires are then
stress-relieved by a process of continuous heat treatment and straightening to produce the
required material properties. Wires are sometimes indented or crimped to improve their bond
Available sizes of wires vary from country to country, with diameters of 5–7 mm being the
most often used. Data for some commonly used wires in Australia are given in Table 2.1 and
a typical stress-strain curve is shown in Figure 2.12. The curve is typical of stress-strain
curves for high-strength prestressing steel, with no distinct yield point. Nevertheless, the so-
called yield stress is often referred to in codes and specifications and, unfortunately, is often
defined differently. Frequently, yield stress is defined as the stress at the 0.2% offset (AS
1310), as shown in Figure 2.12. The ASTM specification A421 specifies minimum yield
strengths for wire at 1% extension. For design purposes, the yield strength of stress-relieved
wires may be taken as 0.85 times the minimum tensile strength (i.e. 0.85f p) and the modulus
of elasticity of the wires may be taken as Ep =200×103 MPa.
Table 2.1 Tensile strengths of Australian prestressing steels (AS 3600–1988).
Material type and Nominal Area Minimum breaking Minimum tensile
Standard diameter mm mm2 load kN strength (fp) MPa
Wire 5 19.6 30.4 1550
5 19.6 33.3 1700
7 38.5 65.5 1700
7-wire strand super 9.3 54.7 102 1860
12.7 100 184 1840
15.2 143 250 1750
7-wire strand regular 12.7 94.3 165 1750
Bars (super grade) 23 415 450 1080
26 530 570 1080
29 660 710 1080
32 804 870 1080
38 1140 1230 1080
Figure 2.12 Typical stress-strain curve for stress-relieved wire.
In recent years, the use of wires in prestressed concrete construction has declined, with 7-wire
strand being preferred in most applications. Where wires are used in post-tensioned
applications, tendons consisting of many individual wires are generally employed.
Stress-relieved strand is the most commonly used prestressing steel. Strand must comply with
the requirements of the relevant local specifications (such as ASTM A416 and AS 1311–
1312). Strand is fabricated from a number of prestressing wires, usually seven (although 19-
wire strand is also available in some countries). Seven-wire strand consists of six wires tightly
wound around a seventh, slightly larger diameter, central wire. The pitch of the six spirally
wound wires is between 12 and 16 times the nominal diameter of the strand. After stranding,
the tendon is further stress-relieved. Low-relaxation (or stabilized) strand is most often used
by today’s prestressing industry.
Seven-wire strand is generally available in two grades, normal and super grade (Grades 250
and 270 in the USA). Diameters ranging from 7.9 to 15.2 mm are typical. Data for some
commonly used Australian strand are given in Table 2.1 and a typical stress-strain curve for a
12.7 mm diameter, super grade, 7-wire strand is shown in Figure 2.13.
The mechanical properties of the strand are slightly different from those of the wire from
which it is made. This is because the stranded wires tend
Figure 2.13 Typical stress-strain curve for 7-wire strand.
to straighten slightly when subjected to tension. For design purposes, the yield stress of stress-
relieved strand may be taken to be 0.85fp and the elastic modulus to be Ep=195×10 3 MPa.
Strand may be compacted by being drawn through a die, thereby compressing the outer six
wires more tightly around the central one. The cross-sectional area is therefore maintained but
the strand diameter is significantly reduced.
The high strength of alloy steel bars is obtained by the introduction of alloying elements in the
manufacture of the steel and by cold working (stretching) the bars. The bars are then stress-
relieved to obtain properties which meet the requirements of the relevant local specification
(e.g. ASTM A722 and AS 1313).
In the USA, both plain and deformed bars are available in two grades (f p=1000 and 1100
MPa) with diameters which range from 12.7 mm to 35 mm Some sizes and
properties of bars commonly used in Australia are presented in Tabie 2.1 and a typical stress-
strain curve is shown in Figure 2.14.
The elastic modulus for bars is generally lower than those for strand and wire. For design
purposes Ep may be taken to be 170×10 3 MPa and the yield stress (0.2% offset) may be taken
to be 0.85fp.
Figure 2.14 Typical stress-strain curve for alloy steel bars.
The stress-strain curves shown in Figures 2.12–2.14 exhibit similar characteristics. There is
no well defined yield point (as exists for lower strength reinforcing steels). Each curve has a
relatively high proportional limit. When the curves become non-linear as loading continues,
the stress gradually increases monotonically until the steel fractures. The elongation at
fracture is usually about 5%. High-strength steel is therefore considerably less ductile than
conventional, non-prestress reinforcing steel. Nevertheless, the material is ductile enough to
permit the design of ductile prestressed concrete flexural members which suffer large
deformations prior to failure.
2.8 Steel relaxation
The initial stress level in prestressing steel after transfer is usually high, often in the range 60–
75% of the tensile strength of the material. At such stress levels, high-strength steel creeps. If
a tendon is stretched and held at a constant length (constant strain), the development of creep
strain in the steel is exhibited as a loss of elastic strain, and hence a loss of stress. This loss of
stress in a specimen subjected to constant strain is known as relaxation. Relaxation in steel is
highly dependent on the stress level and increases at an increasing rate as the stress level
increases. Relaxation (creep) in steel increases rapidly with temperature. Both normal-
relaxation and low-relaxation steels are available. In recent years, low-relaxation steel has
Table 2.2 Basic Relaxation R1000 for Australian steel (AS 3600–1988).
Type of Steel R1000 (%) Low Relaxation R1000 (%) Normal Relaxation
Stress-relieved wire 2.0 6.5
Stress-relieved strand 2.5 7.0
Alloy steel bars 2.5 7.0
become the most popular because of the reduced time-dependent losses of prestress that result
from its use. Low relaxation steel has been stabilized by prestretching at an appropriate
Relaxation measurements are often made over a test period of 1000 hours on a specimen
subjected to constant strain at a constant temperature of 20°C. The initial stress levels usually
vary from 60 to 80% of the ultimate tensile strength. For an initial stress of 0.7 times the
ultimate tensile strength (i.e. σ=0.7f p), the relaxation of a tendon (i.e. the loss of stress due to
relaxation as a percentage of the initial stress) after 1000 h at 20°C is represented by R1000. For
Australian steels, R1000 may be taken from Table 2.2.
The design relaxation R (in percent) after a period of t days may be obtained from Equation
2.22 (AS 3600–1988):
The coefficient k1 depends on the initial stress level in the tendon and is obtained from Figure
2.15. The term k2 depends on the average annual temperature T and may be taken as T/20 but
not less than 1.0.
Very long-term relaxation values for prestressing steels were proposed by the CEB–FIP
(1978) and are given in Table 2.3.
Figure 2.15 Relaxation coefficient, k1 (AS 3600–1988).
Table 2.3 Very long-term relaxation R∞ (in percent) [CEB-FIP (1978)].
pi 0.6 0.7 0.8
Normal relaxation steel 6 12 25
Low relaxation steel 3 6 10
Ghali & Favre (1986) proposed an equation of the following form to approximate the data in
where η =150 for normal-relaxation steel and 67 for low-relaxation steel.
When elevated temperatures exist during steam curing or at other times, relaxation is
increased and occurs rapidly during the period of high temperature. For low-relaxation steel in
a concrete member subjected to an initial period of steam curing, it is recommended that the
design relaxation should be at least double the value given by Equation 2.22 (calculated with
2.9 Non-prestressed reinforcement
Conventional, non-prestressed reinforcement in the form of bars, cold-drawn wires, or welded
wire mesh is used in prestressed concrete structures for the same reasons as it is used in
conventional reinforced concrete construction. These include the following:
(a) To provide additional tensile strength and ductility in regions of the structure where
sufficient tensile strength and ductility are not provided by the prestressing steel. Non-
prestressed, longitudinal bars, for example, are often included in the tension zone of beams
to supplement the prestressing steel and increase the flexural strength. Non-prestressed
reinforcement in the form of stirrups is most frequently used to carry the diagonal tension
caused by shear and torsion in the webs of prestressed concrete beams.
(b) To control flexural cracking at service loads in partially prestressed concrete beams and
slabs where some degree of cracking under full service loads is expected.
(c) To control shrinkage and temperature cracking in regions and directions of low (or no)
(d) To carry compressive forces in regions where the concrete alone may not be adequate,
such as in columns or in the compressive zone of heavily reinforced beams.
(e) Lateral ties or helices are used to provide restraint to bars in compression (i.e. to prevent
lateral buckling of compressive reinforcement prior to the attainment of full strength) and
to provide confinement for the compressive concrete in columns, beams, and connections,
thereby increasing both the strength and deformability of the concrete.
(f) To reduce long-term deflection and shortening due to creep and shrinkage by the inclusion
of longitudinal bars in the compression region of the member.
(g) To provide resistance to the transverse tension that develops in the anchorage zone of
post-tensioned members and to assist the concrete to carry the high bearing stresses
immediately behind the anchorage plates.
(h) To reinforce the overhanging flanges in T-, I-, or L-shaped cross-sections in both the
longitudinal and transverse directions.
Non-prestressed reinforcement is manufactured to meet the requirements of the relevant local
codes or specifications. Types and sizes vary from country to country. In Australia, for
example, reinforcing bars are available in two grades, Grade 230 and 410 (which correspond
to characteristic yield
Table 2.4 Types and sizes of non-prestressed reinforcing bar in Australia.
Steel Grade and Guaranteed Bar Size db Nominal Mass per Nominal Area A s
Minimum Yield Stress (mm) metre (kg/m) (mm2)
Grade 230 (R-bars) fy=230 MPa R6 0.245 31
R10 0.632 80
12 0.910 110
16 1.618 200
20 2.528 310
Grade 410 fy=410 MPa Y-bars 24 3.640 450
28 4.955 620
32 6.471 800
36 8.190 1020
Figure 2.17 Stress-strain curve for non-prestressed steel usually assumed in design.
stresses of 230 and 410 MPa, respectively). Bars must comply with Australian Standard AS
1302, Steel reinforcing bars for concrete. Grade 230 bars are hot-rolled plain round bars 6 or
10 mm diameter (designated R6 and R10 bars) and are commonly used for fitments, such as
ties and stirrups. Grade 410 bars (known as tempcore or Y-bars) are hot-rolled deformed bars
with diameters ranging from 12 to 36 mm (in 4 mm increments). Available bar sizes and
properties are shown in Table 2.4. The regularly spaced, rib-shaped deformations on the
surface of a deformed bar provide a far better bond between the concrete and the steel and
greatly improve the anchorage potential of the bar. It is for this reason that deformed bars
rather than plain round bars are used as longitudinal reinforcement in most reinforced and
partially prestressed concrete members.
In reality, the actual yield stress of a reinforcing bar is usually significantly higher than the
guaranteed minimum indicated in Table 2.4. A typical stress-strain curve for Grade 410 steel
is shown in Figure 2.16. Note the distinct yield point and the large total elongation. Although
possessing less than one third of the strength of prestressing wire or strand, Grade 410 bars
are far more ductile.
Welded wire mesh is sometimes used in prestressed concrete slabs and is manufactured
from hard-drawn wire. In Australia, the characteristic yield strength of the wire is 450 MPa
and it is manufactured to comply with AS 1303, Hard-drawn reinforcing wire for concrete,
and AS 1304, Hard-drawn steel wire reinforcing fabric for concrete. The properties and
designations of available mesh sizes in Australia are given in Table 2.5.
In design calculations, non-prestressed steel is usually assumed to be elastic-plastic, that is
f y is taken to be the strength of the material. When fy is reached, the stress-strain curve is
assumed to be horizontal (perfectly plastic), as shown in Figure 2.17. The stress-strain curve
in compression is assumed to be similar to that in tension. The elastic modulus for non-
prestressed steel is taken to be E s=200×103 MPa.
ACI 318–83 1983. Building code requirements for reinforced concrete. Detroit: American Concrete
ACI Committee 209, Subcommittee II 1978. Prediction of creep, shrinkage and temperature effects, 2,
Draft Report. Detroit: American Concrete Institute.
AS 1310 1987. Steel wire for tendons in prestressed concrete. Sydney: Standards Association of
AS 1311 1987. Steel tendons for prestressed concrete 7-wire stress-relieved strand for tendons in
prestressed concrete. Sydney: Standards Association of Australia.
AS 1313 1989. Steel tendons for prestressed concrete, cold-worked high tensile alloy steel bars for
prestressed concrete. Sydney: Standards Association of Australia.
AS 3600–1988. Australian standard for concrete structures. Sydney: Standards Association of
ASTM Specification A416 1988. Steel strand, uncoated seven-wire stress-relieved strand for
prestressed concrete. Philadelphia: American Society for Testing and Materials.
ASTM Specification A421 1980. Uncoated stress-relieved steel wire for prestressed concrete.
Philadelphia: American Society for Testing and Materials.
ASTM Specification A722 1988. Uncoated high strength steel bar for prestressed concrete.
Philadelphia: American Society for Testing and Materials.
Baž Z.P. 1972. Prediction of concrete creep effects using age-adjusted effective modulus method.
Journal of the American Concrete Institute (ACI Journal) 69, April, 212–7.
British Concrete Society 1978. A simple design method for predicting the elastic modulus and creep of
structural concrete. Technical Report. London: British Concrete Society.
Broken Hill Proprietary Company 1983. Tempcore—Summarised technical information based on
European Tempcore. Data Sheets Sydney.
BS 8110 1985. Structural use of concrete, part 2, code of practice for special circumstances. London:
British Standards Institution.
CEB–FIP 1970. International recommendations for the design and construction of concrete structures.
Paris: Comité Euro-International du Béton.
CEB–FIP 1978. Model code for concrete structures. English Translation, April. Paris: Comité Euro-
International du Béton.
Darwin, D. & D.A.Pecknold 1977. Nonlinear biaxial stress-strain law for concrete. Journal of the
Engineering Mech. Division, ASCE 103, 229–41.
Ghali, A. & R.Favre, 1986. Concrete structures: stresses and deformations. London: Chapman and
Gilbert, R.I. 1979. Time-dependent behaviour of structural concrete slabs. PhD Thesis. Sydney:
School of Civil Engineering, University of New South Wales.
Gilbert, R.I. 1988. Time effects in concrete structures. Amsterdam: Elsevier.
Humes ARC Engineering Services 1985. Properties of reinforcing fabric and bar. Melbourne: Humes
ARC Engineering Services.
Kupfer, H.B., H.K.Hilsdorf & H.Rüsch 1975. Behaviour of concrete under biaxial stresses. ACI
Journal, 66, 656–66.
Neville, A.M. 1970. Creep of concrete: plain, reinforced and prestressed. Amsterdam: North-Holland.
Neville, A.M. 1981. Properties of concrete. London: Pitman.
Neville, A.M., W.H.Dilger & J.J.Brooks 1983. Creep of plain and structural concrete. London:
Parrott, L.J. 1979. Simplified methods for predicting the deformation of structural concrete.
Development Report No. 3. London: Cement and Concrete Association.
Pauw, A. 1960. Static modulus of elasticity of concrete as affected by density. ACI Journal 57, 679–
Rüsch, H. & D.Jungwirth 1976. Stahlbeton-Spannbeton, Band 2. Düsseldorf: Werner-Verlag.
Tasuji, M.E., F.O.Slate & A.H.Nilson 1978. Stress-strain response and fracture of concrete in biaxial
loading. ACI Journal 75, 306–12.
Trost, H. 1967. Auswirkungen des Superpositionsprinzips auf Kriech- und Relaxations Probleme bei
Béton und Spannbeton. Beton- und Stahlbetonbau 62, 230–8, 261–9.
Trost, H. 1978. Creep and creep recovery of very old concrete. RILEM Colloquium on Creep of
Design for serviceability
The level of prestress and the layout of the tendons in a member are usually determined from
the serviceability requirements for that member. If a water-tight and crack-free slab is
required, for example, tension in the slab must be eliminated or limited to some appropriately
low value. If, on the other hand, the deflection under a particular service load is to be
minimized, a load-balancing approach may be used to determine the prestressing force and
cable drape (see Section 1.5.3).
For the serviceability requirements to be satisfied in each region of a member and at all
times after first loading, a reasonably accurate estimate of the magnitude of prestress is
needed in design. This requires reliable procedures for the determination of both the
instantaneous and the time-dependent losses of prestress. Instantaneous losses of prestress
occur during the stressing (and anchoring) operation and include elastic shortening of the
concrete, friction along a post-tensioned cable, and slip at the anchorages. As has been
mentioned in the previous chapters, the time-dependent losses of prestress are caused by creep
and shrinkage of the concrete and stress relaxation in the steel. Procedures for calculating both
the instantaneous and time-dependent losses of prestress are presented in Section 3.7.
There are two critical stages in the design of prestressed concrete for serviceability. The
first stage is immediately after the prestress is transferred to the concrete, i.e. when the
prestress is at a maximum and the external load is usually at a minimum. The instantaneous
losses have taken place but no time-dependent losses have yet occurred. At this stage, the
concrete is usually young and the concrete strength may be relatively low. The prestressing
force immediately after transfer at a particular section is designated Pi . The second critical
stage is after the time-dependent losses have taken place and the full-service load is applied,
i.e. when the prestress is at a minimum and the external service load is at a maximum. The
prestressing force at this stage is designated P e.
At each of these stages (and at all intermediate stages), it is necessary to ensure that the
serviceability requirements of the member are satisfied. It is even more important, of course,
to make sure that strength requirements at each stage are also satisfied. It is not strength,
however, that determines the level of prestress, but serviceability. When the prestressing force
and the amount and distribution of the prestressing steel have been determined, the flexural
strength may be readily increased, if necessary, by the addition of non-prestressed
conventional reinforcement. This is discussed in considerably more detail in Chapter 4. Shear
strength may be improved by the addition of transverse stirrups (as discussed in Chapter 5).
As will be seen throughout this chapter, the presence of bonded conventional reinforcement
also greatly influences both the short- and long-term behaviour at service loads, particularly
for partially prestressed members. The design for strength and serviceability therefore cannot
be performed independently, as the implications of one affect the other.
General design requirements for the serviceability limit states, including load combinations
for serviceability, were discussed in Section 1.7. It is necessary to ensure that the
instantaneous and time-dependent deflection and the axial shortening under service loads are
acceptably small and that any cracking is well controlled by suitably detailed, bonded
reinforcement. To determine the in-service behaviour of a member, it is therefore necessary to
establish the extent of cracking, if any, by checking the magnitude of elastic tensile stresses. If
a member remains uncracked (i.e. the maximum tensile stress at all stages is less than the
tensile strength of concrete), the properties of the gross section may be used in all deflection
and camber calculations. If cracking occurs, a cracked section analysis may be performed to
determine the properties of the cracked section and the post-cracking behaviour of the
member. Such an analysis is described in Section 3.5.2.
3.2 Stress limits
Depending on the serviceability requirements for a particular structure, a designer may set
limits on the tensile and compressive stresses in concrete both at transfer and under the full
service loads. For the design of fully prestressed members (i.e. members in which cracking is
not permitted), some codes of practice (e.g. ACI 318–83) set mandatory maximum limits on
the magnitude of the concrete stress, both tensile and compressive. For partially prestressed
members, where cracking is permitted under normal service loads and the tensile stress limits
(often called permissible stresses) are exceeded, a detailed non-linear analysis is required to
determine behaviour in the post-cracking range.
The concrete stress limits specified in ACI 318–83 (here converted to SI
units) are as follows:
Immediately after transfer (before time-dependent losses):
(or at the ends of a simple member)
The quantity is the characteristic compressive strength of concrete at transfer. Where the
tensile stress exceeds these values, bonded reinforcement should be provided in the tensile
zone to resist the total tensile force in the concrete.
Under full service loads (after all losses):
When an analysis based on transformed cracked sections shows that both short- and long-term
deflections are acceptable, ACI 318–83 allows the tensile stress limit to be increased to
, provided the minimum concrete cover to the tendons is increased by 50% when the
cracked surface is exposed to earth, weather, or other corrosive environments.
Other codes (e.g. AS3600–1988) impose no mandatory concrete permissible stresses. The
choice of stress limit is left entirely to the designer and should be based on the appropriate
serviceability requirements. There is much to recommend this approach. Satisfaction of any
set of stress limits does not guarantee serviceability. Camber and deflection calculations are
still required. It is therefore appropriate to discuss the reasons for and the implications of
selecting particular stress limits.
Firstly, consider whether or not stress limits are required at transfer. There can be little
doubt that the magnitudes of both compressive and tensile concrete stresses at transfer need to
be carefully considered. It is important that the concrete compressive stress at the steel level at
transfer should not exceed about . At higher stress levels, large non-linear creep strains
develop with time, resulting in large creep deformation and high losses of prestress. Designers
must also check strength at transfer and the satisfaction of the above compressive stress limit
will usually, although not necessarily, lead to an adequate factor of safety against compressive
failure at transfer.
It is also advisable to limit the tensile stress at transfer, particularly in unreinforced regions.
The regions of a member which are subjected to tension at transfer are often those which are
later subjected to compression when the full service load is applied. If these regions are
unreinforced and uncontrolled cracking is permitted at transfer, an immediate serviceability
problem exists. When the region is later compressed, cracks may not close completely, local
spalling may occur, and even a loss of shear strength could result. If cracking is permitted at
transfer, bonded reinforcement should be provided to carry all the tension and to ensure that
the cracks are fine and well behaved.
In some cases, stress limits may also be required under full service loads when all prestress
losses have taken place. If cracking is to be avoided, some tensile stress limit must be adopted.
A value in the range is appropriate. If the upper end of this range is adopted,
some cracking may occur under full loads, particularly if the load-independent tension
induced by restrained shrinkage or temperature effects has not been adequately assessed.
Provided bonded reinforcement or tendons are provided near the tensile face, however, the
cracks will be well controlled and the resulting loss of stiffness will not be significant.
For many prestressed concrete situations, there is no reason why tensile cracking should be
avoided at service loads and, therefore, no reason why a limit should be placed on the elastic
tensile stress. If cracking is permitted, the resulting loss of stiffness must be accounted for in
deflection calculations and crack widths must be acceptably small. Crack control may be
achieved by limiting both the spacing of and the change of stress in the bonded reinforcement.
Where the cracked surface is not exposed to a corrosive environment, crack control may be
achieved by limiting the increment of stress in the bonded reinforcement after cracking to
about 200 MPa, and by limiting the centre-to-centre spacing of bonded reinforcement to about
200 mm for beams and 500 mm for slabs (AS 3600–1988). In order to calculate the loss of
stiffness caused by cracking or the increment of steel stress after cracking, a cracked section
analysis is required.
Under full service loads, which occur infrequently, there is often no practical reason why
compressive stress limits should be imposed. Separate checks for flexural strength, ductility
and shear strength are obviously necessary. Excessive compressive stresses may, however,
occur under full service loads in some types of members, such as trough girders or inverted T-
beams, and in the design of these members care should be taken to limit the extreme fibre
compressive stress at service loads. If a large portion of the total service load is permanent,
compressive stress levels in excess of should be avoided.
The primary objective in selecting concrete stress limits is to obtain a serviceable structure.
As was discussed in Section 1.5, elastic stress calculations are not strictly applicable to
prestressed concrete. Creep and shrinkage cause a gradual transfer of compression from the
concrete to the bonded steel. Nevertheless, elastic stress calculations may indicate potential
serviceability problems and the satisfaction of concrete tensile stress limits is a useful
procedure to control the extent of cracking. It should be understood, however, that the
satisfaction of a set of elastic concrete stress limits does
not, in itself, ensure serviceability and it certainly does not ensure adequate strength. The
designer must check separately both strength and serviceability, irrespective of the stress
limits selected. In the end, provided a structure is strong enough and is serviceable, the value
adopted for each stress limit is largely irrelevant.
Codes of practice also set mandatory limits on the tensile stress in the prestressing steel at
various stages of construction. ACI 318–83 specifies that the maximum stress applied to a
tendon during the jacking operation is 0.94fpy (but not greater than 0.85fp ). The relationships
between f py and f p for the various steel types were given in Section 2.7. ACI 318–83 also
requires that the steel stress immediately after transfer does not exceed 0.82fpy (but not greater
than 0.74fp) and, for post-tensioned tendons at anchorages and couplers, 0.70fp.
3.3 Determination of prestress and eccentricity in flexural members
There are a number of possible starting points for the determination of the prestressing force P
and eccentricity e required at a particular cross-section. The starting point depends on the
particular serviceability requirements for the member. The quantities P and e are often
determined to satisfy pre-selected stress limits. Cracking may or may not be permitted under
service loads. As was mentioned in the previous section, satisfaction of concrete stress limits
does not necessarily ensure that deflection, camber, and axial shortening are within acceptable
limits. Separate checks are required for each of these serviceability limit states. Alternatively,
the prestressing force and the cable layout may be selected to minimize deflection under some
portion of the applied load (i.e. a load-balancing approach to design). With such an approach,
cracking may occur when the applied load is substantially different from the selected balanced
load, such as at transfer or under the full service loads, and this needs to be checked and
accounted for in serviceability calculations.
3.3.1 Satisfaction of stress limits
Numerous design approaches have been proposed for the satisfaction of concrete stress limits,
including analytical and graphical techniques (e.g. Magnel 1954, Lin 1963, Warner & Faulkes
1979). A simple and convenient approach is described here.
If the member is required to remain uncracked throughout, suitable stress limits should be
selected for the tensile stress at transfer, Fti , and the tensile stress under full load, F t. In
addition, limits should also be placed on the concrete compressive stress at transfer, F ci, and
under full loads, Fc. If
Figure 3.1 Concrete stresses at transfer.
cracking under the full loads is permitted, the stress limit Ft is relaxed and the remaining three
limits are enforced.
Consider the uncracked cross-section of a beam at the critical moment location, as shown in
Figure 3.1. Also shown in Figure 3.1 are the concrete stresses at transfer caused by the
prestress P i (located at an eccentricity e below the centroidal axis of the concrete section) and
by the external moment Mo resulting from the loads acting at transfer. Often self-weight is the
only load (other than prestress) acting at transfer.
At transfer, the concrete stress in the top fibre must not exceed the tensile stress limit. That
and rearrangement gives
where A is the area of the section, I is the second moment of area of the section about the
centroidal axis, and Zt is the elastic section modulus, with respect to the top fibre (=I/yt ).
Similarly, the concrete stress in the bottom fibre must be greater than the negative
compressive stress limit at transfer:
where F ci is a negative quantity. Rearrangement gives
Figure 3.2 Concrete stresses under full loads (after all prestress losses).
Figure 3.2 shows the concrete stresses caused by the effective prestress after all losses have
taken place (Pe=RPi ) and by the applied moment MT resulting from the full service load.
For a fully prestressed member, the concrete stress in the bottom fibre must be less than the
selected tensile stress limit Ft:
The compressive stress in the top fibre must also satisfy the appropriate stress limit. Therefore,
Equations 3.1–3.4 can be rearranged to express 1/P i as a linear function of e. Rearrangement
of Equation 3.1 gives
and if at=A/Zt, then
Similarly, from Equations 3.2, 3.3 and 3.4, the following equations are obtained:
where α=A/Zb and Fci in Equation 3.6 and Fc in Equation 3.8 are negative numbers.
Each of the linear relationships in Equations 3.5–3.8 may be plotted on a graph of 1/Pi
versus e, as shown in Figure 3.3. The intercept of each straight line on the horizontal axis is
obtained by setting 1/Pi equal to zero in each equation. When 1/P i=0, the eccentricity e equals
1/αfor Equations 3.5 and 3.8 and –1/α for Equations 3.6 and 3.7. A graphical interpretation
of the stress conditions on a prestressed section similar to that shown in Figure 3.3 was first
proposed by Magnel (1954) and may be a useful aid in design.
On one side of each straight line in Figure 3.3, the relevant stress limit is satisfied. The
wedge-shaped area in which all four stress limits are satisfied represents suitable
combinations of Pi and e. In order to minimize prestressing costs, the smallest possible value
for P i would generally be selected. This corresponds to the value at the intersection of
Equations 3.5 and 3.7. However, the corresponding value of e may not be practical. The
maximum eccentricity emax is governed by concrete cover and tendon spacing requirements.
As is seen in Figure 3.3, the smallest possible value for Pi is obtained by substituting the
appropriate maximum eccentricity into Equation 3.7.
Figure 3.3 Magnel’s design diagram.
If a particular cross-section is too small, the plot of Equation 3.6 in Figure 3.3 will lie above
the plot of Equation 3.7 and no acceptable region exists. Similarly, if the line representing
Equation 3.5 is steeper than that of Equation 3.8, no acceptable region exists. It is therefore
not possible to satisfy all four stress limits and a larger section is clearly required. If, on the
other hand, the angle between the plots of Equations 3.6 and 3.7 in Figure 3.3 is large, a large
acceptable region exists and a smaller section may prove more economical.
When the minimum-sized cross-section is used, Equations 3.6 and 3.7 plot on the same line.
By equating Equations 3.2 and 3.3, the section modulus of this minimum-sized section (Zb)min
can be readily found. If the minimum-sized section is used, Equation 3.2 becomes
Similarly, from Equation 3.3,
By subtracting these two equations, an expression for the minimum permissible section
modulus is obtained:
It must be remembered that F ci is always negative. Equation 3.9 is a useful starting point in
the selection of an initial cross-section.
In order to use Equation 3.9 and to be able to plot Equation 3.7 on Figure 3.3, some
estimate of the time-dependent losses must be made so that the loss parameter R can be
determined. As R is varied, the angle between the plots of Equations 3.6 and 3.7 varies and
hence the range of acceptable combinations of Pi and e also varies. Usually, a first estimate of
R within the range 0.75–0.85 is adopted when low-relaxation steel is used. The lower end of
this range (i.e. R≈ 0.75) is more appropriate for a heavily stressed girder with high sustained
compressive stresses in the concrete at the tendon level. In such a member, creep losses will
be relatively high. For lightly stressed members, such as slabs, and for members in which the
sustained compressive stress in the concrete at the tendon level is low, the upper end of the
range is more appropriate (i.e. R≈ 0.85). Any initial estimate of R must be checked after the
prestress, the eccentricity, and the quantity of bonded reinforcement have been determined.
Suitable procedures for determining the time-dependent losses are described in Sections 3.6
For a limited amount of well controlled cracking, ACI 318–83 allows the tensile stress limit
F t to be set as high as provided bonded reinforcement is placed near the tensile face. In
general, however, if cracking is permitted under full service loads, a tensile stress limit Ft is
not specified and Equation 3.7 does not apply. Tensile and compressive stress limits at
transfer are usually enforced and, therefore, Equations 3.5 and 3.6 are still applicable and
continue to provide an upper limit on the level of prestress. The only minimum limit on the
level of prestress is that imposed by Equation 3.8 and, for more practical cross-sections, this
does not influence the design. When there is no need to satisfy a tensile stress limit under full
loads, the plot of Equation 3.7 no longer appears on Figure 3.3. Any level of prestress which
satisfies Equations 3.5, 3.6, and 3.8 may be used, including P i=0 (which corresponds to a
reinforced concrete member). In such a situation, Figure 3.3 is no longer of much use in
Often partially prestressed members are designed such that cracking does not occur under
the sustained or permanent service loads. It is the variable live load that causes cracking.
Cracks therefore open and close as the variable load is applied and removed. The selection of
prestress in such a case can still be made conveniently using a figure similar to Figure 3.3. If
the maximum total service moment MT is replaced in Equation 3.7 by the sustained or
permanent moment Msus, Equation 3.7 becomes
The plot of Equation 3.10 now replaces the plot of Equation 3.7 in Figure 3.3. The line
representing Equation 3.10 crosses the horizontal axis at the
same point (i.e. e=− b), but is steeper and therefore the acceptable region shown in Figure
3.3 is larger. For a given eccentricity, the minimum prestress Pi is less. The tensile stress limit
F t will not be exceeded under the sustained loads, but cracking may occur under peak live
loads. If after the variable load has been removed the cracks are required to close completely,
F t in Equation 3.10 should be set to zero.
If less prestress is used and cracking occurs, the cross-section required for a partially
prestressed member may need to be larger than that required for a fully prestressed member
for a particular deflection limit. In addition, the quantity of non-prestressed reinforcement is
usually significantly greater. Often, however, the reduction in prestressing costs more than
compensates for the additional concrete and non-prestressed reinforcement costs and partially
prestressed members are the most economical structural solution in a wide range of
A one-way slab is simply supported over a span of 12 m and is to be designed to carry a
service load of 7 kPa (kN/m2) in addition to its own self-weight. The slab is post-tensioned by
regularly spaced tendons with parabolic profiles. The material properties are:
The prestressing force and eccentricity are to be determined to satisfy the following concrete
At mid-span, the instantaneous and time-dependent losses are taken to be 8% and 16%,
respectively. In order to obtain an estimate of the slab self-weight (which is the only load
other than the prestress at transfer), a trial slab thickness of 300 mm (span/40) is assumed
initially. For a 1 m wide strip of slab, the self-weight is
and the moments at mid-span both at transfer and under the full service load are
From Equation 3.9,
and the corresponding minimum slab depth is therefore
Select a slab thickness D=300 mm. The relevant section properties are:
Equation 3.5 becomes
Similarly, the following expressions are obtained from Equations 3.6, 3.7 and 3.8,
Each of these four equations is plotted on Figure 3.4.
If 12.7 mm diameter strand is used with 30 mm minimum concrete cover, then
Figure 3.4 Design diagram for Example 3.1.
and, from Figure 3.4 (or Equation 3.7), the corresponding minimum permissible value of Pi is
found to be
At the jacking point, the required prestressing force is
From Table 2.1, a 12.7 mm diameter 7-wire, low-relaxation strand has a cross-sectional area
of 100 mm2 and a minimum breaking load of 184 kN. A flat duct containing four 12.7 mm
strands can therefore be stressed with a maximum jacking force of
The minimum number of cables required in each metre width of slab is therefore
and the maximum spacing between cables is
Use 1–4 strand tendon every 330 mm.
To check deflection, the properties of the gross section can be used in all calculations, since
cracking has been avoided both at transfer and under the full service loads. It is assumed that
of the 7 kPa service load, 3 kPa is sustained or permanent and 4 kPa is temporary.
The uniformly distributed upward load caused by the parabolic cables with drape equal to 114
mm is obtained from Equation 1.7 as
The resultant upward load is and the deflection (camber)
at transfer is
Under full loads:
After the time-dependent losses, the prestressing force has decreased by 16% and therefore
The sustained external load is and the short-term deflection due to
the permanent loads is
For this uncracked slab, the long-term deflection caused by creep and
shrinkage is likely to be at least three times the short-term deflection due to all the sustained
A far more accurate and reliable estimate of the effects of creep and shrinkage is outlined in
The instantaneous deflection caused by the variable portion of the service load, wυ =4.0
and the maximum total deflection is therefore
This may or may not be acceptable depending on the deflection requirements for this
To complete this design, strength checks must be made, losses must be checked, and the
anchorage zones must be designed.
Using the load-balancing approach, the effective prestress after losses Pe and the eccentricity
e are selected such that the transverse load imposed by the prestress wp balances a selected
portion of the external load. The effective prestress Pe in a parabolic cable of drape e required
to balance a uniformly distributed external load wb is obtained from Equation 1.7. That is,
Concrete stresses are checked under the remaining unbalanced service loads to identify
regions of possible cracking and regions of high compression. Deflection under the
unbalanced loads may need to be calculated and controlled. Losses are calculated and stresses
immediately after transfer are also checked. Having determined the amount and layout of the
prestressing steel (and the prestressing force) to satisfy serviceability requirements, the design
for adequate strength can then proceed.
Load balancing is widely used for the design of indeterminate members and also for simple
determinate beams and slabs. It is only strictly applicable, however, prior to cracking when
the member behaves linearly and the principle of superposition, on which load balancing
relies, is valid.
For the 300 mm thick, 12 m span one-way slab of Example 3.1, the prestress required to
balance the slab self-weight (7.2 kPa) is to be determined. The parabolic tendons have zero
eccentricity at each support and e=114 mm at mid-span.
With wb=7.2 kPa and e=0.114 m, Equation 3.11 gives
If at mid-span the time-dependent losses are 16% and the instantaneous losses are 8% (as was
stated in Example 3.1),
which corresponds to 1–4 strand flat ducted cable every 425 mm.
In Example 3.1, the tensile stress limit under full loads was F t=1.41 MPa. In this example,
the prestress is lower and Ft will therefore be exceeded. The bottom fibre elastic stress at mid-
span after all losses and under the full service loads is
which would almost certainly cause cracking. The resulting loss of stiffness must be included
in subsequent deflection calculations using the procedures outlined in Sections 3.5 and 3.6. In
addition, the smaller quantity of prestressing steel required in this example, in comparison
with the slab in Example 3.1, results in reduced flexural strength. A layer of non-prestressed
bottom reinforcement may be required to satisfy strength requirements.
3.4 Cable profiles
When the prestressing force and eccentricity are determined for the critical sections, the
location of the cable at every section along the member must be specified. For a member
which has been designed to be uncracked throughout, the tendons must be located so that the
stress limits are observed on every section. At any section, Equations 3.1–3.4 may be used to
establish a range of values for eccentricity which satisfy the selected stress limits.
If Mo and MT are the moments caused by the external loads at transfer and under full
service loads, respectively, and Pi and Pe are the corresponding prestressing forces at the same
section, the extreme fibre stresses must
satisfy the following:
Equations 3.12–3.15 can be rearranged to provide limits on the tendon eccentricity, as
It should be remembered that Fci and F c are negative numbers.
After Pi and P e have been determined at the critical sections, the friction losses along the
member are estimated (see Section 3.7.3) and the corresponding prestressing forces at
intermediate sections are calculated. At each intermediate section, the maximum eccentricity
that will satisfy both stress limits at transfer is obtained from either Equation 3.16 or 3.17. The
minimum eccentricity required to satisfy the tensile and compressive stress limits under full
loads is obtained from either Equation 3.18 or 3.19. A permissible zone is thus established in
which the line of action of the resulting prestressing force must be located. Such a permissible
zone is shown in Figure 3.5. Relatively few intermediate sections need to be considered to
determine an acceptable cable profile.
When the prestress and eccentricity at the critical sections are selected using the load-
balancing approach, the cable profile should match, as
Figure 3.5 Typical permissible zone for location of cable profile.
closely as practicable, the bending moment diagram caused by the balanced load. In this way,
deflection will be minimized. For cracked, partially prestressed members, Equations 3.16 and
3.17 are usually applicable and fix the maximum eccentricity. The cable profile should then
be selected according to the loading type and moment diagram.
3.5 Short-term analysis of cross-sections
3.5.1 Uncracked cross-sections
The short-term behaviour of a prestressed concrete cross-section can be determined by
transforming the bonded reinforcement into equivalent areas of concrete and performing a
simple, elastic analysis on the equivalent concrete section. The following mathematical
formulation of the short-term analysis of an uncracked cross-section forms the basis of the
time-dependent analysis described in Section 3.6 and was described by Gilbert (1988).
Consider a prestressed concrete cross-section with a vertical axis of symmetry. For a
section containing both non-prestressed and prestressed reinforcement, the transformed
section may be similar to that shown in Figure 3.6. The top surface of the cross-section, rather
than the centroidal axis, is selected here as the reference surface. This is a convenient
selection, but not a necessary one. The position of the centroidal axis of a prestressed concrete
cross-section varies with time owing to the gradual development of creep and shrinkage in the
concrete. The centroidal axis also depends on the quantity of bonded reinforcement and may
change position when unbonded tendons are subsequently grouted. It is convenient, therefore,
to select a fixed reference point that can be used in all stages of the analysis and, for this
reason, reference to any point on the cross-section in Figure 3.6 is made in terms of its
distance y from the top surface.
In Figure 3.6, the non-prestressed reinforcement is transformed into equivalent areas of
concrete (=AsE s/Ec=nA s), i.e. an additional area of concrete equal to (n− s is added to the
section at each bonded steel
Figure 3.6 Transformed section at transfer.
level, as shown; n is the short-term modular ratio (Es/Ec ). If the prestressed steel in Figure 3.6
is bonded to the concrete at transfer, it too should be transformed into an equivalent area of
concrete. Also shown in Figure 3.6 is the strain distribution on the section immediately after
transfer. The strain at a depth y below the top of the cross-section is defined in terms of the
top fibre strain ε and the initial curvature xi , as follows:
If the short-term behaviour of concrete is assumed to be linear-elastic, the initial concrete
stress at y below the top fibre is
The resultant axial force on the section Ni is obtained by integrating the stress block over the
depth of the section, as shown in Equation 3.22. For a prestressed section in pure bending, the
initial axial force on the transformed concrete section immediately after transfer is
compressive and equal in magnitude to the prestressing force, i.e. Ni=− i.P
where A (=∫ is the area of the transformed section and B (=∫ dA) is the first moment of
the transformed area about the top surface of the section.
If the first moment of the stress block about the top fibre is integrated
over the depth of the section, as shown in Equation 3.23, the resultant moment about the top
surface, Mi, is found. For a prestressed concrete beam section, Mi=Mo− idp, where Mo is the
external moment at the section at transfer and dp is the depth to the prestressing steel as shown
in Figure 3.6. Therefore,
where Ī y2 dA) is the second moment of the transformed area about the top surface of the
By rearranging Equations 3.22 and 3.23, expressions are obtained for the initial top fibre
strain and curvature in terms of Ni and Mi:
For any combination of external load and prestress, the corresponding values of Ni and Mi are
readily calculated and may be substituted into Equations 3.24 and 3.25 to obtain the strain
distribution immediately after transfer. Equations 3.24 and 3.25 may also be used to obtain the
increment of elastic strain due to the application of any subsequent load increment.
The short-term behaviour of the post-tensioned cross-section shown in Figure 3.7a is to be
determined immediately after transfer. The section contains a single unbonded cable
containing 10–12.7 mm diameter strands (Ap=1000 mm2 ) located within a 60 mm diameter
duct, and two layers of non-prestressed reinforcement, as shown. The force in the prestressing
steel is P i=1350 kN and the applied moment is Mo=100 kNm. The elastic moduli for concrete
and steel are E c=30×10 3 MPa and Es=Ep=200×10 3 MPa, and therefore n=6.67.
The transformed section is shown in Figure 3.7b. Because the prestressing steel is not
bonded to the concrete, it does not form part of the transformed
Figure 3.7 Post-tensioned cross-section of Example 3.3.
section. In addition, the hole created on the concrete section by the hollow duct must also be
taken into account. The properties of the transformed section with respect to the top reference
The axial force and moment about the top surface at transfer are
The top fibre strain and curvature immediately after transfer are obtained from Equations 3.24
Figure 3.8 Strains and stresses immediately after transfer (Example 3.3).
The concrete stresses are found using Equation 3.21. When y=0, the top fibre stress is
oi 0.76MPa, and when y=800 mm, the bottom fibre stress is σ=− bi 9.83 MPa. The stress in
the steel reinforcement is determined from the strain at the level of the steel. For the top layer
of non-prestressed reinforcement (at y=60 mm),
and for the bottom steel (at y=740 mm),
The distributions of strain and stress on the cross-section immediately after transfer are shown
in Figure 3.8.
3.5.2 Cracked cross-sections
When the tensile stress produced by the external moment at a particular section overcomes the
compression caused by prestress, and the extreme fibre stress reaches the tensile strength of
concrete, cracking occurs. The moment at which cracking first occurs is called the cracking
moment, Mcr. As the compressive force on the concrete gradually decreases with time due to
creep and shrinkage, the cracking moment also decreases with time. If the applied moment at
any time is greater than the cracking moment, cracking will occur and, at each crack, the
concrete below the neutral axis is ineffective. The short-term behaviour of the cracked cross-
section may be calculated approximately using a simple elastic analysis which is based on the
(a) Plane sections remain plane and therefore the strain distribution is linear over the depth of
(b) Perfect bond exists between the concrete and both the prestressed and non-prestressed
steel. At service loads, this is a reasonable assumption.
(c) Instantaneous material behaviour is linear-elastic. This includes the concrete in
compression, the conventional reinforcement and the prestressing steel. Once again, this is
a reasonable assumption at service loads.
(d) Short-term behaviour only is required, i.e. the analysis does not include the inelastic
effects of creep and shrinkage.
(e) Tensile stresses in the concrete are ignored. This is a conservative assumption. An
empirical adjustment to the second moment of area of the cracked section may be made to
account for the contribution of the tensile concrete to the stiffness of the cross-section. This
is the so-called tension stiffening effect.
The instantaneous strains and stresses on a cracked section are shown in Figure 3.9. For an
applied moment M greater than the cracking moment, there are two unknowns associated with
the strain diagram in Figure 3.9b: the depth to the neutral axis dn and the extreme fibre
instantaneous compressive strain ε. When ε and dn are known, the strain diagram is defined
and the concrete and steel stresses are readily determined. To find these two unknowns, there
are two equations of equilibrium. Horizontal equilibrium dictates that
and moment equilibrium requires that
where C, C s, Tp, and Ts may all be expressed as functions of dn and ε.
Figure 3.9 Cracked section analysis.
C is the volume of the triangular compressive stress block acting over the area A' above the
neutral axis. If A' is rectangular (b wide and dn deep), then
From similar triangles, the strains at the levels of the non-prestressed steel are
and therefore the forces in the conventional reinforcement are
The strain in the bonded prestressing steel is equal to the sum of three strain components. The
first component is the tensile strain caused by the effective prestress, ε, i.e. the strain that
exists in the steel prior to the application of any external moment:
Before the external moment is applied, the instantaneous compressive strain in the concrete at
the level of the prestressing steel is
As the external moment increases, the strain in the concrete at the steel level increases from
compressive (ε) to tensile (ε). If perfect bond exists between the tendon and the concrete,
the prestressing steel strain increases by this same amount, i.e. |ε|+ε. From similar triangles,
The total strain in the prestressed steel is therefore given by
and the force in the prestressing steel is
By substituting Equations 3.28, 3.29, 3.30, and 3.35 into Equations 3.26 and 3.27 and solving
the simultaneous equations, ε and dn are found. For manual solution, the following trial and
error procedure may be used:
(a) Select a reasonable value for ε (say
oi ). This will correspond to one particular
value of applied moment.
(b) Select a value for dn.
(c) Calculate strains, stresses, and forces in the steel and concrete.
(d) Check horizontal equilibrium. Is Equation 3.26 satisfied?
If yes: dn is correct.
If no: adjust dn and go to (c).
(e) When the correct value of dn has been determined, calculate the moment corresponding to
the initial selection of ε, using Equation 3.27.
The above procedure may be repeated for several values of ε to determine the change in
elastic behaviour as a function of moment. Behaviour at intermediate values of M may be
determined by interpolation.
From such an analysis, variations in steel stresses after cracking can be found in order to
check for crack control. Estimates of the section stiffness can also be made for use in
deflection calculations. It is noted that after cracking the neutral axis gradually rises as the
applied moment increases. With the area of concrete above the crack becoming smaller, the
second moment of area of the cracked section decreases as the applied moment increases.
This is not the case for reinforced concrete sections where dn remains approximately constant
with increasing moment and the cracked moment of inertia of the section is constant in the
In Figure 3.10, a typical moment-curvature diagram for a prestressed concrete section is
shown. At any moment M>Mcr, the curvature is
where E cIaυis the secant stiffness and e is the depth of the prestressing steel below the
centroidal axis of the cross-section. From Equation 3.36,
Figure 3.10 Typical moment-curvature diagram for a prestressed section.
A conservative estimate of deflection is obtained if the value of Ec Iaυfor the section of
maximum moment is taken as the flexural rigidity of the member.
The tangent stiffness Ec Icr is also shown in Figure 3.10. Icr is the second moment of area of
the cracked section, which may be obtained from a transformed section analysis. For small
variations in applied moment, curvature increments should be calculated using Icr. In
reinforced concrete construction, Icr is constant and equal to Iaυ but this is not so for
The cross-section analysed in Example 3.3 and shown in Figure 3.7 is to be re-analysed to
determine its post-cracking behaviour. It is assumed that the duct has been grouted, thereby
bonding the tendon to the surrounding concrete. The force in the prestressing steel at the time
of application of the external moment is P e=1200 kN. Material properties are as follows:
Sample calculations are provided for the particular applied moment that produces a top fibre
stress σ=− MPa, as shown in Figure 3.11.
When σ=− MPa, the instantaneous top fibre strain is
Figure 3.11 Short-term strain and stress on the cracked section of Example 3.4.
The area of the transformed cross-section prior to cracking and the second moment of area
about the centroidal axis are A=261×103 mm2 and I=14760×10 6 mm4, respectively. The
various strain components in the prestressing steel are obtained from Equations 3.31–3.33:
and from Equation 3.35,
Similarly from Equations 3.29 and 3.30:
The compression in the concrete above the neutral axis is obtained from Equation 3.28:
Trial values of dn are considered below:
dn Tp Ts ΣT C Cs ΣC Σ C
(mm) (kN) (kN) (kN) (kN) (kN) (kN) (kN)
460 1291 146 1437 1380 104 1484 –47
440 1299 164 1463 1320 104 1424 +39
FROM LINEAR INTERPOLATION
449 1295 155 1450 1347 104 1451 –1
With dn=449 mm when ε=−oi 667×10−, the moment and curvature on the section are obtained
from Equations 3.27 and 3.36, respectively.
The secant stiffness is obtained from Equation 3.37:
(cf. EcI=443×10 12 N mm2 for the uncracked section). The stresses in the prestressed and the
non-prestressed tensile steel under this applied moment are
The change in stress in the prestressing steel and the tensile stress in the non-prestressed steel
caused by the applied moment are much less than the tensile stress limits usually specified in
codes of practice for crack control.
Figure 3.12 Moment vs curvature for section of Example 3.4.
For example, AS 3600 (1988) specifies a maximum increment of tensile steel stress equal to
200 MPa between decomposition and the full in-service moment. With the closely spaced
bonded reinforcement near the tension face of the section analysed here, cracks should be well
controlled at this level of applied moment.
Similar calculations can be performed for other values of σ. For example,
When σ=− MPa:
When σ=− MPa:
A plot of the moment-curvature relationship for the section is shown in Figure 3.12.
3.6 Time-dependent analysis of cross-sections
The time-dependent behaviour of a partially prestressed member is greatly affected by the
quantity and location of conventional, non-prestressed reinforcement. Bonded reinforcement
provides restraint to the time-dependent shortening of concrete caused by creep and shrinkage.
As the concrete creeps and shrinks, the reinforcement is gradually compressed. An equal and
opposite tensile force Δ is applied to the concrete at the level of the bonded reinforcement,
thereby reducing the compression caused by prestress. It is the tensile forces that are applied
gradually at each level of bonded reinforcement which result in significant time-dependent
changes in curvature and deflection. An accurate estimate of these forces (Δ is essential if
reliable predictions of long-term behaviour are required.
Procedures specified in codes of practice for predicting losses of prestress due to creep and
shrinkage are usually too simplified to be reliable and often lead to significant error,
particularly for members containing non-prestressed reinforcement. In the following section, a
simple analytical technique is presented for estimating the time-dependent behaviour of a
general, partially prestressed cross-section. The procedure has been described in more detail
by Ghali and Favre (1986) and Gilbert (1988), and makes use of the age-adjusted effective
modulus method to model the effects of creep in concrete (see Equations 2.11–2.14 and the
3.6.2 Uncracked cross-sections
During any time period, creep and shrinkage strains develop in the concrete and relaxation
occurs in the prestressing steel. The gradual change in strain in the concrete with time causes
changes of stress in the bonded reinforcement. The gradual change in force in the steel is
opposed by an equal and opposite force on the concrete (usually tensile) at each steel location,
as shown in Figure 3.13. These forces are induced in the concrete at each level of bonded
reinforcement and result in increments of axial force Δ N(t) and moment about the top
reference surface Δ M(t) given by
Figure 3.13 Tinie-dependent actions and deformations.
where n is the number of layers of conventional, non-prestressed reinforcement and m is the
number of layers of bonded prestressed steel. Equal and opposite actions –Δ N(t) and –ΔM(t)
are applied to the bonded steel portions of the cross-section.
The time-dependent change of strain at any depth y below the top of the cross-section (Δ)
may be expressed in terms of the change in top fibre strain (Δ o) and the change of curvature
The magnitude of Δ is the sum of each of the following components:
(a) The free shrinkage strain ε (which is usually considered to be uniform over the section).
(b) The creep strain caused by the initial concrete stress σexisting at the beginning of the
time period, i.e. (from Equation 2.9), where is the increment of the creep
coefficient associated with the time period under consideration.
(c) The creep and elastic strain caused by Δ and Δ
N(t) M(t) gradually applied to the concrete
section. This term accounts for the internal restraint to creep and shrinkage provided by the
(d) The tensile creep strain in the high-strength prestressing steel (relaxation).
A convenient approach for the determination of the change of strain during any particular
time period (Δ o and Δ in Equation 3.40) involves a relaxation solution procedure first
proposed by Bresler and Selna (1964). During the time interval, the strain at any point on the
cross-section is initially assumed to remain unchanged, i.e. the change of strain due to creep
and shrinkage is artificially prevented. If the total strain is held constant and the creep and
shrinkage components change, then the instantaneous compo-
nent of strain must also change by an equal and opposite amount. As the instantaneous strain
changes, so too does the concrete stress. The concrete stress on the cross-section is therefore
allowed to vary due to relaxation. As a result, the internal actions change and equilibrium is
not maintained. To restore equilibrium, an axial force δ and a bending moment δ must be
applied to the section.
The forces required to restrain the section, −N and −M, are easily determined. If creep of
the concrete was not restrained by bonded reinforcement and the concrete stress remained
constant throughout the time period, the top fibre strain and curvature would increase by
and , respectively. The restraining forces required to prevent this deformation are
determined using expressions similar to Equation 3.22 and 3.23:
where A c, B c, and Īare the concrete area, the first moment of the concrete area and the second
moment of the concrete area about the top surface of the section, respectively. The properties
of the concrete section alone (without any contribution from the steel reinforcement) are used
in Equations 3.41 and 3.42 since only the concrete is subject to creep. The age-adjusted
effective modulus Ē (as defined in Equation 2.14) is used in Equations 3.41 and 3.42 because
the restraining forces δ and δ are gradually applied throughout the time period.
If shrinkage is uniform over the depth of the section and completely unrestrained, the
shrinkage-induced top fibre strain which develops during the time interval is ε and there is
no induced curvature. The restraining forces required to prevent this uniform deformation are
again obtained using expressions similar to Equations 3.22 and 3.23:
For a prestressed concrete section, restraining forces required to prevent the relaxation Rk in
each layer of tendons must also be included. The restraining forces required to prevent the
tensile creep (which causes relaxation) in the m layers of prestressing steel are
The total restraining forces are the sum of the creep, shrinkage, and relaxation components:
For a reinforced concrete section, the relaxation forces Rk in the above equations obviously do
The increments of top fibre strain (Δ o) and curvature (Δ produced by the axial force δ
ε x) N
and the moment δ gradually applied about the top reference level, may be obtained from
the following equations (which are similar to Equations 3.24 and 3.25):
where Ā is the area of the age-adjusted transformed section and and Īare the first and
second moments of the area of the age-adjusted transformed section about the top surface. For
the determination of Ā, , and Ī the age-adjusted effective modulus Ē is used instead of
e e, e
the elastic modulus for concrete E c in the calculation of the transformed area of the bonded
reinforcement. Ē is used in Equations 3.49 and 3.50 because δ and δ produce both elastic
e N M
and creep strains on the cross-section.
The loss of stress in the concrete at any distance y below the top fibre, which occurs while
the strain state is initially held constant (i.e. the initial stress relaxation), is given by
and the change of stress which occurs when δ and δ are applied to the section to restore
The actual change of concrete stress Δ that occurs during the time interval due to the effects
of creep, shrinkage, and relaxation is obtained by adding Equations 3.51 and 3.52:
For non-prestressed steel, the change of stress in the jth layer is
and, for the kth layer of prestressed steel, the change of stress is
The time-dependent behaviour of the cross-section shown in Figure 3.7 is to be determined.
The short-term behaviour of the section immediately after transfer was calculated in Example
3.3. The post-tensioned duct is filled with grout soon after transfer, thereby bonding the
tendon to the concrete and ensuring compatibility of concrete and steel strains throughout the
period of the time analysis. The material properties for the time period under consideration are
The strain and stress distributions immediately after transfer are shown in Figure 3.8, and for
It is assumed in this example that the external moment remains constant and equals 100 kNm
throughout the period of the time analysis.
From Equation 2.14,
and with the post-tensioning duct fully grouted, the properties of the concrete section are
The forces required to restrain the cross-section are determined using Equations 3.41–3.46:
The total restraining forces are obtained by summing the individual components using
Equations 3.47 and 3.48:
The age-adjusted modular ratio is and the age-adjusted transformed section
and its properties about the top reference surface are shown in Figure 3.14.
The increments of top fibre strain and curvature which develop during the
Figure 3.14 Age-adjusted transformed section and properties (Example 3.5).
time interval are obtained from Equations 3.49 and 3.50:
The final top fibre strain and curvature are therefore
The time-dependent changes of the top and bottom fibre concrete stresses are calculated using
and therefore the final concrete stresses are
From Equation 3.54, the change of stress in the non-prestressed steel is
and from Equation 3.55, the loss of stress in the prestressed steel is
Figure 3.15 Initial and final strains and stresses for Example 3.5.
The final steel stresses in each layer at time t are therefore
The initial and final strains and stress on the cross-section are illustrated in Figure 3.15.
The results of several time analyses on the cross-section shown in Figure 3.7 are presented in
Tables 3.1 and 3.2. The effects of varying the quantities of
Table 3.1 Effect of varying tensile steel As2 (As1=0).
κ(×10− Δ (×10−
Ms As1 εoi i Δ c1
T Δ c2
T Δ cp1
(×10− ) −
(mm2 ) 6 1 6 1
(kNm) mm ) (kN) (kN) (kN) mm )
0 −8.8 −0.455 0 0 206 −505 −0.629
100 1800 −28.9 −0.372 0 233 160 −673 +0.035
3600 −44.8 −0.306 0 337 135 −765 +0.402
0 −186 −0.008 0 0 174 −854 +0.221
270 1800 −198 +0.038 0 169 143 −970 +0.677
3600 −206 +0.075 0 248 125 −1034 +0.932
0 −364 +0.438 0 0 142 −1204 +1.071
440 1800 −366 +0.448 0 105 125 −1267 +1.319
3600 −368 +0.455 0 159 115 −1303 +1.463
Table 3.2 Effect of varying compressive steel As1 (As2 =1800 mm2).
κ(×10− Δ (×10−
Ms As1 εoi i Δ c1
T Δ c2
T Δ cp1
(kNm) (mm2) (×10−)6 −1
mm ) (kN) (kN) (kN) (×10− )
0 −28.9 −0.372 0 233 160 −673 +0.035
100 900 −25.4 −0.378 100 244 161 −544 −0.182
1800 −22.3 −0.383 170 253 161 −450 −0.339
0 −198 +0.038 0 169 143 −970 +0.677
270 900 −184 +0.014 136 186 143 −776 +0.353
1800 −172 −0.007 227 198 143 −639 +0.121
0 −366 +0.448 0 105 125 −1267 +1.319
440 900 −343 +0.407 172 127 125 −1009 +0.887
1800 −322 +0.370 285 143 126 −827 +0.581
the compressive and tensile non-prestressed reinforcement (As 1 and As2, respectively) on the
time-dependent deformation can be seen for three different values of sustained bending
moment. At M=100 kNm, the initial concrete stress distribution is approximately triangular
with higher compressive stresses in the bottom fibres (as determined in Examples 3.3 and 3.5).
At M=270 kNm, the initial concrete stress distribution is approximately uniform over the
depth of the section and the curvature is small. At M=440 kNm, the initial stress distribution
is again triangular with high compressive stresses in the top fibres.
From the results in Table 3.1, the effect of increasing the quantity of non-prestressed tensile
reinforcement, As2, is to increase the change in positive or sagging curvature with time. The
increase is most pronounced when the initial concrete compressive stress at the level of the
steel is high, i.e. when the sustained moment is low and the section is initially subjected to a
negative or hogging curvature. When A s2=3600 mm2 and M=100 kNm in Table 3.1, Δ is x
positive despite a large initial negative curvature. Table 3.1 indicates that the addition of non-
prestressed steel in the tensile zone will reduce the time-dependent camber which often causes
problems in precast members subjected to low sustained loads. For sections on which M is
sufficient to cause an initial positive curvature, an increase in A s2 causes an increase in time-
dependent curvature and hence an increase in final deflection (e.g. when M=440 kNm in
The inclusion of non-prestressed steel in the compressive zone, A s1, increases the change in
negative curvature with time, as indicated in Table 3.2. For sections where the initial
curvature is positive, such as when M=440 kNm, the inclusion of As1 reduces the time-
dependent change in curvature (and hence the deflection of the member). However, when x i is
negative, As1 causes an increase in negative curvature and hence an increase in the camber of
the member with time.
The significant unloading of the concrete with time on the sections containing non-
prestressed reinforcement should be noted. In Table 3.2, when M=270 kNm and A s1=1800
mm2, the concrete is subjected to a total gradually applied tensile force (Δ c1+Δ c2+Δ cp1) of
T T T
568 kN. More than 42% of the initial compression in the concrete is shed into the bonded
reinforcement with time. The loss of prestress in the tendon, however, is only 143 kN (10.6%).
It is evident that an accurate picture of the time-dependent behaviour of a partially prestressed
section cannot be obtained unless the restraint provided to creep and shrinkage by the non-
prestressed steel is adequately accounted for. It is also evident that the presence of non-
prestressed reinforcement significantly reduces the cracking moment with time and may in
fact relieve the concrete of much of its initial prestress.
3.6.3 Cracked cross-sections
Under sustained loading, creep causes a change in position of the neutral axis on a cracked
cross-section. In general, the depth to the neutral axis increases with time and, hence, so too
does the area of concrete in compression. An iterative numerical solution procedure is
required to account accurately for this gradual change in the properties of the cracked section
with time. The time period is divided into small intervals and structural behaviour is
calculated at the end of each time increment. The properties of the cross-section are modified
or updated at the end of each time increment. Such a procedure is not suitable for manual
solution and is often too complex for routine use in structural analysis and design.
The procedure described in the previous section for the time analysis of uncracked cross-
sections can be extended to cracked sections, if it is assumed that the cross-sectional area of
the section remains constant with time, that is, if the depth of the concrete above the neutral
axis (dn in Figure 3.16a) is assumed to remain constant throughout the time analysis. This
assumption is in fact necessary if the short-term and time-dependent stress and strain
increments are to be calculated separately and added together to obtain final stresses and
deformations, i.e. if the principle of superposition is to be applied to fully cracked sections in
the same way as it has been applied to uncracked cross-sections. The assumption also greatly
simplifies the analysis and usually results in relatively little error.
Consider a fully cracked cross-section subjected to a sustained bending moment M, as
shown in Figure 3.16a. The short-term and time-dependent strain distributions are illustrated
in Figure 3.16b.
The restraining actions, − N and −M, that are required to prevent the free development of
creep and shrinkage in the concrete and relaxation in the bonded prestressing tendons are
calculated using Equations 3.47 and
Figure 3.16 Time-dependent behaviour of a fully cracked cross-section.
3.48. For a fully cracked cross-section, the terms A c, Bc , and Īin these equations are the
properties of the uncracked part of the concrete cross-section with respect to the top fibre. The
depth of the uncracked concrete dn is calculated from the short-term analysis presented in
The change of the strain distribution with time is calculated using Equations 3.49 and 3.50
and Ā e, , and Īare now the properties of the fully cracked age-adjusted transformed
section, i.e. the properties of the cross-section consisting of the concrete compressive zone
and a transformed area of (or ) at each bonded steel level, where
The change of concrete stress with time at any depth may be determined using
Equations 3.51–3.53 and the change of stress in the jth layer of non-prestressed reinforcement
and in the kth layer of prestressing steel may be found from Equations 3.54 and 3.55,
The change of stress and strain with time on the cross-section shown in Figure 3.17a is to be
determined. The sustained bending moment is M=700 kNm and the initial prestressing force
is P=1350 kN.
The material properties for the time period under consideration are:
The depth of the neutral axis immediately after the application of the applied moment M is
calculated using the iterative short-term analysis outlined in Section 3.5.2. In this example,
Figure 3.17 Cross-sectional details and initial strains (Example 3.6).
(as shown in Figure 3.17b). The initial top fibre strain and curvature are
oi 671×10− and x i=1.415×10− mm−, respectively.
6 6 1
The cracked cross-section and the strain distribution immediately after the application of M
are shown in Figures 3.17b and c.
The age-adjusted effective modulus is obtained from Equation 2.14:
and the properties of the uncracked part of the concrete cross-section (i.e. the concrete
compressive zone) with respect to the top fibre are
From Equations 3.47 and 3.48,
With the areas of the bonded steel reinforcement transformed into equivalent areas of concrete
of modulus Ē, the properties of the age-adjusted transformed section are
The time-dependent increments of top fibre strain and curvature produced by δ and δ are
found using Equations 3.49 and 3.50:
The change of stress in the concrete compression zone is obtained from Equations 3.51–3.53:
At y=474 mm:
and from Equations 3.54 and 3.55, the change of stress in the steel is
The final stresses and strains are illustrated in Figure 3.18.
There is a relatively small time-dependent change of stress in the prestressing steel on this
cracked cross-section. If the concrete surrounding a bonded prestressing tendon is cracked
under the sustained load, the loss of steel stress due to creep and shrinkage of the concrete is
generally small. Most practical, partially prestressed concrete members are designed to
Figure 3.18 Stresses and strains on cross-section of Example 3.6.
remain uncracked under the sustained or permanent in-service loads. Cracking occurs under
the application of the variable live loads. Cracks therefore open and close as the variable live
load is applied and removed. For most of the life of such members, the entire concrete cross-
section is in compression (uncracked) and the time analysis for a general uncracked cross-
section, as outlined in Section 3.6.2, is appropriate.
3.7 Losses of prestress
The losses of prestress that occur in a prestressed member are illustrated in Figure 3.19. When
the prestress is transferred to the concrete, immediate losses of prestress occur. The difference
between the prestressing force imposed at the jack, Pj, and the force in the steel immediately
after transfer at a particular section, Pi, is the immediate loss:
The gradual loss of prestress that takes place with time is called the time-dependent or
deferred loss. If Pe is the force in the prestressing tendon after all losses, then
Both of these losses are made up of several components. The immediate losses are caused by
elastic deformation of the concrete as the prestress is
Figure 3.19 Losses of prestress.
transferred, friction along the draped tendon in a post-tensioned member, and slip at the
anchorage. Other sources of immediate loss of prestress which may need to be accounted for
in some situations include deformation of the forms of precast members, temperature changes
between the time of stressing the tendons and casting the concrete, deformation in the joints
of precast members assembled in sections, and relaxation of the tendons prior to transfer. The
time-dependent losses are caused by the gradual shortening of the concrete at the steel level
due to creep and shrinkage, and by relaxation of the steel itself. Additional losses may occur
due to time-dependent deformation of the joints in segmental construction.
3.7.2 Elastic deformation losses
Immediately after transfer, the change in strain in the prestressing steel Δp caused by elastic
shortening of the concrete is equal to the strain in the concrete at the steel level, ε . The
compatibility equation can be expressed as follows:
The loss of stress in the steel, Δ p, is therefore
where σ is the concrete stress at the steel level immediately after transfer.
For post-tensioned members with one cable or with two or more cables stressed
simultaneously, the elastic deformation of the concrete occurs during the stressing operation
before the tendons are anchored. In this case, elastic shortening losses are zero. In a member
containing more than one tendon and where the tendons are stressed sequentially, the elastic
deformation losses vary from tendon to tendon and are a maximum in the tendon
stressed first and a minimum (zero) in the tendon stressed last. It is relatively simple to
calculate the elastic deformation losses in any tendon provided the stressing sequence is
known. However, these losses are usually small and, for practical purposes, the average
elastic shortening loss is often taken as half the value obtained from Equation 3.58:
3.7.3 Friction along the tendon
Friction occurs in the jack and anchorage and depends on the type of jack and anchorage
system used. This loss is usually allowed for during stressing and need not unduly concern the
In post-tensioned members, friction losses occur along the tendon during the stressing
operation. Friction between the tendon and the duct causes a gradual reduction in prestress
with the distance along the tendon Lpa from the jacking end. The magnitude of the friction loss
depends on the total angular change of the tendon, the distance from the jacking point and the
size and type of the sheathing containing the tendons. A reliable estimate of friction losses
may be obtained from Equation 3.60. An equation of similar form is recommended by
numerous building codes, including ACI 318–83, BS 8110 (1985), and AS 3600–1988.
Pa is the force in the tendon at any point Lpa (in metres) from the jacking end.
Pj is the force in the tendon at the jacking end.
µ is a friction curvature coefficient which depends on the type of duct. For strand in bright and zinc-
coated metal ducts, µ≈ for greased and wrapped wire or strand, µ≈
0.2; 0.15; and for strand in an
unlined concrete duct, µ≈ 0.50. Higher values should be used if either the tendon or the duct are
a t is the sum in radians of the absolute values of all successive angular deviations of the tendon over
the length Lpa.
β is an angular deviation or wobble term and depends on the sheath (or duct) diameter:
For ducts containing strand and having an internal diameter as follows:
For flat metal ducts:
For greased and wrapped bars: β=0.008.
The friction losses in the cable in the end-span of the post-tensioned girder of Figure 3.20 are
to be calculated. For this cable, µ=0.2 and β=0.01.
From Equation 3.60:
Figure 3.20 Tendon profile for end span of Example 3.7.
3.7.4 Anchorage losses
In post-tensioned members, some slip or draw-in occurs when the prestressing force is
transferred from the jack to the anchorage. This causes an additional loss of prestress. The
amount of slip depends on the type of anchorage. For wedge-type anchorages for strand, the
slip Δmay be as high as 6 mm. The loss of prestress caused by Δdecreases with distance
from the anchorage owing to friction and may be negligible at the critical design section.
However, for short tendons, this loss may be significant and should not be ignored in design.
The loss of tension in the tendon caused by slip is opposed by friction in the same way as
the initial prestressing force was opposed by friction, but in the opposite direction, i.e. µ and
β are the same. The graph of variation in prestressing force along a member due to friction
(calculated using Equation 3.60) is modified in the vicinity of the anchorage by the mirror
image reduction shown in Figure 3.21. The slope of the draw-in line adjacent to the anchorage
has the same magnitude as the friction loss line but the opposite sign.
Figure 3.21 Variation in prestress due to draw-in at the anchorage.
In order to calculate the draw-in loss at the anchorage δ di, the length of the draw-in line Ldi
must be determined. By equating the anchorage slip Δwith the integral of the change in strain
in the steel tendon over the length of the draw-in line, Ldi may be determined. From Figure
3.21b, the loss of prestress due to draw-in δ at distance x from point O is
where α twice the slope of the prestress line as shown in Figure 3.21. Therefore,
The magnitude of the slip that should be anticipated in design is usually supplied by the
anchorage manufacturer and should be checked on site. Cautious overstressing at the
anchorage is often an effective means of compensating for slip.
3.7.5 Time-dependent losses of prestress
In Section 3.6, a time analysis was presented for determining the effects of creep, shrinkage,
and relaxation on the behaviour of a prestressed concrete
beam section of any shape and containing any layout of prestressed and non-prestressed
reinforcement. In this section, the approximate procedures which are often specified in codes
of practice for calculating time-dependent losses of prestress are outlined. These methods are
of limited value and often give misleading results because they do not adequately account for
the significant loss of precompression in the concrete that occurs when non-prestressed
reinforcement is present. For a realistic estimate of the time-dependent behaviour of a
prestressed section, the method described in Section 3.6 is recommended.
The loss of stress in a tendon due to shrinkage of concrete may be approximated by
where ε is the shrinkage strain at the time under consideration and may be estimated using
the procedures outlined in Section 2.5. When non-prestressed reinforcement is present and
offers restraint to shrinkage, the stress loss in the tendon will be smaller than that indicated by
Equation 3.62. However, the non-prestressed reinforcement also relieves the concrete of
compression, and the change in the resultant compression in the concrete may be much
greater than the change in tensile force in the tendon. As time increases, more and more of the
compression exerted on the beam by the tendon is carried by the non-prestressed steel and less
and less by the concrete.
Creep strain in the concrete at the level of the tendon depends on the stress in the concrete at
that level. Because the concrete stress varies with time, a reliable estimate of creep losses
requires a detailed time analysis (such as that presented in Section 3.6). An approximate and
conservative estimate can be made by assuming that the concrete stress at the tendon level
remains constant with time and equal to its initial (usually high) value, σ(caused by Pi and
the permanent part of the load). With this assumption, the creep strain at any time t after
transfer (at age ) may be calculated from an expression similar to Equation 2.9):
where is the creep coefficient, which may be estimated using the procedures outlined
in Section 2.5.
If the tendon is bonded to the surrounding concrete, the change of steel
strain caused by creep is equal to ε and the creep loss in the tendon may be approximated
Again, the presence of conventional steel will cause a decrease in the concrete compressive
stress at the steel level and a consequent decrease in creep. In this case, Equation 3.64 will
overestimate creep losses, often significantly.
Relaxation of steel
The loss of stress in a tendon due to relaxation depends on the sustained stress in the steel.
Owing to creep and shrinkage in the concrete, the stress in the tendon decreases with time at a
faster rate than would occur due to relaxation alone. This decrease in stress level in the tendon
affects (reduces) the magnitude of the relaxation losses. An equation similar to Equation 3.65
is often used to modify the design relaxation to include the effects of creep and shrinkage.
The loss of prestress due to relaxation (as a percentage of the initial prestress) may be
where R is the design relaxation, which may be obtained from either Equation 2.22 or 2.23;
Δ p is the loss of stress in the tendon due to creep plus shrinkage (from Equations 3.62 and
3.64); and σ is the stress in the tendon immediately after transfer.
3.8 Deflection calculations
The slope θ deflection υ any point x along a member may be calculated by integrating
the curvature over the length of the member. Provided that deformations are small
compared with the beam dimensions, simple beam theory gives
These equations are general and apply for both elastic and inelastic material
Figure 3.22 Deformation of a typical span and cantilever.
behaviour. For a prestressed concrete beam, the curvature at any point along the span at any
time after first loading can be calculated using the procedures outlined in Sections 3.5 and 3.6.
Consider the span shown in Figure 3.22a. If the curvature at each end of the span (xA and
x B) and at mid-span (xC ) are known and the variation in curvature along the member is
parabolic, then the slope at each support (θ and θ) and the deflection at mid-span (υ) are
A B C
Similarly, if the variation of curvature along a fixed-end cantilever (such as shown in Figure
3.22b) is parabolic, the slope and deflection at the free end are given by
If only the curvatures at each end of the cantilever are known, then
For practical members subjected to usual load configurations, deflection estimates made using
Equations 3.68–3.70 are accurate enough for most design purposes, even where the variation
of curvature along the member is not parabolic.
3.8.2 Short-term deflection
For any uncracked cross-section, the initial curvature may be calculated using Equation 3.25.
A typical numerical example was illustrated in Example 3.3. For a cracked cross-section, the
initial curvature may be found from Equation 3.36 using the procedure presented in Section
3.5.2 and illustrated in Example 3.4. If the initial curvature at each end of the span of a beam
or slab and at the mid-span are calculated, the short-term deflection can be estimated using
Equations 3.68c, 3.69b or 3.70b, whichever is appropriate.
For uncracked, prestressed concrete members, codes of practice generally suggest that the
gross moment of inertia Ig may be used in deflection calculations. The initial curvature at any
cross-section may therefore be approximated by
where P i is the initial prestressing force and e is its eccentricity below the centroidal axis of
After cracking, the stiffness of the cracked cross-section calculated using Equation 3.37
may underestimate the stiffness of the member in the cracked region. The intact concrete
between adjacent cracks carries tensile force, mainly in the direction of the reinforcement, due
to the bond between the steel and the concrete. The average tensile stress in the concrete is
therefore not zero and may be a significant fraction of the tensile strength of concrete. The
stiffening effect of the uncracked tensile concrete is sensibly known as tension stiffening and
is usually accounted for in design by an empirical adjustment to the stiffness of the fully
For conventionally reinforced members, tension stiffening contributes significantly to the
member stiffness, particularly when the maximum moment is not much greater than the
cracking moment. However, as the moment level increases, the tension stiffening effect
decreases owing to additional secondary cracking at the level of the bonded reinforcement.
Shrinkage-induced cracking and tensile creep cause a reduction of the tension stiffening effect
with time. Repeated or cyclic loading also causes a gradual breakdown of tension stiffening.
For a partially prestressed member (or a reinforced member subjected to significant axial
compression), the effect of tension stiffening is less pro-
nounced because the loss of stiffness due to cracking is more gradual and significantly smaller.
In codes of practice, the simplified techniques specified for estimating the deflection of a
cracked concrete member usually involve the determination of an effective moment of inertia
Ie for the member. A number of empirical equations are available for Ie . Most have been
developed specifically for reinforced concrete, where for a cracked member Ie lies between
the gross moment of inertia of the critical section Ig and the moment of inertia of the cracked
transformed section Icr. For a prestressed concrete section, Icr varies with the applied moment
as the depth of the crack gradually changes. The value of Icr is usually considerably less than
Iav, as illustrated in Figure 3.10. The equations used for estimating Ie for a reinforced section
are not therefore directly applicable to prestressed concrete.
The following two well known procedures for modelling tension stiffening may be applied
to prestressed concrete provided Iav replaces Icr in the original formulations:
(a) The empirical equation for Ie proposed by Branson (1963) is perhaps the best known
method and has been adopted in many codes and specifications for reinforced concrete
members, including ACI 318–83 and AS 3600–1988. For a prestressed concrete section,
the following form of the equation can be used:
where Mc is the moment required to cause first cracking and M is the maximum in-
service moment at the section under consideration.
(b) The CEB (1983) has proposed an alternative approach for reinforced concrete which
accounts for the effect of the reinforcement type on tension stiffening and also accounts for
the breakdown of tension stiffening with time due to shrinkage induced tension, tensile
creep, and repeated loading. The CEB proposal may be modified for cracked, prestressed
sections as follows:
1 when deformed non-prestressed bars are present;
=0.5 when plain round bars or bonded tendons only are present;
=0.0 when unbonded tendons only are present;
2 for initial loading;
=0.5 for long-term sustained loads or cycles of load.
Numerous other approaches have been developed for modelling the tension stiffening
phenomenon. Of the two approaches outlined above, the CEB approach is recommended
because it best accounts for the breakdown of tension stiffening under long-term or cyclic
loading and allows for the reduction in tension stiffening when plain bars or bonded tendons
only are present and the steel-concrete bond might not be perfect.
For most practical prestressed or partially prestressed members, however, tension stiffening
is not very significant and a reasonable, conservative estimate of deflection can be obtained
by ignoring tension stiffening and using Ec Iav (from Equation 3.37) in the calculations.
The short-term deflection of a uniformly loaded, simply supported, post-tensioned beam of
span 12m is to be calculated. An elevation of the member is shown in Figure 3.23, together
with details of the cross-section at mid-span (which is identical with that analysed in Example
Figure 3.23 Beam details for Example 3.8.
prestressing cable is parabolic with the depth of the tendon below the top fibre at each support
dp=400 mm and at mid-span dp=600 mm, as shown. The non-prestressed reinforcement is
constant throughout the span. Owing to friction and draw-in losses, the prestressing force at
the left support is P=1300 kN, at mid-span P=1300 kN, and at the right support P=1250 kN,
as shown in Figure 3.23c. The tendon has previously been bonded to the surrounding concrete
by filling the duct with grout.
Two service load cases are to be considered:
(a) a uniformly distributed load of 6 kN/m (which is the self-weight of the member);
(b) a uniformly distributed load of 36 kN/m.
The material properties are
and the flexural tensile strength is taken to be MPa.
At support A The applied moment is zero for both load cases and the prestressing tendon
is located at the mid-depth of the section (dp=400 mm) with a prestressing force P=1300 kN.
Using the cross-sectional analysis described in Section 3.5.1, the initial top fibre strain and
curvature calculated using Equations 3.24 and 3.25 are
At support B The prestressing force is P=1250 kN at dp=400 mm and M=0. As calculated at
support A, the initial top fibre strain and curvature are
At mid-span C The prestressing force is P=1300 kN at a depth of dp=600 mm. For load case
The cross-section is uncracked and from Equations 3.24 and 3.25
for load case (b),
The section at mid-span is cracked and, using the iterative procedure outlined in Section 3.5.2,
the depth to the neutral axis is dn=495 mm. The initial top fibre strain and curvature are
The value of Iav calculated from Equation 3.37 is
Deflection With the initial curvature calculated at each end of the member and at mid-span,
the short-term deflection for each load case is determined using Equation 3.68c. For load case
For load case (b),
For load case (b), tension stiffening in the cracked region of the member near mid-span was
ignored. To include tension stiffening, the moment required to cause first cracking (i.e. the
moment required to produce a bottom fibre tensile stress of 3.8 MPa) is required. From an
analysis of the uncracked transformed section, the cracking moment Mcr is 579 kN m. Using
the procedure specified by the CEB (1983) for calculating Ie, the β coefficients are β=1.0 and
β=0.5 (assuming the member is subjected to load repetitions) and from Equations 3.74 and
The revised curvature at mid-span for load case (b) is
and the revised mid-span deflection for load case (b) is
3.8.3 Long-term deflection
Long-term deflections due to concrete creep and shrinkage are affected by many variables,
including load intensity, mix proportions, member size, age at first loading, curing conditions,
total quantity of compressive and tensile steel, level of prestress, relative humidity, and
temperature. To account accurately for these parameters, a time analysis similar to that
described in Sections 3.6.2 and 3.6.3 is required. The change in curvature during any period
of sustained load may be calculated using Equation 3.50. Typical calculations are illustrated
in Example 3.5 for an uncracked cross-section and in Example 3.6 for a cracked cross-section.
When the final curvature has been determined at each end of the member and at mid-span,
the long-term deflection can be calculated using either Equations 3.68c, 3.69b, or 3.70b.
For reinforced concrete members, codes of practice offer simple approximate methods for
obtaining ball-park estimates of long-term deflection. The long-term deflection is often taken
to be equal to the short-term deflection due to the sustained or permanent loads times a
multiplication factor. For example, the long-term deflection multiplication factor specified in
ACI 318–83 for the long-term deflection after 5 years under load is
where ρis the non-prestressed compressive reinforcement ratio (Asc/bd) at the mid-span for
simple and continuous spans and at the support for cantilevers.
In prestressed concrete construction, a large proportion of the sustained external load is
often balanced by the transverse force exerted by the tendons. Under this balanced load, the
short-term deflection may be zero, but the long-term deflection is not. The restraint to creep
and shrinkage offered by non-symmetrically placed, bonded reinforcement on a section can
significant time-dependent curvature and, hence, significant deflection of the member. The
use of a simple deflection multiplier to calculate long-term deflection from the short-term
deflection is therefore not satisfactory.
In this section, approximate procedures are presented which allow a rough estimate of long-
term deflection. In some situations, this is all that is required. However, for most applications,
the procedures in Sections 3.6.2 and 3.6.3 are recommended.
The final creep induced deflection may be approximated by
where υ is the short-term deflection produced by the sustained portion of the unbalanced
load and is the final creep coefficient. If a beam initially hogs upward under sustained
loads (i.e. υ is upward), in general it will continue to hog upwards with time and υ will
also be upward.
As seen in Section 2.5, the final creep coefficient varies from about 2.0 to 4.0, the upper
end of the range for low to medium strength concrete loaded at early ages and located in a
relatively dry environment. For prestressed concrete beams of average size, with Mpa,
exposed to the open air and initially loaded at ages greater than 7 days, is typically about
The factor α Equation 3.76 depends on the extent of cracking and the reinforcement
quantity (Gilbert 1983) and may vary from 1.0 to about 3.5. For uncracked, lightly reinforced
prestressed members, such as slabs, the increase in curvature due to creep is nearly
proportional to the increase in strain due to creep and α little more than 1.0. For more
heavily reinforced, uncracked members α may be taken as 1.5. For cracked, partially
prestressed members, α usually about 2.5. For members containing compression steel, Asc,
the creep deflection, is significantly smaller. This may be taken into account by multiplying α
by the factor 1+Asc/As, where As is the total area of steel in the tension zone.
The deflection caused by shrinkage warping may be approximated by
where is the shrinkage induced curvature at mid-span (or at the support of a cantilever); L
is the beam span and β depends on the support conditions:
β=0.50 for a cantilever;
β=0.125 for a simply supported member;
β=0.090 for an end span of a continuous beam;
β=0.065 for an interior span of a continuous beam.
is greater than zero for a non-symmetric steel layout and varies along the span as the
eccentricity of the bonded tendon and the layout of non-prestressed steel varies. For
uncracked prestressed members with small quantities of tensile reinforcement, an approximate
estimate of the final shrinkage curvature is
For cracked, partially prestressed members, with significant quantities of conventional
reinforcement, the final shrinkage curvature is significantly higher and may be approximated
For members containing compressive reinforcement, shrinkage deflection is significantly
lower and may be accounted for by multiplying by 1− sc/As.
The final time-dependent deflection of the beam described in Example 3.8 and illustrated in
Figure 3.23 is to be calculated. As in Example 3.8, two load cases are to be considered:
(a) a uniformly distributed constant sustained load of 6 kN/m;
(b) a uniformly distributed constant sustained load of 36 kN/m.
For each load case, the time-dependent material properties are
All other material properties are as specified in Example 3.8.
At support A The sustained moment at A is zero for both load cases and the initial
prestress is P=1300 kN at dp 400 mm. The time-dependent changes of top fibre strain and
curvature calculated using Equations 3.49 and 3.50 are
The final top fibre strain and curvature are
At support B As for support A, the sustained moment is zero, but the initial prestress is
P=1250 kN. Equations 3.49 and 3.50 give
At mid-span For load case (a), M=108 kNm and P=1300 kN at dp=600 mm. For this
For load case (b), the sustained moment is M=648 kNm and for the cracked cross-section,
Equations 3.49 and 3.50 give
Deflection With the final curvature calculated at each end of the member and at mid-span, the
long-term deflection at mid-span for each load case is found using Equation 3.68c. For load
For load case (b),
Consider the more approximate predictions made using Equations 3.76–3.79. The creep
induced deflection is estimated using Equation 3.76. For load case (a), the member is
uncracked with significant quantities of
non-prestressed steel. The factor α taken to be
From Example 3.8, υ =− mm and with
sus 4.6 , Equation 3.76 gives
For load case (b), the cross-section at mid-span is cracked and the factor α taken as
From Example 3.8, υ =18.5 mm and therefore
For load case (a), the shrinkage induced curvature is given by Equation 3.78:
and from Equation 3.77,
For load case (b), Equations 3.79 and 3.77 give, respectively,
The final long-term deflection for each load case is the sum of the initial deflection and the
creep and shrinkage deflection increments.
For load case (a),
(cf. υ 5.8 mm from the more accurate approach).
For load case (b),
which is almost 30% smaller than the estimate made using the more accurate procedure.
ACI 318–83 1983. Building code requirements for reinforced concrete. Detroit: American Concrete
AS 1481–1978. SAA prestressed concrete code. Sydney: Standards Association of Australia.
AS 3600–1988. Australian standard for concrete structures. Sydney: Standards Association of
Bazant, Z.P. 1972. Prediction of concrete creep effects using age-adjusted effective modulus method.
ACI Journal 69, 212–17.
Branson, D.E. 1963. Instantaneous and time-dependent deflection of simple and continuous reinforced
concrete beams. Alabama Highway Research Report, No. 7. Alabama: Bureau of Public Roads.
Bresler, B. & L.Selna 1964. Analysis of time dependent behaviour of reinforced concrete structures.
Symposium on Creep of Concrete, ACI Special Publication SP-9, Detroit, American Concrete
Institute, pp. 115–28.
Comité Euro-International du Béton (CEB) 1983. Fissuration et deformations. Manuel du CEB.
Lausanne: Ecole Polytechnique Fédérale de Lausanne.
Ghali, A. & M.K.Tadros 1985. Partially prestressed concrete structures. Journal of Structural
Engineering, ASCE 111, 1846–65.
Ghali, A. & R.Favre 1986. Concrete structures: stresses and deformations. London: Chapman and
Gilbert, R.I. 1983. Deflection calculations for reinforced concrete beams, Civil Engineering
Transactions, Institution of Engineers, Australia CE25, 128–34.
Gilbert, R.I. 1986. Prestress losses in partially-prestressed concrete beams. Proceedings of the 10th
Australasian Conference on the Mechanics of Structures and Materials, Adelaide, University of
Adelaide, South Australia, pp. 409–16.
Gilbert, R.I. 1988. Time effects in concrete structures. Amsterdam: Elsevier.
Khachaturian, N. & G.Gurfinkel 1969. Prestressed concrete. New York: McGraw-Hill.
Lin, T.Y. 1963. Prestressed concrete structures. New York: Wiley.
Magnel, G. 1954. Prestressed concrete, 3rd edition. London: Concrete Publications Ltd.
Neville, A.M., W.H.Dilger & J.J.Brooks 1983. Creep of plain and structural concrete. London:
Warner, R.F. & K.A.Faulkes 1979. Prestressed concrete. Melbourne: Pitman Australia.
Ultimate flexural strength
The single most important design objective for a structure or a component of a structure is the
provision of adequate strength. The consequences and costs of strength failures are large and
therefore the probability of such failures must be very small.
The satisfaction of concrete and steel stress limits at service loads does not necessarily
ensure adequate strength and does not provide a reliable indication of either the actual
strength or the safety of a structural member. It is important to consider the non-linear
behaviour of the member in the over-loaded range to ensure that it has an adequate structural
capacity. Only by calculating the ultimate capacity of a member can a sufficient margin
between the service load and the ultimate load be guaranteed.
In the 1950s and 1960s, there was a gradual swing away from the use of elastic stress
calculations for the satisfaction of the design objective of adequate strength. The so-called
ultimate strength design approach emerged as the most appropriate procedure. The ultimate
strength of a cross-section in bending Mu is calculated from a rational and well established
flexural strength theory, which involves consideration of the strength of both the concrete and
the steel in the compressive and tensile parts of the cross-section. The prediction of ultimate
flexural strength is described and illustrated in this chapter. When Mu is determined, the
design requirements for the strength limit state (as discussed in Section 1.7.6) may be checked
In addition to calculating the strength of a section, a measure of the ductility of each section
must also be established. Ductility is an important objective in structural design. Ductile
members undergo large deformations prior to failure, thereby providing warning of failure
and allowing indeterminate structures to establish alternative load paths. In fact, it is only with
adequate ductility that the predicted strength of indeterminate members and structures can be
achieved in practice.
4.2 Flexural behaviour at overloads
The load at which collapse of a flexural member occurs is called the ultimate load. If the
member has sustained large deformations prior to collapse, it is said to have ductile behaviour.
If, on the other hand, it has only undergone small deformations prior to failure, the member is
said to have brittle behaviour. There is no defined deformation or curvature which
distinguishes ductile from brittle behaviour. Codes of practice, however, usually impose a
ductility requirement by limiting the curvature at ultimate to some minimum value, thereby
ensuring that significant deformation occurs in a flexural member prior to failure. Since beam
failures that result from a breakdown of bond between the concrete and the steel
reinforcement, or from excessive shear, or from failure of the anchorage zone tend to be
brittle in nature, every attempt should be made to ensure that the region of maximum moment
is the weakest link. The design philosophy should ensure therefore that a member does not fail
before the required design moment capacity of the section is attained.
Consider the prestressed concrete cross-section shown in Figure 4.1. The section contains
non-prestressed reinforcement in the compressive and tensile zones and bonded tensile
prestressing steel. Also shown in Figure 4.1 are typical strain and stress distributions for four
different values of applied
Figure 4.1 Stress and strain distributions caused by increasing moment.
moment. As the applied moment M increases from typical in-service levels into the overload
range, the neutral axis gradually rises and eventually material behaviour becomes non-linear.
The non-prestressed steel may yield if the strain ε exceeds the yield strain (ε y/Es), the
prestressed steel may enter the non-linear part of its stress-strain curve as εincreases, and the
concrete compressive stress distribution becomes non-linear when the extreme fibre stress
exceeds about .
A flexural member which is designed to exhibit ductility at failure usually has failure of the
critical section preceded by yielding of the bonded tensile steel, i.e. by effectively exhausting
the capacity of the tensile steel to carry any additional force. Such a member is said to be
under-reinforced. Because the stress-strain curve for the prestressing steel has no distinct yield
point and the stress increases monotonically as the strain increases (see Figure 2.13), the
capacity of the prestressing steel to carry additional force is never entirely used up until the
steel actually fractures. However, when the steel strain εexceeds about 0.01 (for wire or
strand), the stress–strain curve becomes relatively flat and the rate of increase of stress with
strain is small. After yielding, the resultant internal tensile force, T(=T s+Tp) in Figure 4.1,
remains approximately constant (as does the resultant internal compressive force C, which is
equal and opposite to T). The moment capacity can be further increased by an increase in the
lever arm between C and T. Under increasing deformation, the neutral axis rises, the
compressive zone becomes smaller and smaller and the compressive concrete stress increases.
Eventually, perhaps after considerable deformation, a compressive failure of the concrete
above the neutral axis occurs and the section reaches its ultimate capacity. It is, however, the
strength of the prestressing tendons and the non-prestressed reinforcement in the tensile zone
that control the strength of a ductile section. In fact, the difference between the moment at
first yielding of the tensile steel and the ultimate moment is usually small.
A flexural member which is over-reinforced, on the other hand, does not have significant
ductility at failure and fails without the prestressed or non-prestressed tensile reinforcement
reaching any form of yield. At the ultimate load condition, both the tensile strain at the steel
level and the section curvature are relatively small and, consequently, there is little
deformation or warning of failure.
Because it is the deformation at failure that defines ductility, it is both usual and reasonable
in design to define a minimum ultimate curvature to ensure the ductility of a cross-section.
This is often achieved by placing a maximum limit on the depth to the neutral axis at the
ultimate load condition. Ductility can be increased by the inclusion of non-prestressed
reinforcing steel in the compression zone of the beam. With compressive steel included, the
internal compressive force C is shared between the concrete and the steel. The volume of the
concrete stress block above the neutral axis
is therefore reduced and, consequently, the depth to the neutral axis is decreased. Some
compressive reinforcement is normally included in beams to provide anchorage for transverse
Ductility is desirable in prestressed (and reinforced) concrete flexural members. In
continuous or statically indeterminate members, ductility is particularly necessary. Large
curvatures are required at the peak moment regions in order to permit the inelastic moment
redistribution that must occur if the moment diagram assumed in design is to be realized in
Consider the stress distribution caused by the ultimate moment on the section in Figure 4.1.
The resultant compressive force of magnitude C equals the resultant tensile force T and the
ultimate moment capacity is calculated from the internal couple,
The lever arm l between the internal compressive and tensile resultants (C and T) is usually
about 0.9d, where d is the effective depth of the section and may be defined as the distance
from the extreme compressive fibre to the position of the resultant tensile force in all the steel
on the tensile side of the neutral axis. To find the lever arm l more accurately, the location of
the resultant compressive force in the concrete Cc needs to be determined. The shape of the
actual stress-strain relationship for concrete in compression is required in order to determine
the position of its centroid.
4.3 Flexural strength theory
In the analysis of a cross-section to determine its ultimate bending strength Mu, the following
assumptions are usually made:
(a) The variation of strain on the cross-section is linear, i.e. strains in the concrete and the
bonded steel are calculated on the assumption that plane sections remain plane.
(b) Concrete carries no tensile stress, i.e. the tensile strength of the concrete is ignored.
(c) The stress in the compressive concrete and in the steel reinforcement (both prestressed and
non-prestressed) are obtained from actual or idealized stress–strain relationships for the
4.3.2 Idealized rectangular compressive stress blocks for concrete
In order to simplify numerical calculations for ultimate flexural strength, codes of practice
usually specify idealized rectangular stress blocks for the
Figure 4.2 Ultimate moment conditions and rectangular stress blocks.
compressive concrete above the neutral axis. The dimensions of the stress block are calibrated
such that the volume of the stress block and the position of its centroid are approximately the
same as in the real curvilinear stress block.
In Figure 4.2a, an under-reinforced section at the ultimate moment is shown. The section
has a single layer of bonded prestressing steel. The strain diagram and the actual concrete
stress distribution at ultimate are illustrated in Figures 4.2b and c, respectively. The idealized
rectangular stress block for the compressive concrete at the ultimate flexural limit state
specified in both ACI 318–83 and AS 3600–1988 is shown in Figure 4.2d, and that specified
in BS 8110: Part 1 (1985) is illustrated in Figure 4.2e.
At the ultimate moment, the extreme fibre compressive strain ε is taken in ACI 318–83
(and in AS 3600–1988) to be
while in BS 8110: Part 1 (1985), ε is taken to be 0.0035. In fact, the actual extreme fibre
strain at ultimate may not be close to either of these values. However, for under-reinforced
members, with the flexural strength very much controlled by the strength of the tensile steel
(both prestressed and
non-prestressed), variation in the assumed value of ε does not have a significant effect on Mu.
The depth of the ACI 318–83’s rectangular stress block (in Figure 4.2d) is γn and the
uniform stress intensity is . The parameter γdepends on the concrete strength and may
be taken as
γ given in Table 4.1 for some standard concrete strength grades.
For the rectangular section of Figure 4.2a, the hatched area A'(=γnb) is therefore assumed
to be subjected to a uniform stress of and the resultant compressive force Cc is the
volume of the rectangular stress block.
and the position of Cc is the centroid of the hatched area A', i.e. at a depth of γn/2 below the
extreme compressive fibre (provided, of course, that A' is rectangular).
The ultimate moment is obtained from Equation 4.1:
where σ is the stress in the bonded tendons and is determined from considerations of strain
compatibility and equilibrium.
In accordance with the design philosophy for the strength limit states outlined in Section
1.7.6, the design strength is obtained by multiplying Mu from Equation 4.4 by a capacity
reduction factor . In ACI 318–83, for flexure (and in AS 3600–1988).
The ultimate curvature is the slope of the strain diagram at failure and is therefore given by
Table 4.1 Variation of γwith f'c.
f' c(MPa) 20 25 30 35 40 50
γ 0.85 0.85 0.836 0.80 0.766 0.696
The ultimate curvature xu is an indicator of ductility. Large deformations at ultimate are
associated with ductile failures. To ensure ductility of a section at failure, codes of practice
specify minimum limits for xu. For example, ACI 318–83 limits curvature indirectly by
limiting the quantity of tensile reinforcement, thereby placing a maximum limit of 0.424d on
the depth to the neutral axis at failure. The Australian code AS 3600–1988 suggests that dn
should not exceed 0.4dp. This is equivalent to suggesting that xu should be greater than or
For the cross-section shown in Figure 4.2, the effective depth d equals the depth to the
prestressing steel, dp.
The rectangular stress block specified in BS 8110: Part 1 (1985) is shown in Figure 4.2e. It
has an overall depth of 0.9dn and a uniform stress intensity of The parameter γisn
the partial material safety factor for concrete and equals 1.5 (see Section 1.7.6). The stress in
the bonded prestressing steel is σ /γ, where γ=1.15 for steel. The design strength of the
pu m m
member [designated Mu in BS 8110: Part 1 (1985) but equivalent to in ACI 318–83] is
therefore given by
In the remainder of this chapter, the idealized rectangular stress block and the design
procedure specified in ACI 318–83 (and in AS 3600–1988) will be adopted for all numerical
4.3.3 Prestressed steel strain components
For reinforced concrete sections, the strain in the non-prestressed steel and in the concrete at
the steel level are the same at any stage of loading. For the prestressing tendons on a
prestressed concrete section, this is not so. The strain in the bonded prestressing steel at any
stage of loading is equal to the strain caused by the initial prestress plus the change in strain in
the concrete at the steel level.
To calculate accurately the ultimate flexural strength of a section, an accurate estimate of
the final strain in the prestressed and non-prestressed steel is required. The tensile strain in the
prestressing steel at ultimate ε is very much larger than the tensile strain in the concrete at
the steel level, owing to the large initial prestress. For a bonded tendon, ε is usually
considered to be the sum of several sub-components. Figure 4.3 indicates the strain
distributions on a prestressed section at three stages of loading.
Figure 4.3 Strain distributions at three stages of loading.
Stage (a) shows the elastic concrete strain caused by the effective prestress when the
externally applied moment is zero. The strain in the concrete at the steel level is compressive,
with magnitude equal to
where A is the area of the section and I is the second moment of area of the section about its
centroidal axis. The stress and strain in the prestressing steel are
provided that the steel stress is within the elastic range.
Stage (b) is the concrete strain distribution when the applied moment is sufficient to
decompress the concrete at the steel level. Provided that there is bond between the steel and
the concrete, the change in strain in the prestressing steel is equal to the change in concrete
strain at the steel level. The strain in the prestressing steel at stage (b) is therefore equal to the
value at stage (a) plus a tensile increment of strain equal in magnitude to ε (from Equation
Strain diagram (c) in Figure 4.3 corresponds to the ultimate load condition. The concrete
strain at the steel level ε can be expressed in terms of the extreme compressive fibre strain ε
and the depth to the neutral axis at failure dn as
From the requirements of strain compatibility, the change in strain in the
prestressing steel between load stages (b) and (c) is also equal to ε. Therefore, the strain in
the prestressing tendon at the ultimate load condition may be obtained from
ε can therefore be determined in terms of the position of the neutral axis at failure dn and the
extreme compressive fibre strain ε . If ε is known, the stress in the prestressing steel at
ultimate σ can be determined from the stress-strain diagram for the prestressing steel. With
the area of prestressing steel known, the tensile force at ultimate Tp can be calculated. In
general, however, the steel stress is not known at failure and it is necessary to equate the
tensile force in the steel tendon (plus the tensile force in any non-prestressed tensile steel)
with the concrete compressive force (plus the compressive force in any non-prestressed
compressive steel) in order to locate the neutral axis depth, and hence find ε .
In general, the magnitude of ε in Equation 4.11 is very much less than either ε or ε, and
ce pe pt
may usually be ignored without introducing serious errors.
4.3.4 Determination of Mu for a singly reinforced section with bonded tendons
Consider the section shown in Figure 4.2a and the idealized compressive stress block shown
in Figure 4.2d. In order to calculate the ultimate bending strength using Equation 4.4, the
depth to the neutral axis dn and the final stress in the prestressing steel σ must first be
An iterative trial and error procedure is usually used to determine the value of dn for a given
section. The depth to the neutral axis is adjusted until horizontal equilibrium is satisfied, i.e.
C=T. Both C and T are functions of dn. For this singly reinforced cross-section, C is the
volume of the compressive stress block given by Equation 4.3 and T depends on the strain in
the prestressing steel, ε . For any value of dn, the strain in the prestressing steel is calculated
using Equation 4.11 (and Equations 4.8–4.10). The steel stress at ultimate σ , which
corresponds to the calculated value of strain ε, can be obtained from the stress-strain curve
for the prestressing steel and the corresponding tensile force is T=σ A p.
When the correct value of dn is found (i.e. when C=T), the ultimate flexural strength Mu
may be calculated from Equation 4.4.
A suitable iterative procedure is outlined below. About three iterations are usually required
to determine a good estimate of dn and hence Mu.
(1) Select an appropriate trial value of dn and determine ε from Equation 4.11. By equating
the tensile force in the steel to the compressive
force in the concrete, the stress in the tendon may be determined:
(2) Plot the point ε and σ on the graph containing the stress-strain curve for the
prestressing steel. If the point falls on the curve, then the value of dn selected in step 1 is the
correct one. If the point is not on the curve, then the stress–strain relationship for the
prestressing steel is not satisfied and the value of dn is not correct.
(3) If the point ε and σ obtained in step 2 is not sufficiently close to the stress–strain curve
for the steel, repeat steps 1 and 2 with a new estimate of dn. A larger value for dn is required
if the point plotted in step 2 is below the stress–strain curve and a smaller value is required
if the point is above the curve.
(4) Interpolate between the plots from steps 2 and 3 to obtain a close estimate for ε and σ
and the corresponding value for dn.
(5) With the correct values of σ and dn determined in step 4, calculate the ultimate moment
Mu. If the area above the neutral axis is rectangular, Mu is obtained from Equation 4.4. Non-
rectangular-shaped cross-sections are discussed in more detail in Section 4.6.
The ultimate flexural strength Mu of the rectangular section of Figure 4.4a is to be calculated.
The steel tendon consists of ten 12.7 mm diameter strands (Ap=1000 mm 2) with an effective
prestress P e=1200 kN. The
Figure 4.4 Section details and stress and strain distributions at ultimate (Example 4.1).
stress–strain relationship for prestressing steel is as shown in Figure 4.5 and the elastic
modulus is Ep=195×10 3 MPa. The concrete properties are MPa, Ec =29800 MPa, and
from Equation 4.2, γ =0.801.
The initial strain in the tendons due to the effective prestress is given by Equation 4.9:
The strain in the concrete caused by the effective prestress at the level of the prestressing steel
(ε in Figure 4.4b) is calculated using Equation 4.8. Because ε is very small compared with
ε , it is usually acceptable to use the properties of the gross cross-section for its determination.
The concrete strain at the prestressed steel level at failure is obtained from Equation 4.10:
and the final strain in the prestressing steel is given by Equation 4.11:
The magnitude of resultant compressive force C carried by the concrete on the rectangular
section is the volume of the idealized rectangular stress block in Figure 4.4d and is given by
The resultant tensile force T is given by
Horizontal equilibrium requires that C=T and hence
Trial values of dn can now be selected and the corresponding values of ε and σ (calculated
from the above two equations) are plotted on the
stress–strain curve for the steel, as shown in Figure 4.5:
Trial dn (mm) ε
pu σ (MPa)
pu Point plotted on Figure 4.5
230 0.0120 1918 (1)
210 0.0128 1751 (2)
220 0.0124 1835 (3)
Point 3 lies sufficiently close to the stress–strain curve for the tendon and therefore the correct
value for dn is close to 220 mm (0.34 dp).
Figure 4.5 Stress–strain curve for strand (Example 4.1).
From Equation 4.5, the curvature at ultimate is
which is greater than the minimum value required for ductility given by Equation 4.6,
The ultimate moment is found using Equation 4.4:
The design strength of the section in flexure is , where the value of for bending can be
obtained from Table 1.1. In structural design, the moment M* caused by the most severe
factored load combination for strength (see Section 1.7.3) must be less than or equal to .
4.3.5 Sections containing non-prestressed reinforcement and bonded tendons
Frequently, in addition to the prestressing reinforcement, prestressed concrete beams contain
non-prestressed longitudinal reinforcement in both the compressive and tensile zones. This
reinforcement may be included for a variety of reasons. For example, non-prestressed
reinforcement is included in the tensile zone to provide additional flexural strength when the
strength provided by the prestressing steel is not adequate. Non-prestressed tensile steel is
also included to improve crack control when cracking is anticipated at service loads. Non-
prestressed compressive reinforcement may be used to strengthen the compressive zone in
beams that might otherwise be over-reinforced. In such beams, the inclusion of compression
reinforcement not only increases the ultimate strength, but also causes increased curvature at
failure and therefore improves ductility. The use of compressive reinforcement also reduces
long-term deflections caused by creep and shrinkage and therefore improves serviceability. If
for no other reason, compression reinforcement may be included to provide anchorage and
bearing for the transverse reinforcement (stirrups) in beams.
When compressive reinforcement is included, closely spaced transverse ties should be used
to brace laterally the highly stressed bars in compression and prevent them from buckling
outward. In general, the spacing of these ties should not exceed about 16 times the diameter of
the compressive bar.
Consider the doubly reinforced section shown in Figure 4.6a. The resultant compressive
force consists of a steel component Cs(=σA sc) and a concrete component
The stress in the compressive reinforcement is determined from the geometry of the linear
strain diagram shown in Figure 4.6b. The magnitude of strain in the compressive steel is
If ε is less than or equal to the yield strain of the non-prestressed steel (ε y/Es), then
σ =εEs. If ε exceeds the yield strain, then σ=f y.
sc sc sc sc
Figure 4.6 Doubly reinforced section at ultimate.
The resultant tensile force in Figure 4.6d consists of a prestressed component Tp(=σ Ap) and
a non-prestressed component Ts(=σA st). The stress in the non-prestressed steel is determined
from the strain at ultimate, ε, which is given by
If , then σ=εEs. If ε>ε then σ=fy .
st st st y , st
In order to calculate the depth to the neutral axis at ultimate, dn, a trial and error procedure
similar to that outlined in Section 4.3.4 can be employed. Successive values of dn are tried
until the value which satisfies the horizontal equilibrium equation is determined:
Since one of the reasons for the inclusion of compressive reinforcement is to improve
ductility, most doubly reinforced beams are, or should be, under-reinforced, i.e. the non-
prestressed tensile steel is at yield at ultimate. Whether or not the compressive steel has
yielded depends on its quantity Asc and its depth from the top compressive surface of the
section, dc .
If it is assumed initially that both the compressive and the tensile non-prestressed steel are
at yield, then
From Equation 4.14:
When the value of σ (calculated from Equation 4.15) and the value of ε (calculated from
Equation 4.11) satisfy the stress–strain relationship of the prestressing steel, the correct value
of dn has been found. The non-prestressed steel strains should be checked to ensure that the
steel has, in fact, yielded. If the compressive steel is not at yield, then the compressive force
Cs has been overestimated and the correct value of dn is slightly greater than the calculated
value. The compressive steel stress in Equation 4.15 should be taken as εEs, instead of f y.
Further iteration may be required to determine the correct value of dn and the corresponding
internal forces Cc , Cs, Tp and Ts.
With horizontal equilibrium satisfied, the ultimate moment of the section may be
determined by taking moments of the internal forces about any convenient point on the
section. Taking moments about the non-prestressed tensile reinforcement level gives
For the rectangular section shown in Figure 4.6a, the lever arms to each of the internal forces
In the above equations, Cs and Cc are the magnitudes of the compressive forces in the steel
and concrete, respectively, and are therefore considered to be positive.
The ultimate curvature is obtained from Equation 4.5 and the minimum curvature required
for ductility is given by Equation 4.17, which is the same as Equation 4.6 except that the
depth to the prestressing steel dp is replaced by d (the depth to the resultant tensile force T):
To the cross-section analysed in Example 4.1 and shown in Figure 4.4, three 24 mm diameter
non-prestressed reinforcing bars (Ast =1350 mm2) are added in the tensile zone at a depth
do=690 mm. The ultimate moment Mu for the section is to be calculated. The yield stress of
steel is f y=400 MPa and all other material properties and cross-sectional details are as
specified in Example 4.1.
The strain in the prestressing steel at ultimate is as calculated in Example 4.1:
and the magnitude of the compressive force Cc carried by the concrete above the neutral axis
From Equation 4.13, the non-prestressed steel is at yield (i.e. ), provided that
the depth to the neutral axis dn is less than or equal to 0.6do(=414 mm). If σ is assumed to
equal f y, the resultant tensile force T(=T p+Ts ) is given by
Horizontal equilibrium requires that Cc =T and hence
Trial values of dn can now be selected and the respective values of ε and σ plotted on the
stress–strain curve for the prestressing steel as shown in Figure 4.7:
Trial dn (mm) ε
pu σ (MPa)
pu Point Plotted on Figure 4.7
270 0.0108 1712 (4)
290 0.0103 1879 (5)
277 0.0106 1770 (6)
Since point 6 lies sufficiently close to the stress–strain curve for the tendon, the correct value
for dn is 277 mm.
From Equation 4.5, the ultimate curvature is
Figure 4.7 Stress-strain curve for strand (Example 4.2).
dn is much less than 0.6do(=414 mm) and therefore the non-prestressed steel has yielded, as
was assumed. The depth from the top surface to the resultant force in the tensile steel at
The minimum curvature required to ensure some measure of ductility is obtained from
which is greater than xu. The section is therefore non-ductile and, in design, it would be
prudent to insert some non-prestressed compressive reinforcement to increase the ultimate
curvature and improve ductility (at least to the level required by Equation 4.17).
At ultimate, the compressive force in the concrete is Cc=8340dn= 2310 kN and the tensile
force in the tendon is Tp=σ Ap=1770 kN. The ultimate moment is calculated from Equation
Figure 4.8 Section details and conditions at ultimate for Example 4.3.
Consider the effect on both strength and ductility of the addition of two 24 mm diameter bars
in the compression zone of the section in Example 4.2. Details of the cross-section are shown
in Figure 4.8, together with the stress and strain distributions at ultimate. All data are as
specified in Examples 4.1 and 4.2.
From Example 4.2, the ultimate strain in the tendons is
and the strain in the non-prestressed tensile reinforcement is greater than ε The magnitude of
the compression steel strain at ultimate is given by Equation 4.12:
The stress in the compression steel can be readily obtained from ε for any value of dn. By
equating C=T, an expression for σ similar to Equation 4.15 is obtained. If the compression
steel is assumed to be at yield, Equation 4.15 gives
Values of ε and σ for trial values of dn are tabulated below and plotted as points (7)–(9) in
Trial dn ε
sc σ (MPa)
pu Point plotted on Figure 4.9
250 0.0114 >ε
y 1905 (7)
230 0.0120 >ε
y 1738 (8)
239 0.0117 >ε
y 1813 (9)
Figure 4.9 Stress–strain curve for strand (Example 4.3).
From Figure 4.9, the point corresponding to dn=239 mm lies on the actual stress–strain curve
and therefore represents the correct solution. It is also apparent in Figure 4.9 that the strain in
the prestressing steel at ultimate is increased by the introduction of compressive
reinforcement [from point (6) to point (9)] and the depth to the neutral axis is decreased. The
ultimate curvature is obtained from Equation 4.5:
which represents a 12% increase in final curvature caused by the introduction of the
The depth d to the resultant tensile force (T=Tp+Tst ) remains at 659 mm and the magnitude
of the resultant forces on the cross-section are
Cc =1993 kN, Cs=360 kN, Tst=540 kN, and Tp=1813 kN. The ultimate moment is calculated
using Equation 4.16:
which is a 5.6% increase in strength. In general, for non-ductile sections, the addition of
compressive reinforcement causes a significant increase in curvature at ultimate (i.e. a
significant increase in ductility) and a less significant but nevertheless appreciable increase in
4.4 Approximate code-oriented procedures
4.4.1 Bonded tendons
Approximate equations or procedures are specified in some codes of practice for the
estimation of stress in a bonded tendon at the ultimate moment. These are generally
conservative and may be used in lieu of the more accurate determination of σ based on strain
compatibility (as outlined in the previous sections). For example, when the effective prestress
σ (=Pe /Ap) is not less than 0.5 f p, AS 3600–1988 specifies that the stress in the bonded steel
at ultimate may be taken as
The same equation (with different notation) is also specified in ACI 318–83. The parameter γ
is defined in Equation 4.2. The term k 1 depends on the particular type of prestressing steel and
may be taken as
where f py is the specified yield strength of the prestressing tendon. The term k 2 is given by
where b is the width of the compressive face of the cross-section and dp is the distance from
the extreme compressive fibre to the centroid of the tendons. When compression
reinforcement is present, k 2 should be taken not less than 0.17. In addition, if the depth to the
compressive steel dc exceeds 0.15 dp, then Asc should be set to zero in Equation 4.19. Other
more accurate procedures are available for calculating σ based on mathematical expressions
for the shape of the stress-strain curve of the prestressing steel, such as that proposed recently
by Loov (1988).
Consider a rectangular section such as that shown in Figure 4.6 containing tensile
prestressing steel, and both tensile and compressive non-prestressed reinforcement (A p, Ast ,
and Asc, respectively). Assuming the non-prestressed tensile steel is at yield, the total tensile
force in the steel at ultimate is
The magnitude of the total compressive force C consists of a concrete component Cc (given
by Equation 4.3) and a steel component Cs=σ Asc. That is,
If the non-prestressed compressive steel is initially assumed to be at yield and the stress in the
prestressing steel σ is obtained from Equation 4.18, the depth to the neutral axis at ultimate
may be obtained by equating C and T. Thus,
The calculated value of dn can be used to check that the compressive steel has in fact yielded.
If the steel has not yielded, a revised estimate of σ (=Es ε) may be made and used to
calculate a new value of dn. Relatively few iterations are required for convergence.
By taking moments about the level of the tensile steel, the ultimate moment Mu is given by
where d o is the distance from the extreme compressive surface to the non-prestressed tensile
BS 8110: Part 1 (1985) tabulates approximate values for the tensile stress in the tendons
and the depth to the neutral axis at the ultimate limit state.
Table 4.2 Conditions at the ultimate limit state for rectangular beams with bonded tendons [BS 8110:
Part 1 (1985)].
0.4fp 0.5fp 0.6fp 0.4fp 0.5fp 0.6f p
0.05 1.00 1.00 1.00 0.11 0.11 0.11
0.10 1.00 1.00 1.00 0.22 0.22 0.22
0.15 0.95 0.97 0.99 0.31 0.32 0.32
0.20 0.88 0.90 0.92 0.38 0.39 0.40
0.25 0.84 0.86 0.88 0.46 0.47 0.48
0.30 0.80 0.83 0.85 0.52 0.54 0.55
0.35 0.76 0.80 0.83 0.58 0.60 0.63
0.40 0.72 0.77 0.81 0.62 0.67 0.70
0.45 0.68 0.74 0.79 0.66 0.72 0.77
0.50 0.64 0.71 0.77 0.69 0.77 0.83
The tabulated values are based on the idealized rectangular stress block shown in Figure 4.2e.
Using the notation adopted in this chapter (and not that of BS 8110), the tensile stress in a
bonded tendon may be taken as
where λ may be interpolated from Table 4.2 for any value of the effective prestress σ ; γ is
the partial material safety factor and equals 1.15. The depth to the neutral axis is also obtained
from Table 4.2. For a cross-section containing only bonded prestressing tendons at a depth dp,
BS 8110 specifies the design resistance moment (design strength) as
A comparison of the solution calculated in Example 4.1 (using the actual stress–strain
relationship of the prestressing steel) can be made with the
value obtained using the approximate estimate of σ obtained from Equation 4.18. For this
example, fp=1910 MPa and fpy=1780 MPa (obtained from Figure 4.5) and the constants k1 and
k 2 are
From Equation 4.18, the stress in the tendon at ultimate is
which is 4.6% less than the more accurate value obtained by trial and error in Example 4.1.
From Equation 4.20,
which compares with dn=220 mm in Example 4.1. The ultimate strength is calculated using
Equation 4.4 (or Equation 4.21):
This is about 4% more conservative than the value obtained in Example 4.1. As expected, the
simplified empirical procedure predicts a reasonable and conservative estimate of strength.
However, the ultimate curvature is less conservative because the depth to the neutral axis is
underestimated. The ultimate curvature is obtained from Equation 4.5:
and is 4.6% greater than the previously predicted value. Nevertheless, for practical purposes,
the simplified method is a useful design alternative.
The calculations are now repeated using the procedure specified in BS 8110: Part 1 (1985).
In Example 4.1,
and from Table 4.2, λ
=0.89 and dn=0.47dp=305 mm.
The stress in the bonded tendons is approximated using Equation 4.22:
and Equation 4.23 gives
and the ultimate curvature is
Direct comparison between the values for Mu predicted by the approach in AS 3600–1988
(and in ACI 318–83) and the BS 8110 approach is not possible, since the partial material
safety factors are included in the latter and not in the former.
In this example, Example 4.3 is reworked using the approximate formula for σ given in
Assuming all non-prestressed steel is at yield, the depth to the neutral axis is obtained from
The non-prestressed steel strains are in fact much greater than the yield strain (=0.002) and
the assumption to this effect is therefore correct. The resultant forces on the cross-section are
Cc =1915 kN, Cs=360 kN, Tst=540 kN, and Tp=1735 kN, and the ultimate moment is obtained
from Equation 4.6:
This is about 3% less than the more accurate value calculated in Example 4.3.
4.4.2 Unbonded tendons
Where the prestressing steel is not bonded to the concrete, the stress in the tendon at ultimate,
σ , is significantly less than that predicted by Equation 4.18 and accurate determination of the
ultimate flexural strength is more difficult than for a section containing bonded tendons. This
is because the final strain in the tendon is more difficult to determine accurately. The ultimate
strength of a section containing unbonded tendons may be as low as 75% of the strength of an
equivalent section containing bonded tendons. Hence, from a strength point of view, bonded
construction is to be preferred.
An unbonded tendon is not restrained by the concrete along its length and slip between the
tendon and the duct takes place as the external loads are applied. The steel strain is more
uniform along the length of the member and tends to be lower in regions of maximum
moment than would be the case for a bonded tendon. The ultimate strength of the section may
be reached before the stress in the unbonded tendon reaches the yield stress f py. For members
not containing any bonded reinforcement, crack control may be a problem if cracking occurs
in the member for any reason. If flexural cracking occurs, the number of cracks in the tensile
zone is fewer than in a beam containing bonded reinforcement, but the cracks are wider and
Approximate equations for the stress in an unbonded tendon at the ultimate limit state are
also specified in codes of practice. AS 3600–1988 (and ACI 318–83), for example, specify the
following equations for σ : pu
(a) If the span to depth ratio of the member is 35 or less:
but σ should not be taken greater than fpy or (σ +400).
(b) If the span to depth ratio of the member is greater than 35:
but not greater than fpy or (σ +200).
The approximate expressions specified in BS 8110: Part 1 (1985) for σ and the depth to the
neutral axis dn for members containing unbonded
To ensure ductility and some measure of crack control, it is good practice to include non-
prestressed bonded tensile reinforcement in members with unbonded tendons. However, it is
usual practice in most post-tensioning applications to grout the tendons within the duct after
(or during) construction. Indeed, in Australia, for example, bonded construction is mandatory.
The ultimate flexural strength of a simply supported post-tensioned beam is to be calculated.
The beam spans 12 m and contains a single unbonded cable. The cross-section of the beam at
mid-span is shown in Figure 4.4a. Material properties are as specified in Example 4.1.
The stress in the tendon caused by the effective prestressing force P e=1200 kN is
With the span-to-depth ratio equal to 16, the stress in the unbonded tendon at ultimate,
according to AS 3600–1988 and ACI 318–83, is given by Equation 4.24a:
and therefore the tensile force in the steel is Tp=1350 kN (=Cc). The depth to the neutral axis
is calculated using Equation 4.20:
and Equation 4.4 gives
Using the alternative approach outlined in BS 8110: Part 1 (1985), estimates of σ and dn are
made using Equations 4.25a and b, respectively:
and from Equation 4.23,
4.5 Design calculations
The magnitude of the prestressing force P e and the quantity of the prestressing steel A p are
usually selected to satisfy the serviceability requirements of the member, i.e. to control
deflection or to reduce or eliminate cracking. With serviceability satisfied, the member is then
checked for adequate strength. The ultimate moment Mu for the section containing the
prestressing steel (plus any non-prestressed steel added for crack control) is calculated and the
design strength is compared with the design action, in accordance with the design
requirements outlined in Section 1.7.6. For example, in ACI 318–83 and in AS 3600–1988,
the flexural strength is . The design action M* is the moment caused by the most severe
factored load combination specified for the strength limit state (see Section 1.7.3). The design
requirement is that .
The prestressing steel needed for the satisfaction of serviceability requirements may not be
enough to provide adequate strength. When this is the case, the ultimate moment capacity can
be increased by the inclusion of additional non-prestressed tensile reinforcement. Additional
compressive reinforcement may also be required to improve ductility.
4.5.2 Calculation of additional non-prestressed tensile reinforcement
Consider the singly reinforced cross-section shown in Figure 4.10a. It is assumed that the
effective prestress P e, the area of the prestressing steel Ap, and the cross-sectional dimensions
have been designed to satisfy the serviceability requirements of the member. The idealized
strain and stress distributions specified by ACI 318–83 and AS 3600–1988 for the ultimate
Figure 4.10 Cross-sections containing tensile reinforcement at the ultimate limit state (AS 3600–1988
and ACI 318–83).
state are also shown in Figure 4.10a. The ultimate moment for the section is denoted Mu1,
The tendon stress at ultimate σ may be calculated from the actual stress-strain curve for the
steel (as illustrated in Example 4.1) or from the approximation of Equation 4.18 (as illustrated
in Example 4.4).
If the design strength is greater than or equal to M*, then no additional steel is
necessary. The cross-section has adequate strength. If is less than M*, the section is not
adequate and additional tensile reinforcement is required.
In addition to providing adequate strength, it is important also to ensure that the section is
ductile. In order that the curvature at ultimate x u is large enough to impart ductility, an upper
limit for the depth to the neutral axis of about 0.4dp is usually specified. However, to ensure
ductility, a more satisfactory range for the depth to the neutral axis at failure is . If
the value of dn1 in Figure 4.10a is outside this range, some additional non-prestressed
compressive reinforcement is required to relieve the concrete compressive zone and reduce dn.
The design procedure outlined in
Section 4.5.3 for doubly reinforced cross-sections is recommended in such a situation.
For the cross-section shown in Figure 4.10a, if is less than M* and if dn1 is small so
that ductility is not a problem, the aim in design is to calculate the minimum area of non-
prestressed tensile reinforcement Ast to be added to the section to satisfy strength requirements
(i.e. the value of Ast such that ). In Figure 4.10b, the new cross-section containing
A st is shown, together with the revised strain and stress distributions at ultimate. With dn small
enough to ensure ductility, the steel strain is greater than the yield strain ε y/Es), so that
σ=f y. The addition of A st to the cross-section causes an increase in the resultant tension at
ultimate (Tp+Tst) and hence an increase in the resultant compression (Cc ). To accommodate
this additional compression, the depth of the compressive stress block in Figure 4.10b must be
greater than the depth of the stress block in Figure 4.10a (i.e. γn>γn1). The increased value
of dn results in a reduction in the ultimate curvature (i.e. a decrease in ductility), a reduction in
the strain in the prestressing steel, and a consequent decrease in σ . The decrease in σ is
relatively small, however, provided that the section has adequate ductility (i.e. provided that
the value of dn remains less than about 0.3dp).
If σ is assumed to remain constant, a first estimate of the magnitude of the area of non-
prestressed steel Ast required to increase the ultimate strength from Mu1 (the strength of the
section prior to the inclusion of the additional steel) to Mu (the required strength of the
section) may be obtained from
where l is the lever arm between the tension force in the additional steel Ts and the equal and
opposite compressive force C c2 which results from the increase in the depth of the
compressive stress block. The lever arm l may be approximated initially as
where dn 1 is the depth to the neutral axis corresponding to Mu 1.
The ultimate strength of the singly reinforced section shown in Figure 4.11 is Mu1=1120 kNm.
The stress and strain distributions corresponding to Mu1 are also shown in Figure 4.11 and the
material properties are MPa (γ =0.801) and fp=1860 MPa.
Calculate the additional amount of non-prestressed tensile reinforcement
Figure 4.11 Singly reinforced cross-section at ultimate (Example 4.7).
(f y=400 MPa) required to increase the ultimate strength of the section to Mu=1450kNm.
For the section in Figure 4.11, dn1=172.4 mm=0.23dp and the section is ductile. If the
additional tensile steel is to be added at do =840 mm, then the lever arm l in Equation 4.27 may
be approximated by
and the required area of non-prestressed steel is estimated using Equation 4.27:
Choose three 24 mm diameter bars (Ast =1350 mm2) located at a depth do=840 mm.
A check of this section to verify that kN mand that the section is ductile can
next be made using the trial and error procedure illustrated in Example 4.2.
4.5.3 Design of a doubly reinforced cross-section
For a singly reinforced section (such as that shown in Figure 4.12a) in which dn1 is greater
than about 0.3dp, the inclusion of additional tensile reinforcement may cause ductility
problems. In such cases, the ultimate strength may be increased by the inclusion of suitable
quantities of both tensile and compressive non-prestressed steel without causing any reduction
in curvature, i.e. without increasing dn . If the depth to the neutral axis is held constant at dn1,
the values of both Cc (the compressive force carried by the concrete) and Tp (the tensile force
in the prestressing steel) in Figures 4.12a and b are the same. In each figure, Cc is equal to Tp.
With the strain diagram in
Figure 4.12 Doubly reinforced section at ultimate (AS 3600–1988 and ACI 318–83).
Figure 4.12b known, the strains at the levels of the non-prestressed steel may be calculated
using Equations 4.12 and 4.13, and hence the non-prestressed steel stresses σ and σ may be
determined. The equal and opposite forces which result from the inclusion of the non-
prestressed steel are
If Mu1 is the strength of the singly reinforced section in Figure 4.12a (calculated using
Equation 4.26) and Mu is the required strength of the doubly reinforced cross-section, the
minimum area of the tensile reinforcement is given is
For conventional non-prestressed steel, σ=fy provided that the depth to the neutral axis dn
satisfies the stated ductility requirements. For equilibrium, the forces in the top and bottom
non-prestressed steel are equal and opposite, i.e. Cs=Ts since Cc =Tp. From Equation 4.28,
If the depth to the neutral axis in Figure 4.12a is greater than about 0.4dp, then the section is
non-ductile and the value of dn must be reduced. An appropriate value of dn may be selected
(say dn=0.3dp). For this value of dn, all the steel strains (ε, ε, and ε) and hence all the steel
sc st pt
stresses at ultimate (σ, σ, and σ ) may be determined. With ε calculated from the assumed
sc st pu pt
value for dn, the total strain in the prestressing steel can be calculated using Equation 4.11 and
the stress σ can be read directly from the stress–strain curve. In this way, the magnitude of
the tensile force in the tendon (Tp=A pσ ) and the compressive force in the concrete
may be evaluated. If the required strength of the section is Mu, the
minimum area of compressive steel can be obtained by taking moments about the level of the
non-prestressed reinforcement. That is,
Horizontal equilibrium requires that Ts=Cc+Cs− p and therefore the area of non-prestressed
tensile steel is
Additional non-prestressed steel is required to increase the ultimate flexural strength of the
section in Figure 4.4 (and analysed in Example 4.1) to Mu=1300 kNm.
From Example 4.1, Mu1=1030 kNm and dn1=220 mm. If only non-prestressed tensile steel
were to be added, the lever arm l in Equation 4.27 would be
and from Equation 4.27,
This corresponds to the addition of four 24 mm diameter bars in the bottom of the section
shown in Figure 4.4 at a depth do=690 mm.
A check of the section to verify that kN m can next be made using the trial and
error procedure illustrated in Example 4.1. In this example, however, the neutral axis depth
increases above 0.4d and the curvature at ultimate is less than the recommended minimum
value. For this section,
it is appropriate to supply the additional moment capacity via both tensile and compressive
If the depth to the neutral axis is held constant at the value determined in Example 4.1, i.e.
dn=220 mm, then the stress and strain in the prestressed steel remain as previously calculated,
If the depth to the compressive reinforcement is dc=60 mm, then from Equation 4.12,
From Equation 4.13,
The area of additional tensile steel is obtained using Equation 4.29:
and from Equation 4.30,
Use three 24 mm diameter non-prestressed tensile bars at do=690 mm and three 24 mm
diameter bars in the top of the section at dc=60 mm.
4.6 Flanged sections
Flanged sections such as those shown in Figure 4.13a are commonly used in prestressed
concrete construction, where the bending efficiency of I-, T-, and box-shaped sections can be
effectively utilized. Frequently, in the construction of prestressed floor systems, beams or
wide bands are poured monolithically with the slabs. In such cases, a portion of slab acts as
either a top or a bottom flange of the beam, as shown in Figure 4.13b. Codes of practice
generally specify the width of the slab which may be assumed to be part of the beam cross-
section (i.e. the effective width of the flange, bef).
Both AS 3600–1988 and BS 8110: Part 1 (1985) contain the following
Figure 4.13 Typical flanged sections.
except that the overhanging part of the effective flange should not exceed half the clear
distance to the next parallel beam. The term bw is the width of the web of the section. Lo is the
distance along the beam between the points of zero bending moment a